# Lee Cronin <Lee.Cronin@glasgow.ac.uk>
 
data_jg2433-1 

loop_
_publ_author_name
'Jamie M. Cameron'
'Jing Gao'
'De-Liang Long'
'Leroy Cronin'
_publ_section_title
;
 Self-assembly and structural transformations of high-nuclearity palladium-rich polyoxometalates
;
_journal_name_full               'Inorganic Chemistry Frontiers'
_journal_page_first              ?
_journal_page_last               ?
_journal_volume                  ?
_journal_year                    ?
_audit_author_name               'Leroy Cronin'
_audit_contact_author_address
;
   WestCHEM
   School of Chemistry
   University of Glasgow  
   Glasgow
   United Kingdom
   G12 8QQ
;
_audit_contact_author_email      'L.Cronin@chem.gla.ac.uk'
_audit_contact_author_fax        '+44-141-330-4888'
_audit_contact_author_phone      '+44-141-330-6650'
 
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum            'H150 K26 O274 Pd10 Se10 W52' 
_chemical_formula_weight          16965.60 
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'W'  'W'  -0.8490   6.8722 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Pd'  'Pd'  -0.9988   1.0072 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Se'  'Se'  -0.0929   2.2259 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'K'  'K'   0.2009   0.2494 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            triclinic 
_symmetry_space_group_name_H-M    P-1 
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, -z' 
 
_cell_length_a                    20.3612(2) 
_cell_length_b                    22.5889(3) 
_cell_length_c                    33.0969(4) 
_cell_angle_alpha                 74.3670(10) 
_cell_angle_beta                  72.4090(10) 
_cell_angle_gamma                 89.4760(10) 
_cell_volume                      13930.5(3) 
_cell_formula_units_Z             2 
_cell_measurement_temperature     150(2) 
_cell_measurement_reflns_used     64660 
_cell_measurement_theta_min       2.90 
_cell_measurement_theta_max       28.2 
 
_exptl_crystal_description        block
_exptl_crystal_colour             'light orange' 
_exptl_crystal_size_max           0.40 
_exptl_crystal_size_mid           0.24 
_exptl_crystal_size_min           0.18 
_exptl_crystal_density_meas       none 
_exptl_crystal_density_diffrn     4.045 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              14968 
_exptl_absorpt_coefficient_mu     23.807 
_exptl_absorpt_correction_type    Analytical 
_exptl_absorpt_correction_T_min   0.0381 
_exptl_absorpt_correction_T_max   0.0981 
_exptl_absorpt_process_details     
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.33.55 (release 05-01-2010 CrysAlis171 .NET)
(compiled Jan  5 2010,16:28:46)
Analytical numeric absorption correction using a multifaceted crystal
			model based on expressions derived by R.C. Clark & J.S. Reid.
(Clark, R. C. & Reid, J. S. (1995). Acta Cryst. A51, 887-897)
;
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       150(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Oxford Gemini A Ultra CCD' 
_diffrn_measurement_method        'ω & π scans' 
_diffrn_detector_area_resol_mean  ? 
_diffrn_standards_number          ? 
_diffrn_standards_interval_count  ? 
_diffrn_standards_interval_time   ? 
_diffrn_standards_decay_%         none 
_diffrn_reflns_number             225993 
_diffrn_reflns_av_R_equivalents   0.1138 
_diffrn_reflns_av_sigmaI/netI     0.0837 
_diffrn_reflns_limit_h_min        -25 
_diffrn_reflns_limit_h_max        25 
_diffrn_reflns_limit_k_min        -27 
_diffrn_reflns_limit_k_max        27 
_diffrn_reflns_limit_l_min        -40 
_diffrn_reflns_limit_l_max        40 
_diffrn_reflns_theta_min          2.91 
_diffrn_reflns_theta_max          26.00 
_reflns_number_total              54630 
_reflns_number_gt                 33779 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.33.55 (release 05-01-2010 CrysAlis171 .NET)
(compiled Jan  5 2010,16:28:46)
;
_computing_cell_refinement
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.33.55 (release 05-01-2010 CrysAlis171 .NET)
(compiled Jan  5 2010,16:28:46)
;
_computing_data_reduction
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.33.55 (release 05-01-2010 CrysAlis171 .NET)
(compiled Jan  5 2010,16:28:46)
;
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     Diamond3 
_computing_publication_material   WinGX 
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.1603P)²+0.0000P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    none 
_refine_ls_hydrogen_treatment     none 
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        none 
_refine_ls_number_reflns          54630 
_refine_ls_number_parameters      2858 
_refine_ls_number_restraints      1 
_refine_ls_R_factor_all           0.1184 
_refine_ls_R_factor_gt            0.0811 
_refine_ls_wR_factor_ref          0.2402 
_refine_ls_wR_factor_gt           0.2132 
_refine_ls_goodness_of_fit_ref    0.964 
_refine_ls_restrained_S_all       0.964 
_refine_ls_shift/su_max           0.002 
_refine_ls_shift/su_mean          0.000 
 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
W1 W 0.64047(5) -0.12890(5) 0.97309(4) 0.0480(2) Uani 1 1 d . . . 
W2 W 0.90166(8) -0.13045(7) 0.82090(6) 0.0456(3) Uani 0.95 1 d P . . 
W2' W 0.894(3) -0.121(2) 0.8321(17) 0.078(17) Uiso 0.05 1 d P . . 
W3' W 0.812(2) -0.082(2) 0.7328(16) 0.060(14) Uiso 0.05 1 d P . . 
W3 W 0.80144(9) -0.07093(8) 0.74086(6) 0.0444(4) Uani 0.95 1 d P . . 
W4 W 0.69519(9) 0.01787(8) 0.96233(7) 0.0448(4) Uani 0.95 1 d P . . 
W4' W 0.692(3) 0.023(3) 0.9739(15) 0.064(16) Uiso 0.05 1 d P . . 
W5 W 0.59961(5) 0.08229(5) 0.87983(4) 0.0483(2) Uani 1 1 d . . . 
W6 W 0.94236(6) -0.03957(5) 0.93622(4) 0.0501(3) Uani 1 1 d . . . 
W7 W 0.66390(6) 0.47092(5) 0.85256(4) 0.0497(2) Uani 1 1 d . . . 
W8 W 0.54251(5) -0.06483(5) 0.89198(4) 0.0488(2) Uani 1 1 d . . . 
W9 W 0.60182(6) 0.39052(5) 1.01915(4) 0.0524(3) Uani 1 1 d . . . 
W10 W 0.67841(6) 0.13252(5) 0.71548(4) 0.0526(3) Uani 1 1 d . . . 
W11 W 1.01319(6) 0.37956(5) 0.51859(4) 0.0490(2) Uani 1 1 d . . . 
W12 W 0.63798(6) -0.01830(6) 0.72134(4) 0.0543(3) Uani 1 1 d . . . 
W13 W 1.27665(6) 0.42942(6) 0.82902(4) 0.0553(3) Uani 1 1 d . . . 
W14 W 0.68591(6) 0.25802(5) 1.00810(4) 0.0478(2) Uani 1 1 d . . . 
W15 W 1.26491(6) 0.34239(6) 0.49942(4) 0.0538(3) Uani 1 1 d . . . 
W16 W 0.66649(6) 0.53964(5) 0.93383(4) 0.0530(3) Uani 1 1 d . . . 
W17 W 0.91425(6) 0.47546(5) 0.91880(4) 0.0515(3) Uani 1 1 d . . . 
W18 W 1.15410(6) 0.39510(6) 0.42791(4) 0.0537(3) Uani 1 1 d . . . 
W19 W 1.18647(6) 0.55134(6) 0.77345(4) 0.0525(3) Uani 1 1 d . . . 
W20 W 0.81305(6) 0.54775(5) 0.84608(4) 0.0518(3) Uani 1 1 d . . . 
W21 W 0.59386(5) 0.32410(5) 0.93736(4) 0.0479(2) Uani 1 1 d . . . 
W22 W 1.05510(6) 0.01930(6) 0.58606(4) 0.0586(3) Uani 1 1 d . . . 
W23 W 1.33908(6) 0.20593(6) 0.56097(4) 0.0590(3) Uani 1 1 d . . . 
W24' W 0.8645(14) 0.0945(13) 0.6975(8) 0.068(8) Uiso 0.10 1 d P . . 
W24 W 0.86326(10) 0.08885(8) 0.68641(7) 0.0495(4) Uani 0.90 1 d P . . 
W25 W 1.35486(6) 0.50983(6) 0.59471(4) 0.0545(3) Uani 1 1 d . . . 
W26 W 0.78954(6) -0.11105(5) 1.00974(4) 0.0496(2) Uani 1 1 d . . . 
W27 W 1.43667(6) 0.39191(6) 0.64617(4) 0.0574(3) Uani 1 1 d . . . 
W28 W 0.76823(6) 0.47027(5) 1.00839(4) 0.0532(3) Uani 1 1 d . . . 
W29 W 1.43569(6) 0.50035(7) 0.76241(4) 0.0595(3) Uani 1 1 d . . . 
W30 W 1.01287(6) 0.30243(6) 0.44171(4) 0.0548(3) Uani 1 1 d . . . 
W31 W 0.95172(6) 0.45662(5) 0.80601(4) 0.0493(2) Uani 1 1 d . . . 
W32 W 1.11364(7) 0.16760(6) 0.43733(4) 0.0567(3) Uani 1 1 d . . . 
W33 W 0.93493(7) 0.24773(6) 0.61670(4) 0.0571(3) Uani 1 1 d . . . 
W34 W 0.75068(6) -0.20855(5) 0.89411(4) 0.0495(2) Uani 1 1 d . . . 
W35 W 0.84924(6) 0.33808(5) 0.99700(4) 0.0495(2) Uani 1 1 d . . . 
W36 W 0.65136(6) -0.14549(5) 0.81371(4) 0.0500(2) Uani 1 1 d . . . 
W37 W 0.97520(6) 0.15504(6) 0.52959(4) 0.0569(3) Uani 1 1 d . . . 
W38 W 1.22697(6) 0.58933(6) 0.66102(4) 0.0521(3) Uani 1 1 d . . . 
W39 W 0.53321(6) 0.05232(6) 0.79354(4) 0.0542(3) Uani 1 1 d . . . 
W40 W 1.19383(7) 0.03203(6) 0.49622(4) 0.0590(3) Uani 1 1 d . . . 
W41 W 1.26890(6) 0.27092(6) 0.42001(4) 0.0578(3) Uani 1 1 d . . . 
W42 W 1.10822(6) 0.39097(6) 0.82478(4) 0.0523(3) Uani 1 1 d . . . 
W43 W 0.88986(6) -0.18598(5) 0.93897(4) 0.0514(3) Uani 1 1 d . . . 
W44 W 1.47670(6) 0.54437(6) 0.64092(4) 0.0590(3) Uani 1 1 d . . . 
W45 W 1.22068(7) 0.01615(6) 0.68050(4) 0.0635(3) Uani 1 1 d . . . 
W46 W 0.99651(7) 0.02293(6) 0.81516(4) 0.0629(3) Uani 1 1 d D . . 
W47 W 1.34667(6) 0.62607(6) 0.70768(4) 0.0576(3) Uani 1 1 d . . . 
W48 W 1.34710(6) 0.13636(6) 0.47979(4) 0.0616(3) Uani 1 1 d . . . 
W49 W 1.39188(6) 0.35031(6) 0.76690(4) 0.0585(3) Uani 1 1 d . . . 
W50 W 1.35430(7) 0.03673(7) 0.58589(5) 0.0667(3) Uani 1 1 d . . . 
W51 W 1.02921(10) 0.03273(9) 0.69535(6) 0.0501(4) Uani 0.80 1 d P . . 
W51' W 1.0443(6) 0.0494(6) 0.6969(4) 0.077(4) Uiso 0.20 1 d P . . 
W52 W 1.21156(7) -0.05645(6) 0.60240(4) 0.0630(3) Uani 1 1 d . . . 
Pd1 Pd 1.24092(12) 0.18322(11) 0.67505(8) 0.0565(5) Uani 1 1 d . . . 
Pd2 Pd 1.12378(11) 0.37107(10) 0.59184(7) 0.0505(5) Uani 1 1 d . . . 
Pd3 Pd 1.27819(11) 0.29442(11) 0.71469(8) 0.0553(5) Uani 1 1 d . . . 
Pd4 Pd 1.17848(11) 0.43784(10) 0.65201(7) 0.0516(5) Uani 1 1 d . . . 
Pd5 Pd 0.84472(10) 0.24639(10) 0.92135(7) 0.0464(4) Uani 1 1 d . . . 
Pd6 Pd 0.73060(10) 0.32445(10) 0.83526(7) 0.0462(4) Uani 1 1 d . . . 
Pd7 Pd 0.71820(10) 0.20399(9) 0.79677(7) 0.0462(4) Uani 1 1 d . . . 
Pd8 Pd 0.86119(10) 0.10980(10) 0.91069(7) 0.0474(4) Uani 1 1 d . . . 
Pd9 Pd 0.84322(10) 0.22274(9) 0.82983(7) 0.0460(4) Uani 1 1 d . . . 
Pd10 Pd 1.14381(11) 0.28995(11) 0.68378(8) 0.0543(5) Uani 1 1 d . . . 
Se1 Se 0.80573(12) -0.04924(11) 0.89060(8) 0.0435(5) Uani 1 1 d . . . 
Se2 Se 1.11464(13) 0.25126(12) 0.52053(9) 0.0481(6) Uani 1 1 d . . . 
Se3 Se 0.70544(12) 0.01524(12) 0.80588(8) 0.0443(5) Uani 1 1 d . . . 
Se4 Se 0.76401(13) 0.39388(12) 0.91736(9) 0.0468(6) Uani 1 1 d . . . 
Se5 Se 1.19367(14) 0.11197(13) 0.58089(9) 0.0522(6) Uani 1 1 d . . . 
Se6 Se 1.29624(13) 0.45768(14) 0.71405(9) 0.0503(6) Uani 1 1 d . . . 
Se7 Se 0.98514(13) 0.21391(13) 0.85525(9) 0.0490(6) Uani 1 1 d . . . 
Se8 Se 1.01985(14) 0.38043(14) 0.68494(10) 0.0538(6) Uani 1 1 d . . . 
Se9 Se 1.15352(15) 0.18856(15) 0.77119(10) 0.0578(7) Uani 1 1 d . . . 
Se10 Se 0.83088(14) 0.31649(13) 0.74001(9) 0.0495(6) Uani 1 1 d . . . 
K1 K 0.9780(3) 0.1903(3) 0.7377(2) 0.0639(16) Uani 1 1 d . . . 
K2 K 0.6773(3) 0.1772(3) 0.92490(19) 0.0489(12) Uani 1 1 d . . . 
K3 K 1.3130(3) 0.3483(3) 0.5932(2) 0.0614(16) Uani 1 1 d . . . 
K4 K 0.5000 0.0000 1.0000 0.059(2) Uani 1 2 d S . . 
K5 K 1.2185(4) 0.2597(4) 0.8474(3) 0.0719(19) Uani 1 1 d . . . 
K6 K 1.0188(4) 0.0940(4) 0.9565(3) 0.0715(19) Uani 1 1 d . . . 
K7 K 0.9811(5) 0.4961(4) 0.4289(3) 0.076(2) Uani 1 1 d . . . 
K8 K 0.7444(4) 0.3091(4) 0.6596(3) 0.080(2) Uani 1 1 d . . . 
K9 K 1.0351(4) 0.5451(4) 0.6958(3) 0.079(2) Uani 1 1 d . . . 
K10 K 1.1332(5) 0.5066(5) 0.8990(3) 0.089(3) Uani 1 1 d . . . 
K11 K 0.8169(4) 0.4848(3) 0.7478(2) 0.0629(16) Uani 1 1 d . . . 
K12 K 1.1517(5) 0.0312(4) 0.3911(3) 0.085(2) Uani 1 1 d . . . 
K13 K 0.3995(4) 0.3101(5) 1.0061(3) 0.086(3) Uani 1 1 d . . . 
K14 K 1.0211(5) 0.3055(6) 0.9335(4) 0.101(3) Uani 1 1 d . . . 
K15 K 1.5778(5) 0.4192(4) 0.6969(3) 0.088(2) Uani 1 1 d . . . 
K16 K 0.9778(6) -0.1421(5) 0.6711(4) 0.110(3) Uani 1 1 d . . . 
K17 K 0.5795(7) 0.6732(5) 0.8767(3) 0.112(4) Uani 1 1 d . . . 
K18 K 0.4710(6) 0.2341(5) 0.8894(4) 0.099(3) Uani 1 1 d . . . 
K19 K 1.0007(6) 0.6267(5) 0.8227(5) 0.093(3) Uani 0.80 1 d P . . 
K20 K 0.3323(7) -0.0648(6) 0.9174(4) 0.051(3) Uani 0.50 1 d P . . 
K21 K 1.1243(15) 0.7528(13) 0.6222(9) 0.080(7) Uani 0.50 1 d P . . 
K21' K 1.1513(18) 0.7586(17) 0.6016(12) 0.107(11) Uani 0.50 1 d P . . 
K22 K 1.5050(8) 0.2288(8) 0.6141(7) 0.083(5) Uani 0.50 1 d P . . 
K25 K 1.5000 0.5000 0.5000 0.083(6) Uiso 0.50 2 d SP . . 
K25' K 1.4615(13) 0.5719(12) 0.4626(8) 0.092(6) Uiso 0.40 1 d P . . 
K26 K 1.4004(7) 0.6865(8) 0.5759(6) 0.062(4) Uani 0.40 1 d P . . 
K27 K 0.4899(9) 0.4701(7) 0.9457(6) 0.061(4) Uani 0.40 1 d P . . 
O1 O 0.8185(8) 0.1882(8) 0.8945(5) 0.038(3) Uani 1 1 d . . . 
O2 O 0.6806(9) -0.1795(9) 0.9354(6) 0.050(4) Uani 1 1 d . . . 
O3 O 0.6541(8) 0.3015(9) 0.8922(6) 0.049(4) Uani 1 1 d . . . 
O4 O 0.6804(9) 0.1242(8) 0.8442(6) 0.048(4) Uani 1 1 d . . . 
O5 O 0.9576(8) -0.1283(8) 0.9392(7) 0.049(4) Uani 1 1 d . . . 
O6 O 0.5605(8) 0.0907(8) 0.8314(6) 0.042(4) Uani 1 1 d . . . 
O7 O 0.6361(8) 0.0494(8) 0.9281(5) 0.044(4) Uani 1 1 d . . . 
O8 O 1.2006(10) 0.3381(9) 0.5507(7) 0.057(5) Uani 1 1 d . . . 
O9 O 0.8316(10) 0.0111(8) 0.7325(5) 0.048(4) Uani 1 1 d . . . 
O10 O 1.4405(9) 0.5570(9) 0.5958(7) 0.060(5) Uani 1 1 d . . . 
O11 O 0.6137(9) 0.2574(8) 0.9822(5) 0.043(4) Uani 1 1 d . . . 
O12 O 0.6822(9) 0.4206(10) 1.0280(6) 0.055(5) Uani 1 1 d . . . 
O13 O 0.6547(8) 0.0356(9) 0.7704(5) 0.045(4) Uani 1 1 d . . . 
O14 O 0.5808(10) 0.1213(10) 0.7459(6) 0.062(5) Uani 1 1 d . . . 
O15 O 0.5761(9) -0.1798(9) 1.0137(7) 0.054(5) Uani 1 1 d . . . 
O16 O 0.7020(10) -0.1796(9) 0.8517(6) 0.055(5) Uani 1 1 d . . . 
O17 O 0.9624(9) 0.3083(8) 0.5608(6) 0.048(4) Uani 1 1 d . . . 
O18 O 0.7438(8) 0.2366(8) 0.8395(6) 0.045(4) Uani 1 1 d . . . 
O19 O 1.2011(11) 0.2085(11) 0.4231(7) 0.064(5) Uani 1 1 d . . . 
O20 O 0.6163(10) -0.0883(8) 0.7731(6) 0.050(4) Uani 1 1 d . . . 
O21 O 0.7494(9) 0.2367(9) 0.9653(6) 0.054(5) Uani 1 1 d . . . 
O22 O 0.7544(8) 0.2816(8) 0.7470(6) 0.047(4) Uani 1 1 d . . . 
O23 O 0.8797(10) -0.0752(9) 0.9963(6) 0.052(4) Uani 1 1 d . . . 
O24 O 0.8569(10) 0.5044(8) 0.9691(6) 0.051(4) Uani 1 1 d . . . 
O25 O 1.1039(9) -0.0025(9) 0.5321(6) 0.051(4) Uani 1 1 d . . . 
O26 O 1.1787(9) 0.3652(9) 0.6325(6) 0.054(5) Uani 1 1 d . . . 
O27 O 0.6274(9) -0.0574(8) 0.9933(6) 0.048(4) Uani 1 1 d . . . 
O28 O 0.8009(9) -0.1075(8) 0.8681(6) 0.048(4) Uani 1 1 d . . . 
O29 O 0.5158(10) 0.2987(10) 0.9366(6) 0.055(5) Uani 1 1 d . . . 
O30 O 0.8031(10) -0.2104(8) 0.9328(6) 0.050(4) Uani 1 1 d . . . 
O31 O 0.7232(10) -0.0512(9) 0.9229(6) 0.050(4) Uani 1 1 d . . . 
O32 O 0.5879(9) -0.1228(8) 0.8599(6) 0.048(4) Uani 1 1 d . . . 
O33 O 0.7437(10) 0.5829(10) 0.8856(6) 0.059(5) Uani 1 1 d . . . 
O34 O 0.5374(12) 0.3991(9) 1.0631(8) 0.066(5) Uani 1 1 d . . . 
O35 O 0.8509(9) -0.0866(9) 0.6932(6) 0.049(4) Uani 1 1 d . . . 
O36 O 0.6084(10) -0.2115(8) 0.8162(6) 0.050(4) Uani 1 1 d . . . 
O37 O 0.9215(9) 0.4041(8) 0.9635(6) 0.048(4) Uani 1 1 d . . . 
O38 O 0.7629(10) -0.1331(9) 1.0680(7) 0.058(5) Uani 1 1 d . . . 
O39 O 0.5506(11) 0.1369(9) 0.9018(7) 0.060(5) Uani 1 1 d . . . 
O40 O 0.7581(9) 0.2981(8) 1.0204(6) 0.045(4) Uani 1 1 d . . . 
O41 O 1.1456(9) 0.4804(9) 0.7775(6) 0.049(4) Uani 1 1 d . . . 
O42 O 0.9910(10) 0.5189(10) 0.9057(6) 0.059(5) Uani 1 1 d . . . 
O43 O 0.6425(9) 0.0002(10) 0.8567(6) 0.054(5) Uani 1 1 d . . . 
O44 O 1.0254(8) 0.4045(8) 0.8091(6) 0.047(4) Uani 1 1 d . . . 
O45 O 0.8686(9) 0.3017(8) 0.9552(6) 0.049(4) Uani 1 1 d . . . 
O46 O 0.7329(8) -0.1434(8) 0.7668(7) 0.048(4) Uani 1 1 d . . . 
O47 O 0.8335(9) -0.1827(8) 0.9977(6) 0.049(4) Uani 1 1 d . . . 
O48 O 0.5488(10) 0.0011(9) 0.7550(6) 0.055(5) Uani 1 1 d . . . 
O49 O 1.0802(9) 0.4281(10) 0.4630(6) 0.054(5) Uani 1 1 d . . . 
O50 O 1.2172(10) 0.1545(10) 0.7415(7) 0.060(5) Uani 1 1 d . . . 
O51 O 0.9591(10) 0.4360(9) 0.5278(7) 0.058(5) Uani 1 1 d . . . 
O52 O 0.9554(10) 0.1493(10) 0.8967(7) 0.062(5) Uani 1 1 d . . . 
O53 O 0.7708(9) 0.0635(9) 0.9249(7) 0.058(5) Uani 1 1 d . . . 
O54 O 0.6036(9) 0.4079(8) 0.9021(6) 0.049(4) Uani 1 1 d . . . 
O55 O 0.7130(10) 0.4123(8) 0.8317(6) 0.049(4) Uani 1 1 d . . . 
O56 O 1.3631(10) 0.4743(12) 0.8170(7) 0.069(6) Uani 1 1 d . . . 
O57 O 0.6953(9) 0.1659(8) 0.7537(6) 0.050(4) Uani 1 1 d . . . 
O58 O 0.9693(10) 0.2330(8) 0.4892(7) 0.054(5) Uani 1 1 d . . . 
O59 O 1.0238(9) 0.1354(9) 0.4738(8) 0.062(5) Uani 1 1 d . . . 
O60 O 0.4631(9) -0.1048(9) 0.9192(7) 0.055(5) Uani 1 1 d . . . 
O61 O 1.5001(10) 0.4663(9) 0.6352(7) 0.056(5) Uani 1 1 d . . . 
O62 O 0.8504(8) -0.1064(9) 0.7782(6) 0.048(4) Uani 1 1 d . . . 
O63 O 0.5279(9) 0.0089(8) 0.9100(7) 0.052(4) Uani 1 1 d . . . 
O64 O 0.9437(11) 0.2692(10) 0.8779(6) 0.059(5) Uani 1 1 d . . . 
O65 O 0.5540(10) 0.3613(8) 0.9863(6) 0.050(4) Uani 1 1 d . . . 
O66 O 0.7125(9) -0.1465(9) 0.9987(6) 0.051(4) Uani 1 1 d . . . 
O67 O 1.4159(10) 0.6026(9) 0.6622(6) 0.058(5) Uani 1 1 d . . . 
O68 O 0.9934(11) 0.5291(11) 0.7920(7) 0.069(6) Uani 1 1 d . . . 
O69 O 0.7203(10) -0.0576(8) 0.8023(5) 0.049(4) Uani 1 1 d . . . 
O70 O 0.9357(9) -0.0545(9) 0.8137(6) 0.051(4) Uani 1 1 d . . . 
O71 O 0.8642(10) 0.5344(10) 0.8866(7) 0.059(5) Uani 1 1 d . . . 
O72 O 0.8314(9) -0.2054(8) 0.8476(6) 0.046(4) Uani 1 1 d . . . 
O73 O 1.3145(10) 0.2786(9) 0.5239(8) 0.064(6) Uani 1 1 d . . . 
O74 O 1.1502(11) 0.0955(9) 0.4654(7) 0.060(5) Uani 1 1 d . . . 
O75 O 1.3409(9) 0.4434(11) 0.7515(6) 0.058(5) Uani 1 1 d . . . 
O76 O 0.8722(9) 0.2574(9) 0.7627(6) 0.052(4) Uani 1 1 d . . . 
O77 O 0.7609(12) 0.5062(10) 1.0500(7) 0.068(6) Uani 1 1 d . . . 
O78 O 1.2124(11) -0.0109(11) 0.4588(8) 0.068(6) Uani 1 1 d . . . 
O79 O 1.3064(9) 0.5737(8) 0.6182(7) 0.054(5) Uani 1 1 d . . . 
O80 O 1.1828(10) 0.5179(9) 0.6678(7) 0.056(5) Uani 1 1 d . . . 
O81 O 0.9590(11) 0.3094(10) 0.4081(7) 0.063(5) Uani 1 1 d . . . 
O82 O 0.9452(9) 0.2080(8) 0.8186(6) 0.048(4) Uani 1 1 d . . . 
O83 O 0.8093(9) 0.3554(8) 0.7786(6) 0.049(4) Uani 1 1 d . . . 
O84 O 1.0969(10) 0.3125(10) 0.8467(6) 0.059(5) Uani 1 1 d . . . 
O85 O 0.9680(9) -0.1615(9) 0.7902(6) 0.057(5) Uani 1 1 d . . . 
O86 O 0.9956(11) -0.0398(10) 0.7064(6) 0.064(5) Uani 1 1 d . . . 
O87 O 1.4161(10) 0.1247(10) 0.4381(7) 0.064(5) Uani 1 1 d . . . 
O88 O 0.6123(11) 0.4694(9) 0.9748(6) 0.055(5) Uani 1 1 d . . . 
O89 O 0.5874(9) -0.0954(10) 0.9345(6) 0.053(5) Uani 1 1 d . . . 
O90 O 0.9229(9) -0.1612(9) 0.8761(6) 0.052(4) Uani 1 1 d . . . 
O91 O 1.2424(9) 0.2687(8) 0.6722(7) 0.053(4) Uani 1 1 d . . . 
O92 O 0.6673(9) 0.0595(11) 1.0007(7) 0.059(5) Uani 1 1 d . . . 
O93 O 0.6286(9) 0.5266(8) 0.8920(6) 0.046(4) Uani 1 1 d . . . 
O94 O 0.6824(12) 0.1942(10) 0.6698(7) 0.066(5) Uani 1 1 d . . . 
O95 O 1.0137(10) 0.0812(9) 0.5565(7) 0.059(5) Uani 1 1 d . . . 
O96 O 1.2773(10) 0.0851(11) 0.4762(7) 0.067(6) Uani 1 1 d . . . 
O97 O 0.6224(11) 0.5999(9) 0.9477(8) 0.065(5) Uani 1 1 d . . . 
O98 O 0.8563(9) 0.4853(8) 0.8245(6) 0.048(4) Uani 1 1 d . . . 
O99 O 0.6645(10) 0.1919(10) 1.0489(7) 0.058(5) Uani 1 1 d . . . 
O100 O 1.1558(12) 0.0827(11) 0.5504(8) 0.074(6) Uani 1 1 d . . . 
O101 O 1.1419(10) 0.3703(9) 0.7578(6) 0.056(5) Uani 1 1 d . . . 
O102 O 1.4417(10) 0.3745(11) 0.7045(7) 0.064(5) Uani 1 1 d . . . 
O103 O 1.3593(10) 0.3408(10) 0.6653(7) 0.062(5) Uani 1 1 d . . . 
O104 O 0.7233(10) -0.2844(9) 0.9104(6) 0.055(5) Uani 1 1 d . . . 
O105 O 1.2414(9) 0.5065(11) 0.8093(7) 0.061(5) Uani 1 1 d . . . 
O106 O 1.3138(9) 0.0140(11) 0.6488(6) 0.059(5) Uani 1 1 d . . . 
O107 O 1.0845(10) 0.3671(10) 0.4067(6) 0.058(5) Uani 1 1 d . . . 
O108 O 1.0207(10) 0.0378(10) 0.7523(5) 0.058(5) Uani 1 1 d . . . 
O109 O 1.0149(9) -0.0262(9) 0.9494(7) 0.056(5) Uani 1 1 d . . . 
O110 O 1.4792(9) 0.5117(10) 0.7019(6) 0.056(5) Uani 1 1 d . . . 
O111 O 1.0407(10) 0.3076(10) 0.6971(7) 0.061(5) Uani 1 1 d . . . 
O112 O 1.4544(10) 0.4157(9) 0.7707(8) 0.063(5) Uani 1 1 d . . . 
O113 O 1.1910(10) 0.4604(9) 0.3854(7) 0.057(5) Uani 1 1 d . . . 
O114 O 1.3216(11) 0.3152(12) 0.7577(9) 0.077(7) Uani 1 1 d . . . 
O115 O 1.0161(11) 0.2403(12) 0.6274(7) 0.073(6) Uani 1 1 d . . . 
O116 O 1.0781(11) 0.2464(9) 0.4222(7) 0.063(5) Uani 1 1 d . . . 
O117 O 0.9040(10) 0.0307(9) 0.9303(7) 0.056(5) Uani 1 1 d . . . 
O118 O 1.1719(9) 0.5932(9) 0.7198(5) 0.048(4) Uani 1 1 d . . . 
O119 O 0.7394(9) 0.5355(9) 0.8230(7) 0.055(5) Uani 1 1 d . . . 
O120 O 1.2755(10) 0.4612(9) 0.6148(7) 0.055(5) Uani 1 1 d . . . 
O121 O 1.0899(10) 0.4194(11) 0.8689(7) 0.067(6) Uani 1 1 d . . . 
O122 O 0.9773(10) -0.0285(10) 0.8741(6) 0.058(5) Uani 1 1 d . . . 
O123 O 1.2691(11) 0.2054(10) 0.6082(7) 0.065(5) Uani 1 1 d . . . 
O124 O 1.4077(13) 0.2417(11) 0.5691(8) 0.076(6) Uani 1 1 d . . . 
O125 O 1.0452(10) 0.4051(10) 0.6279(7) 0.062(5) Uani 1 1 d . . . 
O126 O 0.8558(10) 0.6157(9) 0.8066(7) 0.056(5) Uani 1 1 d . . . 
O127 O 0.9296(10) 0.4379(9) 0.8760(6) 0.052(4) Uani 1 1 d . . . 
O128 O 1.1963(10) 0.2568(11) 0.7677(7) 0.060(5) Uani 1 1 d . . . 
O129 O 1.0769(12) -0.0427(16) 0.8048(8) 0.105(11) Uani 1 1 d . . . 
O130 O 0.6245(10) 0.3085(9) 1.0418(6) 0.054(5) Uani 1 1 d . . . 
O131 O 0.8931(11) 0.1236(9) 0.5378(7) 0.060(5) Uani 1 1 d . . . 
O132 O 1.3207(11) 0.4055(9) 0.4933(8) 0.067(6) Uani 1 1 d . . . 
O133 O 0.9287(11) -0.2540(10) 0.9513(7) 0.066(5) Uani 1 1 d . . . 
O134 O 0.8882(10) 0.3644(9) 0.8332(6) 0.054(5) Uani 1 1 d . . . 
O135 O 1.2770(10) 0.5326(9) 0.7135(7) 0.056(5) Uani 1 1 d . . . 
O136 O 1.0555(16) 0.0734(15) 0.8174(12) 0.121(11) Uiso 1 1 d D . . 
O137 O 1.0842(11) 0.3122(9) 0.4864(6) 0.056(5) Uani 1 1 d . . . 
O138 O 1.2648(9) 0.6156(10) 0.7552(7) 0.057(5) Uani 1 1 d . . . 
O139 O 0.6125(10) 0.4927(10) 0.8191(6) 0.058(5) Uani 1 1 d . . . 
O140 O 1.3236(10) 0.2834(10) 0.3658(7) 0.064(5) Uani 1 1 d . . . 
O141 O 1.0911(10) 0.1903(9) 0.5047(6) 0.055(5) Uani 1 1 d . . . 
O142 O 1.1176(12) 0.1487(12) 0.3899(8) 0.072(6) Uani 1 1 d . . . 
O143 O 0.7522(9) -0.0340(9) 0.9953(6) 0.051(4) Uani 1 1 d . . . 
O144 O 0.9639(10) 0.1878(10) 0.5744(7) 0.064(5) Uani 1 1 d . . . 
O145 O 1.3831(12) 0.6986(11) 0.7037(8) 0.071(6) Uani 1 1 d . . . 
O146 O 1.2107(8) 0.3897(10) 0.8145(6) 0.054(5) Uani 1 1 d . . . 
O147 O 1.0771(11) 0.1359(10) 0.6779(7) 0.066(5) Uani 1 1 d . . . 
O148 O 0.8421(10) -0.0862(10) 0.9310(6) 0.057(5) Uani 1 1 d . . . 
O149 O 1.1063(10) 0.2146(10) 0.7367(7) 0.064(5) Uani 1 1 d . . . 
O150 O 1.2455(11) 0.4135(11) 0.8857(8) 0.069(6) Uani 1 1 d . . . 
O151 O 0.5221(11) -0.0217(10) 0.8386(7) 0.061(5) Uani 1 1 d . . . 
O152 O 1.1284(11) 0.5783(11) 0.8115(7) 0.068(6) Uani 1 1 d . . . 
O153 O 0.9499(11) 0.0773(12) 0.6952(8) 0.074(6) Uani 1 1 d . . . 
O154 O 0.9867(11) -0.0360(10) 0.6076(8) 0.073(6) Uani 1 1 d . . . 
O155 O 1.5543(11) 0.5864(11) 0.6158(8) 0.068(6) Uani 1 1 d . . . 
O156 O 1.4123(11) 0.4401(10) 0.5959(7) 0.062(5) Uani 1 1 d . . . 
O157 O 0.8082(9) 0.3980(8) 1.0306(6) 0.047(4) Uani 1 1 d . . . 
O158 O 0.7314(10) -0.0345(9) 0.7119(7) 0.060(5) Uani 1 1 d . . . 
O159 O 1.0528(11) 0.0551(10) 0.6312(6) 0.060(5) Uani 1 1 d . . . 
O160 O 1.1973(19) -0.0570(9) 0.6601(7) 0.109(12) Uani 1 1 d . . . 
O161 O 0.9709(9) 0.3559(9) 0.4760(6) 0.048(4) Uani 1 1 d . . . 
O162 O 0.8972(13) 0.2978(9) 0.6492(7) 0.065(6) Uani 1 1 d . . . 
O163 O 1.3680(11) 0.5371(11) 0.5386(7) 0.064(5) Uani 1 1 d . . . 
O164 O 1.1196(12) -0.0379(10) 0.6096(8) 0.071(6) Uani 1 1 d . . . 
O165 O 1.2033(13) 0.2631(10) 0.4936(7) 0.069(6) Uani 1 1 d . . . 
O166 O 0.6893(9) 0.3594(8) 0.9563(6) 0.045(4) Uani 1 1 d . . . 
O167 O 1.2044(11) 0.3324(9) 0.4082(7) 0.060(5) Uani 1 1 d . . . 
O168 O 0.8896(11) 0.1726(8) 0.6610(7) 0.062(5) Uani 1 1 d . . . 
O169 O 1.3666(9) 0.4703(10) 0.6671(6) 0.056(5) Uani 1 1 d . . . 
O170 O 0.8904(10) 0.2963(11) 1.0324(7) 0.063(5) Uani 1 1 d . . . 
O171 O 0.6612(13) 0.0639(10) 0.6887(7) 0.071(6) Uani 1 1 d . . . 
O172 O 0.7296(10) 0.5247(8) 0.9688(6) 0.053(4) Uani 1 1 d . . . 
O173 O 1.2083(10) 0.3929(10) 0.4664(8) 0.065(5) Uani 1 1 d . . . 
O174 O 1.4338(12) 0.2899(12) 0.7868(8) 0.073(6) Uani 1 1 d . . . 
O175 O 0.9446(10) 0.4534(9) 0.7548(6) 0.053(4) Uani 1 1 d . . . 
O176 O 1.2279(11) -0.0184(11) 0.5388(6) 0.062(5) Uani 1 1 d . . . 
O177 O 1.0800(10) 0.4204(10) 0.6955(7) 0.059(5) Uani 1 1 d . . . 
O178 O 0.7341(11) 0.4618(10) 0.8992(6) 0.059(5) Uani 1 1 d . . . 
O179 O 0.8046(9) 0.4138(10) 0.9510(6) 0.055(5) Uani 1 1 d . . . 
O180 O 1.2955(10) 0.6463(9) 0.6680(7) 0.063(5) Uani 1 1 d . . . 
O181 O 1.3321(11) 0.3603(10) 0.8229(6) 0.057(5) Uani 1 1 d . . . 
O182 O 1.3137(11) 0.2056(10) 0.4489(8) 0.067(6) Uani 1 1 d . . . 
O183 O 0.4496(10) 0.0707(12) 0.7994(7) 0.068(6) Uani 1 1 d . . . 
O184 O 0.8497(10) 0.1261(12) 0.7494(8) 0.074(6) Uani 1 1 d . . . 
O185 O 1.3109(9) -0.0360(10) 0.5846(8) 0.070(6) Uani 1 1 d . . . 
O186 O 1.3866(10) 0.5687(12) 0.7483(7) 0.068(6) Uani 1 1 d . . . 
O187 O 0.6151(10) -0.0482(10) 0.6850(7) 0.059(5) Uani 1 1 d . . . 
O188 O 1.3567(12) 0.1227(10) 0.5864(8) 0.070(6) Uani 1 1 d . . . 
O189 O 0.8383(11) 0.2443(11) 0.5985(8) 0.070(6) Uani 1 1 d . . . 
O190 O 0.8740(12) 0.0612(11) 0.6447(9) 0.078(7) Uani 1 1 d . . . 
O191 O 1.3097(9) 0.3244(10) 0.4424(7) 0.060(5) Uani 1 1 d . . . 
O192 O 1.1902(10) 0.6426(11) 0.6289(7) 0.065(5) Uani 1 1 d . . . 
O193 O 1.2329(11) 0.0482(9) 0.6028(7) 0.061(5) Uani 1 1 d . . . 
O194 O 1.3574(12) 0.0692(11) 0.5266(7) 0.071(6) Uani 1 1 d . . . 
O195 O 1.4990(11) 0.5278(13) 0.7786(9) 0.080(7) Uani 1 1 d . . . 
O196 O 0.7693(9) 0.1059(9) 0.6983(6) 0.053(4) Uani 1 1 d . . . 
O197 O 1.4990(11) 0.3523(11) 0.6211(8) 0.071(6) Uani 1 1 d . . . 
O198 O 1.2112(13) -0.1326(11) 0.6060(7) 0.073(6) Uani 1 1 d . . . 
O199 O 1.0703(10) 0.3824(10) 0.5495(6) 0.058(5) Uani 1 1 d . . . 
O200 O 0.9256(16) 0.0661(13) 0.8194(10) 0.097(9) Uani 1 1 d . . . 
O201 O 1.2644(9) 0.1547(9) 0.5395(6) 0.050(4) Uani 1 1 d . . . 
O202 O 1.2348(13) 0.0952(11) 0.6770(8) 0.075(6) Uani 1 1 d . . . 
O203 O 1.2171(13) -0.0225(13) 0.7342(7) 0.078(7) Uani 1 1 d . . . 
O204 O 1.4365(11) 0.0183(13) 0.5811(9) 0.083(7) Uani 1 1 d . . . 
O205 O 1.1235(10) 0.0204(11) 0.6856(7) 0.069(6) Uani 1 1 d . . . 
O206 O 1.3878(11) 0.1873(12) 0.5035(8) 0.078(7) Uani 1 1 d . . . 
O211 O 1.1272(16) 0.1547(15) 0.8847(10) 0.099(8) Uiso 1 1 d . . . 
O212 O 0.5527(10) 0.1239(10) 0.9870(6) 0.057(5) Uiso 1 1 d . . . 
O213 O 1.0351(11) 0.3533(11) 0.9930(7) 0.066(5) Uiso 1 1 d . . . 
O214 O 1.1586(11) 0.2839(11) 0.9297(7) 0.065(5) Uiso 1 1 d . . . 
O215 O 0.7576(17) 0.4197(17) 0.6938(11) 0.110(10) Uiso 1 1 d . . . 
O216 O 0.9212(14) 0.5113(13) 0.6623(9) 0.086(7) Uiso 1 1 d . . . 
O219 O 0.6349(10) -0.0335(10) 0.5965(6) 0.056(5) Uiso 1 1 d . . . 
O220 O 0.9134(12) 0.4304(11) 0.3940(7) 0.069(6) Uiso 1 1 d . . . 
O221 O 0.8462(15) 0.4947(14) 0.5003(10) 0.093(8) Uiso 1 1 d . . . 
O222 O 0.4621(14) 0.2488(14) 1.0653(9) 0.089(7) Uiso 1 1 d . . . 
O223 O 0.2955(14) 0.2807(13) 0.9784(9) 0.087(7) Uiso 1 1 d . . . 
O224 O 0.3976(18) 0.0539(17) 0.9152(12) 0.114(10) Uiso 1 1 d . . . 
O225 O 0.8319(12) 0.6343(11) 0.9274(8) 0.072(6) Uiso 1 1 d . . . 
O226 O 0.4721(11) 0.4363(10) 0.8722(7) 0.062(5) Uiso 1 1 d . . . 
O227 O 1.5432(18) 0.7075(17) 0.5656(12) 0.114(10) Uiso 1 1 d . . . 
O228 O 1.2760(16) 0.1154(15) 0.3749(10) 0.099(8) Uiso 1 1 d . . . 
O229 O 1.2047(13) 0.0312(12) 0.8025(8) 0.078(6) Uiso 1 1 d . . . 
O230 O 0.9807(19) 0.1876(18) 0.9939(12) 0.118(11) Uiso 1 1 d . . . 
O231 O 0.8883(15) 0.4264(14) 0.6243(10) 0.094(8) Uiso 1 1 d . . . 
O232 O 0.8113(15) -0.2598(14) 0.7858(10) 0.094(8) Uiso 1 1 d . . . 
O233 O 1.0690(14) 0.8561(14) 0.5791(9) 0.089(7) Uiso 1 1 d . . . 
O234 O 1.1736(17) 0.6264(16) 0.8846(11) 0.106(9) Uiso 1 1 d . . . 
O235 O 0.4685(16) -0.1376(15) 0.8134(10) 0.102(9) Uiso 1 1 d . . . 
O236 O 0.6875(16) -0.3386(16) 0.8098(11) 0.104(9) Uiso 1 1 d . . . 
O237 O 1.5409(16) 0.2227(15) 0.8018(10) 0.099(8) Uiso 1 1 d . . . 
O238 O 0.7848(19) 0.4463(18) 0.4516(12) 0.121(11) Uiso 1 1 d . . . 
O239 O 0.1925(16) 0.3623(15) 0.9849(10) 0.101(9) Uiso 1 1 d . . . 
O240 O 0.7717(17) 0.1326(16) 0.5979(11) 0.106(9) Uiso 1 1 d . . . 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
W1 O15 1.726(19) . ? 
W1 O66 1.894(18) . ? 
W1 O27 1.894(18) . ? 
W1 O2 1.914(19) . ? 
W1 O89 1.915(17) . ? 
W1 O31 2.339(18) . ? 
W1 K13 4.011(10) 2_657 ? 
W2 O85 1.699(19) . ? 
W2 O70 1.79(2) . ? 
W2 O90 1.95(2) . ? 
W2 O62 1.961(15) . ? 
W2 O72 2.042(16) . ? 
W2 O28 2.322(18) . ? 
W2' O70 1.60(6) . ? 
W2' O90 1.76(6) . ? 
W2' O28 1.97(5) . ? 
W2' O85 2.11(5) . ? 
W2' O72 2.16(6) . ? 
W2' O62 2.16(5) . ? 
W2' Se1 3.02(5) . ? 
W3' O35 1.35(5) . ? 
W3' O62 1.85(5) . ? 
W3' O46 1.98(5) . ? 
W3' O9 2.13(5) . ? 
W3' O158 2.14(5) . ? 
W3' K12 3.78(5) 2_756 ? 
W3' K16 3.83(5) . ? 
W3 O35 1.721(18) . ? 
W3 O62 1.833(16) . ? 
W3 O9 1.880(18) . ? 
W3 O46 1.981(16) . ? 
W3 O158 2.003(19) . ? 
W3 O69 2.289(18) . ? 
W3 K12 4.021(9) 2_756 ? 
W4 O92 1.74(2) . ? 
W4 O53 1.777(17) . ? 
W4 O7 1.901(16) . ? 
W4 O143 1.99(2) . ? 
W4 O27 2.025(17) . ? 
W4 O31 2.26(2) . ? 
W4 K2 3.531(6) . ? 
W4 K4 3.7783(17) . ? 
W4' O92 1.36(5) . ? 
W4' O143 1.92(6) . ? 
W4' O53 1.93(6) . ? 
W4' O27 2.07(6) . ? 
W4' O7 2.11(5) . ? 
W4' K2 3.48(6) . ? 
W4' K4 3.74(5) . ? 
W4' K20 3.86(5) 2_657 ? 
W5 O39 1.752(18) . ? 
W5 O4 1.802(17) . ? 
W5 O7 1.929(16) . ? 
W5 O6 1.961(16) . ? 
W5 O63 2.036(18) . ? 
W5 O43 2.26(2) . ? 
W5 K2 3.542(6) . ? 
W5 K4 3.8205(11) . ? 
W6 O109 1.711(19) . ? 
W6 O117 1.752(19) . ? 
W6 O122 1.91(2) . ? 
W6 O23 1.963(17) . ? 
W6 O5 2.006(18) . ? 
W6 O148 2.38(2) . ? 
W6 K6 3.713(8) . ? 
W6 K6 3.750(7) 2_757 ? 
W7 O139 1.723(18) . ? 
W7 O55 1.812(17) . ? 
W7 O54 1.944(17) . ? 
W7 O119 1.953(18) . ? 
W7 O93 2.026(18) . ? 
W7 O178 2.373(19) . ? 
W7 K11 3.837(7) . ? 
W7 K27 3.927(17) . ? 
W8 O60 1.718(17) . ? 
W8 O89 1.880(17) . ? 
W8 O63 1.907(18) . ? 
W8 O151 1.94(2) . ? 
W8 O32 1.957(18) . ? 
W8 O43 2.32(2) . ? 
W8 K4 4.0747(12) . ? 
W8 K20 4.105(13) . ? 
W9 O34 1.69(2) . ? 
W9 O65 1.898(17) . ? 
W9 O12 1.908(16) . ? 
W9 O130 1.911(19) . ? 
W9 O88 1.946(18) . ? 
W9 K27 3.905(18) . ? 
W9 K27 3.913(17) 2_667 ? 
W10 O94 1.74(2) . ? 
W10 O57 1.751(19) . ? 
W10 O196 1.907(19) . ? 
W10 O14 1.921(19) . ? 
W10 O171 2.062(18) . ? 
W10 O13 2.383(18) . ? 
W10 K8 3.970(9) . ? 
W11 O51 1.71(2) . ? 
W11 O199 1.777(19) . ? 
W11 O17 1.886(16) . ? 
W11 O49 1.968(18) . ? 
W11 O161 2.041(17) . ? 
W11 O137 2.33(2) . ? 
W11 K7 3.619(7) . ? 
W11 K7 3.700(8) 2_766 ? 
W12 O187 1.70(2) . ? 
W12 O171 1.86(2) . ? 
W12 O158 1.881(19) . ? 
W12 O20 1.930(18) . ? 
W12 O48 1.938(19) . ? 
W12 O13 2.376(18) . ? 
W13 O150 1.73(2) . ? 
W13 O146 1.868(16) . ? 
W13 O105 1.90(2) . ? 
W13 O56 1.917(19) . ? 
W13 O181 1.94(2) . ? 
W13 O75 2.44(2) . ? 
W13 K5 3.856(9) . ? 
W13 K10 3.864(9) . ? 
W14 O99 1.68(2) . ? 
W14 O21 1.778(19) . ? 
W14 O11 1.915(16) . ? 
W14 O40 1.931(16) . ? 
W14 O130 1.982(18) . ? 
W14 O166 2.451(16) . ? 
W14 K2 3.735(6) . ? 
W15 O132 1.760(18) . ? 
W15 O8 1.78(2) . ? 
W15 O73 1.896(18) . ? 
W15 O173 1.97(2) . ? 
W15 O191 1.98(2) . ? 
W15 O165 2.28(2) . ? 
W15 K3 3.560(7) . ? 
W16 O97 1.71(2) . ? 
W16 O93 1.864(18) . ? 
W16 O88 1.881(19) . ? 
W16 O33 1.91(2) . ? 
W16 O172 1.947(17) . ? 
W16 O178 2.53(2) . ? 
W16 K27 3.803(18) . ? 
W16 K17 3.830(12) . ? 
W17 O42 1.727(18) . ? 
W17 O127 1.787(19) . ? 
W17 O37 1.910(17) . ? 
W17 O71 1.95(2) . ? 
W17 O24 1.989(19) . ? 
W17 O179 2.425(18) . ? 
W17 K19 3.968(13) . ? 
W18 O113 1.73(2) . ? 
W18 O167 1.88(2) . ? 
W18 O49 1.886(19) . ? 
W18 O173 1.91(2) . ? 
W18 O107 1.94(2) . ? 
W18 O137 2.389(18) . ? 
W19 O152 1.69(3) . ? 
W19 O41 1.766(18) . ? 
W19 O118 1.882(17) . ? 
W19 O105 1.95(2) . ? 
W19 O138 2.001(18) . ? 
W19 O135 2.40(2) . ? 
W19 K10 3.808(9) . ? 
W20 O126 1.75(2) . ? 
W20 O98 1.848(17) . ? 
W20 O71 1.90(2) . ? 
W20 O119 1.928(18) . ? 
W20 O33 1.94(2) . ? 
W20 O178 2.44(2) . ? 
W20 K11 3.865(8) . ? 
W20 K19 3.996(11) . ? 
W21 O29 1.705(18) . ? 
W21 O3 1.814(18) . ? 
W21 O54 1.913(17) . ? 
W21 O11 1.945(16) . ? 
W21 O65 1.979(16) . ? 
W21 O166 2.416(18) . ? 
W21 K2 3.778(6) . ? 
W21 K13 3.889(8) . ? 
W21 K27 3.930(17) . ? 
W21 K18 4.140(10) . ? 
W22 O154 1.72(2) . ? 
W22 O95 1.83(2) . ? 
W22 O159 1.869(19) . ? 
W22 O25 1.952(16) . ? 
W22 O164 2.01(2) . ? 
W22 O100 2.31(2) . ? 
W22 K16 3.948(11) . ? 
W23 O124 1.75(2) . ? 
W23 O123 1.77(2) . ? 
W23 O188 1.92(2) . ? 
W23 O73 1.928(19) . ? 
W23 O206 2.01(3) . ? 
W23 O201 2.299(18) . ? 
W23 K3 3.639(7) . ? 
W24' O153 1.76(4) . ? 
W24' O168 1.82(3) . ? 
W24' O9 1.93(3) . ? 
W24' O196 1.95(3) . ? 
W24' O184 1.98(3) . ? 
W24' O190 2.04(4) . ? 
W24' K1 3.91(3) . ? 
W24 O190 1.62(3) . ? 
W24 O168 1.860(17) . ? 
W24 O153 1.88(2) . ? 
W24 O196 1.891(19) . ? 
W24 O9 1.951(17) . ? 
W24 O184 2.39(2) . ? 
W25 O163 1.73(2) . ? 
W25 O120 1.803(19) . ? 
W25 O79 1.943(16) . ? 
W25 O156 1.95(2) . ? 
W25 O10 2.066(17) . ? 
W25 O169 2.407(18) . ? 
W25 K25 3.6569(12) . ? 
W25 K3 3.771(7) . ? 
W25 K26 3.944(18) . ? 
W25 K25' 4.10(3) . ? 
W26 O38 1.76(2) . ? 
W26 O23 1.888(19) . ? 
W26 O143 1.893(19) . ? 
W26 O47 1.92(2) . ? 
W26 O66 1.939(18) . ? 
W26 O148 2.407(18) . ? 
W27 O197 1.69(3) . ? 
W27 O103 1.803(19) . ? 
W27 O102 1.90(2) . ? 
W27 O156 1.928(19) . ? 
W27 O61 2.013(19) . ? 
W27 O169 2.38(2) . ? 
W27 K25' 3.44(3) 2_866 ? 
W27 K3 3.745(7) . ? 
W27 K15 3.867(10) . ? 
W28 O77 1.749(19) . ? 
W28 O157 1.887(17) . ? 
W28 O172 1.892(17) . ? 
W28 O24 1.90(2) . ? 
W28 O12 1.925(17) . ? 
W28 O179 2.50(2) . ? 
W29 O195 1.72(2) . ? 
W29 O186 1.86(2) . ? 
W29 O110 1.875(18) . ? 
W29 O56 1.90(2) . ? 
W29 O112 1.91(2) . ? 
W29 O75 2.496(19) . ? 
W29 K15 3.834(10) . ? 
W30 O81 1.76(2) . ? 
W30 O58 1.889(18) . ? 
W30 O161 1.901(19) . ? 
W30 O116 1.918(18) . ? 
W30 O107 1.926(19) . ? 
W30 O137 2.41(2) . ? 
W31 O68 1.73(2) . ? 
W31 O175 1.764(18) . ? 
W31 O44 1.908(17) . ? 
W31 O98 2.010(18) . ? 
W31 O127 2.144(19) . ? 
W31 O134 2.271(18) . ? 
W31 K9 3.546(8) . ? 
W31 K11 3.762(7) . ? 
W32 O142 1.72(2) . ? 
W32 O19 1.88(2) . ? 
W32 O59 1.883(18) . ? 
W32 O74 1.911(18) . ? 
W32 O116 1.91(2) . ? 
W32 O141 2.33(2) . ? 
W32 K12 3.771(9) . ? 
W33 O162 1.78(2) . ? 
W33 O115 1.79(2) . ? 
W33 O17 1.907(16) . ? 
W33 O168 1.937(16) . ? 
W33 O144 2.15(2) . ? 
W33 O189 2.23(2) . ? 
W33 K8 4.077(9) . ? 
W34 O104 1.696(19) . ? 
W34 O72 1.867(17) . ? 
W34 O30 1.891(18) . ? 
W34 O2 1.903(18) . ? 
W34 O16 1.93(2) . ? 
W34 O28 2.334(18) . ? 
W34 K13 3.932(10) 2_657 ? 
W35 O170 1.72(2) . ? 
W35 O45 1.739(18) . ? 
W35 O40 1.909(18) . ? 
W35 O37 1.944(18) . ? 
W35 O157 2.000(18) . ? 
W35 O179 2.339(19) . ? 
W35 K14 3.680(10) . ? 
W36 O36 1.705(18) . ? 
W36 O32 1.867(17) . ? 
W36 O16 1.87(2) . ? 
W36 O46 1.891(19) . ? 
W36 O20 1.900(17) . ? 
W36 O69 2.320(18) . ? 
W36 K17 4.114(11) 1_545 ? 
W37 O131 1.74(2) . ? 
W37 O144 1.79(2) . ? 
W37 O58 1.931(18) . ? 
W37 O95 1.95(2) . ? 
W37 O59 1.98(2) . ? 
W37 O141 2.321(19) . ? 
W38 O192 1.71(2) . ? 
W38 O80 1.78(2) . ? 
W38 O79 1.902(17) . ? 
W38 O118 1.956(17) . ? 
W38 O180 2.011(19) . ? 
W38 O135 2.35(2) . ? 
W38 K9 3.784(8) . ? 
W38 K26 4.003(16) . ? 
W39 O183 1.71(2) . ? 
W39 O151 1.88(2) . ? 
W39 O48 1.899(16) . ? 
W39 O14 1.907(19) . ? 
W39 O6 1.909(17) . ? 
W39 O13 2.417(15) . ? 
W40 O78 1.73(2) . ? 
W40 O176 1.86(2) . ? 
W40 O25 1.893(17) . ? 
W40 O74 1.903(18) . ? 
W40 O96 1.92(2) . ? 
W40 O100 2.32(3) . ? 
W40 K12 3.832(8) . ? 
W41 O140 1.750(19) . ? 
W41 O191 1.89(2) . ? 
W41 O182 1.91(2) . ? 
W41 O19 1.94(2) . ? 
W41 O167 1.947(19) . ? 
W41 O165 2.36(2) . ? 
W42 O121 1.69(2) . ? 
W42 O84 1.71(2) . ? 
W42 O44 1.908(15) . ? 
W42 O146 2.010(16) . ? 
W42 O41 2.171(19) . ? 
W42 O101 2.29(2) . ? 
W42 K14 3.506(11) . ? 
W42 K5 3.755(8) . ? 
W43 O133 1.73(2) . ? 
W43 O90 1.906(19) . ? 
W43 O5 1.910(17) . ? 
W43 O30 1.940(18) . ? 
W43 O47 1.957(18) . ? 
W43 O148 2.43(2) . ? 
W44 O155 1.70(2) . ? 
W44 O10 1.81(2) . ? 
W44 O61 1.87(2) . ? 
W44 O67 1.923(18) . ? 
W44 O110 1.969(18) . ? 
W44 K15 3.878(9) . ? 
W44 K26 3.944(18) . ? 
W45 O203 1.73(2) . ? 
W45 O202 1.78(2) . ? 
W45 O106 1.877(18) . ? 
W45 O205 1.94(2) . ? 
W45 O160 2.06(2) . ? 
W45 O193 2.41(2) . ? 
W46 O136 1.694(18) . ? 
W46 O200 1.73(3) . ? 
W46 O122 1.91(2) . ? 
W46 O108 1.923(17) . ? 
W46 O70 2.170(19) . ? 
W46 O129 2.21(3) . ? 
W46 K1 4.042(8) . ? 
W47 O145 1.76(2) . ? 
W47 O180 1.88(2) . ? 
W47 O138 1.878(19) . ? 
W47 O67 1.916(17) . ? 
W47 O186 1.96(2) . ? 
W47 O135 2.486(18) . ? 
W47 K26 4.002(19) . ? 
W48 O87 1.721(19) . ? 
W48 O182 1.87(2) . ? 
W48 O206 1.88(3) . ? 
W48 O96 1.89(2) . ? 
W48 O194 1.92(2) . ? 
W48 O201 2.307(18) . ? 
W49 O174 1.69(2) . ? 
W49 O114 1.79(2) . ? 
W49 O102 1.93(2) . ? 
W49 O181 1.955(19) . ? 
W49 O112 2.01(2) . ? 
W49 O75 2.34(2) . ? 
W49 K15 3.871(9) . ? 
W49 K5 3.907(8) . ? 
W50 O204 1.69(2) . ? 
W50 O194 1.88(2) . ? 
W50 O185 1.89(2) . ? 
W50 O106 1.916(19) . ? 
W50 O188 1.95(2) . ? 
W50 O193 2.39(2) . ? 
W51 W51' 0.512(11) . ? 
W51 O86 1.68(2) . ? 
W51 O108 1.873(18) . ? 
W51 O205 1.88(2) . ? 
W51 O153 1.90(3) . ? 
W51 O159 1.950(18) . ? 
W51 O147 2.38(2) . ? 
W51' O108 1.69(2) . ? 
W51' O205 1.71(2) . ? 
W51' O147 1.94(3) . ? 
W51' O153 2.03(3) . ? 
W51' O159 2.10(2) . ? 
W51' O86 2.16(3) . ? 
W51' K1 3.861(14) . ? 
W52 O198 1.69(2) . ? 
W52 O160 1.84(2) . ? 
W52 O164 1.87(2) . ? 
W52 O185 1.951(18) . ? 
W52 O176 1.97(2) . ? 
W52 O193 2.41(2) . ? 
Pd1 O91 1.908(19) . ? 
Pd1 O202 1.97(2) . ? 
Pd1 O50 2.02(2) . ? 
Pd1 O123 2.03(2) . ? 
Pd1 Pd10 3.122(3) . ? 
Pd1 K3 3.957(8) . ? 
Pd2 O125 1.97(2) . ? 
Pd2 O26 1.973(18) . ? 
Pd2 O199 1.985(19) . ? 
Pd2 O8 2.02(2) . ? 
Pd2 Pd4 3.236(3) . ? 
Pd2 Pd10 3.243(3) . ? 
Pd2 K7 3.701(8) 2_766 ? 
Pd2 K3 3.894(7) . ? 
Pd3 O91 1.98(2) . ? 
Pd3 O103 1.99(2) . ? 
Pd3 O128 2.01(2) . ? 
Pd3 O114 2.04(2) . ? 
Pd3 Pd10 3.209(3) . ? 
Pd3 K3 3.716(7) . ? 
Pd3 K5 4.041(8) . ? 
Pd4 O26 1.92(2) . ? 
Pd4 O120 1.974(19) . ? 
Pd4 O80 2.02(2) . ? 
Pd4 O177 2.05(2) . ? 
Pd4 Pd10 3.235(3) . ? 
Pd4 K3 3.765(8) . ? 
Pd4 K9 3.963(10) . ? 
Pd5 O1 1.931(16) . ? 
Pd5 O21 2.015(18) . ? 
Pd5 O45 2.036(18) . ? 
Pd5 O64 2.06(2) . ? 
Pd5 Pd8 3.202(3) . ? 
Pd5 Pd9 3.223(3) . ? 
Pd5 K2 3.719(6) . ? 
Pd5 K14 4.012(11) . ? 
Pd6 O18 1.973(17) . ? 
Pd6 O3 1.990(17) . ? 
Pd6 O55 1.991(16) . ? 
Pd6 O83 2.018(17) . ? 
Pd6 Pd9 3.232(3) . ? 
Pd6 K2 3.720(6) . ? 
Pd6 K11 3.996(7) . ? 
Pd7 O18 1.957(18) . ? 
Pd7 O57 2.015(19) . ? 
Pd7 O22 2.017(17) . ? 
Pd7 O4 2.019(17) . ? 
Pd7 Pd9 3.132(3) . ? 
Pd7 K2 3.942(6) . ? 
Pd8 O1 1.979(16) . ? 
Pd8 O53 1.986(17) . ? 
Pd8 O52 1.99(2) . ? 
Pd8 O117 2.016(19) . ? 
Pd8 K6 3.919(7) . ? 
Pd8 K2 3.972(6) . ? 
Pd9 O1 1.976(15) . ? 
Pd9 O18 1.988(17) . ? 
Pd9 O82 2.037(18) . ? 
Pd9 O76 2.044(18) . ? 
Pd9 K1 3.671(7) . ? 
Pd9 K2 3.777(6) . ? 
Pd10 O26 2.003(19) . ? 
Pd10 O91 2.005(18) . ? 
Pd10 O149 2.04(2) . ? 
Pd10 O111 2.07(2) . ? 
Pd10 K1 3.739(7) . ? 
Pd10 K3 3.782(7) . ? 
Se1 O31 1.691(19) . ? 
Se1 O28 1.696(19) . ? 
Se1 O148 1.736(18) . ? 
Se2 O141 1.72(2) . ? 
Se2 O165 1.74(2) . ? 
Se2 O137 1.768(18) . ? 
Se3 O69 1.699(18) . ? 
Se3 O43 1.727(19) . ? 
Se3 O13 1.757(16) . ? 
Se4 O178 1.67(2) . ? 
Se4 O166 1.696(17) . ? 
Se4 O179 1.720(19) . ? 
Se5 O100 1.70(3) . ? 
Se5 O193 1.73(2) . ? 
Se5 O201 1.734(18) . ? 
Se6 O75 1.710(17) . ? 
Se6 O169 1.723(18) . ? 
Se6 O135 1.73(2) . ? 
Se7 O52 1.68(2) . ? 
Se7 O82 1.684(18) . ? 
Se7 O64 1.71(2) . ? 
Se7 K6 3.937(8) . ? 
Se8 O111 1.67(2) . ? 
Se8 O177 1.70(2) . ? 
Se8 O125 1.73(2) . ? 
Se8 K9 3.857(10) . ? 
Se9 O50 1.69(2) . ? 
Se9 O149 1.69(2) . ? 
Se9 O128 1.74(2) . ? 
Se9 K5 3.865(9) . ? 
Se10 O22 1.675(17) . ? 
Se10 O83 1.691(19) . ? 
Se10 O76 1.695(18) . ? 
Se10 K8 3.646(9) . ? 
Se10 K11 3.881(8) . ? 
K1 O149 2.66(2) . ? 
K1 O76 2.68(2) . ? 
K1 O82 2.69(2) . ? 
K1 O111 2.75(2) . ? 
K1 O184 2.87(2) . ? 
K1 O147 2.89(2) . ? 
K1 O200 3.25(3) . ? 
K1 O153 3.36(3) . ? 
K1 O115 3.36(2) . ? 
K2 O18 2.701(18) . ? 
K2 O1 2.733(16) . ? 
K2 O212 2.77(2) . ? 
K2 O3 2.81(2) . ? 
K2 O21 2.82(2) . ? 
K2 O11 2.979(19) . ? 
K2 O7 2.981(19) . ? 
K2 O92 3.08(2) . ? 
K2 O39 3.11(2) . ? 
K2 O53 3.18(2) . ? 
K2 O4 3.19(2) . ? 
K3 O91 2.72(2) . ? 
K3 O26 2.72(2) . ? 
K3 O103 2.78(2) . ? 
K3 O120 2.86(2) . ? 
K3 O156 2.95(2) . ? 
K3 O8 3.07(2) . ? 
K3 O73 3.10(3) . ? 
K3 O132 3.16(2) . ? 
K3 O124 3.19(3) . ? 
K3 O123 3.22(2) . ? 
K4 O63 2.81(2) . ? 
K4 O63 2.81(2) 2_657 ? 
K4 O27 2.864(18) . ? 
K4 O27 2.864(18) 2_657 ? 
K4 O212 2.88(2) . ? 
K4 O212 2.88(2) 2_657 ? 
K4 O7 3.037(16) . ? 
K4 O7 3.038(16) 2_657 ? 
K4 W4' 3.74(5) 2_657 ? 
K4 W4 3.7783(17) 2_657 ? 
K5 O84 2.74(2) . ? 
K5 O211 2.78(3) . ? 
K5 O214 2.82(2) . ? 
K5 O128 2.83(2) . ? 
K5 O146 2.87(2) . ? 
K5 O114 3.01(3) . ? 
K5 O181 3.02(2) . ? 
K6 O52 2.71(2) . ? 
K6 O230 2.72(4) . ? 
K6 O211 2.74(3) . ? 
K6 O109 2.79(2) . ? 
K6 O23 2.91(2) 2_757 ? 
K6 O109 2.95(2) 2_757 ? 
K6 O117 3.20(2) . ? 
K6 W6 3.751(7) 2_757 ? 
K6 K6 4.364(16) 2_757 ? 
K7 O125 2.67(2) 2_766 ? 
K7 O220 2.71(2) . ? 
K7 O49 2.85(2) . ? 
K7 O51 2.86(2) 2_766 ? 
K7 O231 2.97(3) 2_766 ? 
K7 O221 3.03(3) . ? 
K7 O51 3.08(2) . ? 
K7 O161 3.11(2) . ? 
K7 O199 3.11(2) 2_766 ? 
K7 O216 3.12(3) 2_766 ? 
K7 W11 3.700(8) 2_766 ? 
K8 O94 2.79(2) . ? 
K8 O22 2.86(2) . ? 
K8 O189 3.02(3) . ? 
K8 O162 3.04(3) . ? 
K8 O215 3.05(4) . ? 
K8 K15 4.263(13) 1_455 ? 
K9 O175 2.69(2) . ? 
K9 O220 2.74(2) 2_766 ? 
K9 O177 2.96(2) . ? 
K9 O68 2.96(2) . ? 
K9 O80 2.98(2) . ? 
K9 O216 3.04(3) . ? 
K9 O118 3.38(2) . ? 
K9 K11 4.334(11) . ? 
K10 O121 2.70(3) . ? 
K10 O234 2.71(4) . ? 
K10 O42 2.85(2) . ? 
K10 O152 2.94(2) . ? 
K10 O77 3.08(2) 2_767 ? 
K10 O150 3.11(3) . ? 
K10 O105 3.12(2) . ? 
K10 K19 4.615(16) . ? 
K10 K14 4.794(16) . ? 
K11 O175 2.75(2) . ? 
K11 O83 2.811(19) . ? 
K11 O98 2.89(2) . ? 
K11 O216 2.89(3) . ? 
K11 O55 2.99(2) . ? 
K11 O119 3.02(2) . ? 
K11 O215 3.09(4) . ? 
K12 O142 2.73(3) . ? 
K12 O35 2.748(19) 2_756 ? 
K12 O190 2.79(3) 2_756 ? 
K12 O154 2.81(3) 2_756 ? 
K12 O78 2.82(3) . ? 
K12 O228 3.00(3) . ? 
K12 O74 3.17(2) . ? 
K12 W3' 3.78(5) 2_756 ? 
K12 W3 4.021(9) 2_756 ? 
K12 K16 4.224(14) 2_756 ? 
K13 O223 2.70(3) . ? 
K13 O222 2.72(3) . ? 
K13 O97 2.81(2) 2_667 ? 
K13 O29 2.83(2) . ? 
K13 O104 3.04(2) 2_657 ? 
K13 O65 3.17(2) . ? 
K13 O15 3.19(2) 2_657 ? 
K13 O2 3.19(2) 2_657 ? 
K13 K27 3.803(19) . ? 
K13 W34 3.932(10) 2_657 ? 
K13 W1 4.011(10) 2_657 ? 
K14 O213 2.57(3) . ? 
K14 O84 2.78(2) . ? 
K14 O214 2.81(2) . ? 
K14 O230 2.82(4) . ? 
K14 O121 2.91(2) . ? 
K14 O45 2.96(2) . ? 
K14 O64 3.02(2) . ? 
K14 O37 3.16(2) . ? 
K15 O102 2.87(2) . ? 
K15 O110 2.89(2) . ? 
K15 O112 2.91(3) . ? 
K15 O61 2.92(2) . ? 
K15 K8 4.263(13) 1_655 ? 
K16 O154 2.69(2) . ? 
K16 O35 2.84(2) . ? 
K16 O86 2.93(3) . ? 
K16 O233 3.06(3) 1_545 ? 
K16 O142 3.22(3) 2_756 ? 
K16 K21 4.02(3) 1_545 ? 
K16 K12 4.224(14) 2_756 ? 
K16 K21' 4.53(4) 1_545 ? 
K17 O236 2.68(3) 1_565 ? 
K17 O36 2.77(2) 1_565 ? 
K17 O34 2.79(3) 2_667 ? 
K17 O97 2.86(2) . ? 
K17 O222 2.89(3) 2_667 ? 
K17 O93 3.40(2) . ? 
K17 W36 4.114(11) 1_565 ? 
K17 K13 4.144(14) 2_667 ? 
K17 K27 4.644(19) . ? 
K18 O39 2.73(2) . ? 
K18 O29 2.74(2) . ? 
K18 O237 2.90(3) 1_455 ? 
K18 O15 2.96(2) 2_657 ? 
K19 O68 2.69(3) . ? 
K19 O152 2.77(3) . ? 
K19 O42 3.09(3) . ? 
K19 O126 3.18(2) . ? 
K19 O71 3.27(2) . ? 
K20 O92 2.75(2) 2_657 ? 
K20 O99 2.79(2) 2_657 ? 
K20 O60 2.82(2) . ? 
K20 O224 2.98(4) . ? 
K20 W4' 3.86(5) 2_657 ? 
K21 K21' 0.71(4) . ? 
K21 O81 2.77(4) 2_766 ? 
K21 O192 2.80(4) . ? 
K21 O233 2.81(4) . ? 
K21 O198 2.98(4) 1_565 ? 
K21 K16 4.02(3) 1_565 ? 
K21' O192 2.72(4) . ? 
K21' O198 2.81(5) 1_565 ? 
K21' O233 2.83(5) . ? 
K21' O81 2.87(4) 2_766 ? 
K21' K16 4.53(4) 1_565 ? 
K22 O124 2.79(3) . ? 
K22 O197 2.86(3) . ? 
K22 K25' 4.48(3) 2_866 ? 
K25 K25' 2.07(3) . ? 
K25 K25' 2.07(3) 2_866 ? 
K25 O163 2.83(2) 2_866 ? 
K25 O163 2.83(2) . ? 
K25 O156 3.06(2) . ? 
K25 O156 3.06(2) 2_866 ? 
K25 W25 3.6569(12) 2_866 ? 
K25 K3 4.816(7) 2_866 ? 
K25' O163 2.58(3) . ? 
K25' O197 2.72(3) 2_866 ? 
K25' O156 2.77(3) 2_866 ? 
K25' W27 3.44(2) 2_866 ? 
K25' K25' 4.13(5) 2_866 ? 
K25' K22 4.48(3) 2_866 ? 
K25' K3 4.58(3) 2_866 ? 
K25' K26 4.97(3) . ? 
K26 O227 2.85(4) . ? 
K26 O79 2.94(2) . ? 
K26 O10 2.98(3) . ? 
K26 O180 3.05(3) . ? 
K26 O67 3.08(3) . ? 
K27 O226 2.86(3) . ? 
K27 O54 2.90(3) . ? 
K27 O93 2.93(2) . ? 
K27 O88 2.93(3) . ? 
K27 O34 2.95(3) 2_667 ? 
K27 O65 2.96(3) . ? 
K27 O88 3.42(3) 2_667 ? 
K27 W9 3.912(17) 2_667 ? 
O2 K13 3.19(2) 2_657 ? 
O15 K18 2.96(2) 2_657 ? 
O15 K13 3.19(2) 2_657 ? 
O23 K6 2.91(2) 2_757 ? 
O34 K17 2.79(2) 2_667 ? 
O34 K27 2.95(3) 2_667 ? 
O35 K12 2.748(19) 2_756 ? 
O36 K17 2.77(2) 1_545 ? 
O51 K7 2.86(2) 2_766 ? 
O77 K10 3.08(2) 2_767 ? 
O81 K21 2.77(4) 2_766 ? 
O81 K21' 2.87(4) 2_766 ? 
O88 K27 3.42(3) 2_667 ? 
O92 K20 2.75(2) 2_657 ? 
O97 K13 2.81(2) 2_667 ? 
O99 K20 2.79(2) 2_657 ? 
O104 K13 3.04(2) 2_657 ? 
O109 K6 2.94(2) 2_757 ? 
O125 K7 2.67(2) 2_766 ? 
O142 K16 3.22(3) 2_756 ? 
O154 K12 2.81(3) 2_756 ? 
O156 K25' 2.77(3) 2_866 ? 
O190 K12 2.79(3) 2_756 ? 
O197 K25' 2.72(3) 2_866 ? 
O198 K21' 2.81(5) 1_545 ? 
O198 K21 2.98(4) 1_545 ? 
O199 K7 3.11(2) 2_766 ? 
O216 K7 3.12(3) 2_766 ? 
O220 K9 2.74(2) 2_766 ? 
O222 K17 2.89(3) 2_667 ? 
O231 K7 2.97(3) 2_766 ? 
O233 K16 3.06(3) 1_565 ? 
O236 K17 2.68(3) 1_545 ? 
O237 K18 2.90(3) 1_655 ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O15 W1 O66 98.5(8) . . ? 
O15 W1 O27 100.9(9) . . ? 
O66 W1 O27 88.7(8) . . ? 
O15 W1 O2 101.0(8) . . ? 
O66 W1 O2 88.3(8) . . ? 
O27 W1 O2 158.1(7) . . ? 
O15 W1 O89 97.5(8) . . ? 
O66 W1 O89 163.9(8) . . ? 
O27 W1 O89 88.4(9) . . ? 
O2 W1 O89 88.5(8) . . ? 
O15 W1 O31 173.0(8) . . ? 
O66 W1 O31 81.5(7) . . ? 
O27 W1 O31 72.1(7) . . ? 
O2 W1 O31 86.0(7) . . ? 
O89 W1 O31 82.6(7) . . ? 
O15 W1 K13 49.9(7) . 2_657 ? 
O66 W1 K13 89.6(6) . 2_657 ? 
O27 W1 K13 150.1(5) . 2_657 ? 
O2 W1 K13 51.5(5) . 2_657 ? 
O89 W1 K13 100.6(7) . 2_657 ? 
O31 W1 K13 137.0(5) . 2_657 ? 
O85 W2 O70 104.2(9) . . ? 
O85 W2 O90 95.9(9) . . ? 
O70 W2 O90 91.3(8) . . ? 
O85 W2 O62 98.3(9) . . ? 
O70 W2 O62 96.2(8) . . ? 
O90 W2 O62 161.8(7) . . ? 
O85 W2 O72 99.3(9) . . ? 
O70 W2 O72 156.2(8) . . ? 
O90 W2 O72 82.8(7) . . ? 
O62 W2 O72 83.7(7) . . ? 
O85 W2 O28 168.8(8) . . ? 
O70 W2 O28 86.8(7) . . ? 
O90 W2 O28 81.7(7) . . ? 
O62 W2 O28 82.2(7) . . ? 
O72 W2 O28 69.6(7) . . ? 
O70 W2' O90 105(3) . . ? 
O70 W2' O28 105(3) . . ? 
O90 W2' O28 97(2) . . ? 
O70 W2' O85 95(3) . . ? 
O90 W2' O85 88(2) . . ? 
O28 W2' O85 157(3) . . ? 
O70 W2' O72 171(3) . . ? 
O90 W2' O72 84(2) . . ? 
O28 W2' O72 74.5(19) . . ? 
O85 W2' O72 84.1(19) . . ? 
O70 W2' O62 95(3) . . ? 
O90 W2' O62 158(3) . . ? 
O28 W2' O62 86(2) . . ? 
O85 W2' O62 80.9(18) . . ? 
O72 W2' O62 76.4(18) . . ? 
O70 W2' Se1 77.6(19) . . ? 
O90 W2' Se1 89.8(19) . . ? 
O28 W2' Se1 31.8(9) . . ? 
O85 W2' Se1 171(2) . . ? 
O72 W2' Se1 104.3(19) . . ? 
O62 W2' Se1 104(2) . . ? 
O35 W3' O62 116(3) . . ? 
O35 W3' O46 118(3) . . ? 
O62 W3' O46 90(2) . . ? 
O35 W3' O9 106(3) . . ? 
O62 W3' O9 88(2) . . ? 
O46 W3' O9 132(2) . . ? 
O35 W3' O158 97(3) . . ? 
O62 W3' O158 146(2) . . ? 
O46 W3' O158 79.9(19) . . ? 
O9 W3' O158 76.2(17) . . ? 
O35 W3' K12 32.6(18) . 2_756 ? 
O62 W3' K12 145(2) . 2_756 ? 
O46 W3' K12 116.1(19) . 2_756 ? 
O9 W3' K12 90.5(16) . 2_756 ? 
O158 W3' K12 65.8(13) . 2_756 ? 
O35 W3' K16 35.3(17) . . ? 
O62 W3' K16 81.0(16) . . ? 
O46 W3' K16 116.3(18) . . ? 
O9 W3' K16 110.3(17) . . ? 
O158 W3' K16 132.7(19) . . ? 
K12 W3' K16 67.4(8) 2_756 . ? 
O35 W3 O62 100.1(8) . . ? 
O35 W3 O9 102.9(8) . . ? 
O62 W3 O9 96.3(8) . . ? 
O35 W3 O46 101.0(8) . . ? 
O62 W3 O46 90.3(8) . . ? 
O9 W3 O46 153.6(8) . . ? 
O35 W3 O158 91.2(9) . . ? 
O62 W3 O158 167.8(8) . . ? 
O9 W3 O158 85.5(8) . . ? 
O46 W3 O158 83.1(8) . . ? 
O35 W3 O69 170.3(7) . . ? 
O62 W3 O69 85.9(7) . . ? 
O9 W3 O69 83.8(7) . . ? 
O46 W3 O69 71.2(7) . . ? 
O158 W3 O69 82.3(8) . . ? 
O35 W3 K12 33.2(6) . 2_756 ? 
O62 W3 K12 131.5(6) . 2_756 ? 
O9 W3 K12 87.4(5) . 2_756 ? 
O46 W3 K12 107.2(6) . 2_756 ? 
O158 W3 K12 60.5(6) . 2_756 ? 
O69 W3 K12 142.3(5) . 2_756 ? 
O92 W4 O53 101.8(10) . . ? 
O92 W4 O7 97.1(8) . . ? 
O53 W4 O7 95.9(8) . . ? 
O92 W4 O143 93.7(8) . . ? 
O53 W4 O143 90.2(8) . . ? 
O7 W4 O143 166.2(8) . . ? 
O92 W4 O27 98.9(9) . . ? 
O53 W4 O27 158.2(8) . . ? 
O7 W4 O27 88.3(8) . . ? 
O143 W4 O27 81.7(7) . . ? 
O92 W4 O31 169.7(9) . . ? 
O53 W4 O31 87.0(8) . . ? 
O7 W4 O31 87.2(7) . . ? 
O143 W4 O31 80.7(7) . . ? 
O27 W4 O31 71.8(7) . . ? 
O92 W4 K2 60.9(7) . . ? 
O53 W4 K2 64.0(6) . . ? 
O7 W4 K2 57.6(6) . . ? 
O143 W4 K2 135.9(5) . . ? 
O27 W4 K2 134.0(5) . . ? 
O31 W4 K2 128.8(5) . . ? 
O92 W4 K4 73.4(6) . . ? 
O53 W4 K4 146.1(6) . . ? 
O7 W4 K4 52.9(5) . . ? 
O143 W4 K4 123.3(5) . . ? 
O27 W4 K4 48.3(5) . . ? 
O31 W4 K4 102.2(5) . . ? 
K2 W4 K4 85.65(10) . . ? 
O92 W4' O143 111(3) . . ? 
O92 W4' O53 111(3) . . ? 
O143 W4' O53 88(2) . . ? 
O92 W4' O27 111(3) . . ? 
O143 W4' O27 82(2) . . ? 
O53 W4' O27 138(3) . . ? 
O92 W4' O7 101(3) . . ? 
O143 W4' O7 147(3) . . ? 
O53 W4' O7 85(2) . . ? 
O27 W4' O7 81.6(19) . . ? 
O92 W4' K2 62(2) . . ? 
O143 W4' K2 143(2) . . ? 
O53 W4' K2 64.8(16) . . ? 
O27 W4' K2 134(2) . . ? 
O7 W4' K2 58.4(14) . . ? 
O92 W4' K4 77(2) . . ? 
O143 W4' K4 128(2) . . ? 
O53 W4' K4 139(2) . . ? 
O27 W4' K4 49.5(13) . . ? 
O7 W4' K4 54.3(13) . . ? 
K2 W4' K4 86.9(12) . . ? 
O92 W4' K20 29.1(17) . 2_657 ? 
O143 W4' K20 82.7(15) . 2_657 ? 
O53 W4' K20 116(2) . 2_657 ? 
O27 W4' K20 103.7(17) . 2_657 ? 
O7 W4' K20 129(2) . 2_657 ? 
K2 W4' K20 87.8(11) . 2_657 ? 
K4 W4' K20 90.6(11) . 2_657 ? 
O39 W5 O4 104.9(10) . . ? 
O39 W5 O7 97.1(9) . . ? 
O4 W5 O7 93.2(7) . . ? 
O39 W5 O6 95.5(8) . . ? 
O4 W5 O6 93.7(8) . . ? 
O7 W5 O6 163.5(7) . . ? 
O39 W5 O63 97.7(9) . . ? 
O4 W5 O63 157.4(8) . . ? 
O7 W5 O63 84.9(8) . . ? 
O6 W5 O63 83.0(8) . . ? 
O39 W5 O43 168.5(9) . . ? 
O4 W5 O43 86.3(8) . . ? 
O7 W5 O43 84.9(7) . . ? 
O6 W5 O43 80.7(6) . . ? 
O63 W5 O43 71.2(7) . . ? 
O39 W5 K2 61.5(7) . . ? 
O4 W5 K2 64.0(6) . . ? 
O7 W5 K2 57.3(6) . . ? 
O6 W5 K2 138.9(5) . . ? 
O63 W5 K2 130.6(6) . . ? 
O43 W5 K2 127.7(5) . . ? 
O39 W5 K4 73.2(7) . . ? 
O4 W5 K4 143.4(6) . . ? 
O7 W5 K4 51.9(5) . . ? 
O6 W5 K4 122.9(5) . . ? 
O63 W5 K4 45.8(6) . . ? 
O43 W5 K4 99.6(5) . . ? 
K2 W5 K4 84.87(10) . . ? 
O109 W6 O117 104.7(9) . . ? 
O109 W6 O122 102.8(9) . . ? 
O117 W6 O122 93.4(10) . . ? 
O109 W6 O23 98.3(9) . . ? 
O117 W6 O23 93.1(9) . . ? 
O122 W6 O23 155.5(8) . . ? 
O109 W6 O5 94.6(8) . . ? 
O117 W6 O5 160.7(8) . . ? 
O122 W6 O5 83.2(8) . . ? 
O23 W6 O5 82.9(8) . . ? 
O109 W6 O148 163.9(8) . . ? 
O117 W6 O148 88.9(8) . . ? 
O122 W6 O148 84.5(7) . . ? 
O23 W6 O148 72.0(7) . . ? 
O5 W6 O148 71.9(7) . . ? 
O109 W6 K6 45.4(6) . . ? 
O117 W6 K6 59.3(7) . . ? 
O122 W6 K6 105.9(6) . . ? 
O23 W6 K6 97.7(6) . . ? 
O5 W6 K6 139.8(5) . . ? 
O148 W6 K6 146.6(5) . . ? 
O109 W6 K6 49.6(7) . 2_757 ? 
O117 W6 K6 112.8(7) . 2_757 ? 
O122 W6 K6 145.0(6) . 2_757 ? 
O23 W6 K6 50.0(6) . 2_757 ? 
O5 W6 K6 78.9(6) . 2_757 ? 
O148 W6 K6 117.4(4) . 2_757 ? 
K6 W6 K6 71.6(2) . 2_757 ? 
O139 W7 O55 103.5(9) . . ? 
O139 W7 O54 101.9(9) . . ? 
O55 W7 O54 90.7(8) . . ? 
O139 W7 O119 100.1(9) . . ? 
O55 W7 O119 94.3(9) . . ? 
O54 W7 O119 155.7(8) . . ? 
O139 W7 O93 97.6(8) . . ? 
O55 W7 O93 158.9(8) . . ? 
O54 W7 O93 83.6(8) . . ? 
O119 W7 O93 83.3(8) . . ? 
O139 W7 O178 168.4(9) . . ? 
O55 W7 O178 86.4(8) . . ? 
O54 W7 O178 83.7(7) . . ? 
O119 W7 O178 72.9(7) . . ? 
O93 W7 O178 72.8(7) . . ? 
O139 W7 K11 87.9(7) . . ? 
O55 W7 K11 49.2(6) . . ? 
O54 W7 K11 139.8(6) . . ? 
O119 W7 K11 51.1(7) . . ? 
O93 W7 K11 134.2(5) . . ? 
O178 W7 K11 94.3(5) . . ? 
O139 W7 K27 82.4(7) . . ? 
O55 W7 K27 135.0(6) . . ? 
O54 W7 K27 45.1(6) . . ? 
O119 W7 K27 129.1(7) . . ? 
O93 W7 K27 46.5(6) . . ? 
O178 W7 K27 94.9(5) . . ? 
K11 W7 K27 170.2(3) . . ? 
O60 W8 O89 99.5(9) . . ? 
O60 W8 O63 100.9(8) . . ? 
O89 W8 O63 90.1(9) . . ? 
O60 W8 O151 96.8(9) . . ? 
O89 W8 O151 163.7(8) . . ? 
O63 W8 O151 88.0(9) . . ? 
O60 W8 O32 99.4(8) . . ? 
O89 W8 O32 89.4(8) . . ? 
O63 W8 O32 159.5(7) . . ? 
O151 W8 O32 86.8(8) . . ? 
O60 W8 O43 172.6(8) . . ? 
O89 W8 O43 83.1(7) . . ? 
O63 W8 O43 72.1(7) . . ? 
O151 W8 O43 80.8(8) . . ? 
O32 W8 O43 87.5(7) . . ? 
O60 W8 K4 83.5(7) . . ? 
O89 W8 K4 60.7(6) . . ? 
O63 W8 K4 37.4(6) . . ? 
O151 W8 K4 122.9(6) . . ? 
O32 W8 K4 149.8(6) . . ? 
O43 W8 K4 91.9(5) . . ? 
O60 W8 K20 32.7(7) . . ? 
O89 W8 K20 125.2(6) . . ? 
O63 W8 K20 80.9(6) . . ? 
O151 W8 K20 70.5(6) . . ? 
O32 W8 K20 115.7(5) . . ? 
O43 W8 K20 141.1(5) . . ? 
K4 W8 K20 82.64(16) . . ? 
O34 W9 O65 103.3(10) . . ? 
O34 W9 O12 102.7(10) . . ? 
O65 W9 O12 153.8(8) . . ? 
O34 W9 O130 101.3(9) . . ? 
O65 W9 O130 89.9(9) . . ? 
O12 W9 O130 88.5(9) . . ? 
O34 W9 O88 103.9(9) . . ? 
O65 W9 O88 85.4(8) . . ? 
O12 W9 O88 85.0(9) . . ? 
O130 W9 O88 154.8(8) . . ? 
O34 W9 K27 87.3(8) . . ? 
O65 W9 K27 47.1(6) . . ? 
O12 W9 K27 131.2(7) . . ? 
O130 W9 K27 136.8(7) . . ? 
O88 W9 K27 46.5(7) . . ? 
O34 W9 K27 44.5(7) . 2_667 ? 
O65 W9 K27 108.8(6) . 2_667 ? 
O12 W9 K27 87.5(7) . 2_667 ? 
O130 W9 K27 143.1(6) . 2_667 ? 
O88 W9 K27 61.0(6) . 2_667 ? 
K27 W9 K27 66.6(4) . 2_667 ? 
O94 W10 O57 105.0(9) . . ? 
O94 W10 O196 101.0(10) . . ? 
O57 W10 O196 93.3(8) . . ? 
O94 W10 O14 101.2(10) . . ? 
O57 W10 O14 92.6(9) . . ? 
O196 W10 O14 154.7(8) . . ? 
O94 W10 O171 96.7(10) . . ? 
O57 W10 O171 158.2(9) . . ? 
O196 W10 O171 79.6(9) . . ? 
O14 W10 O171 85.8(10) . . ? 
O94 W10 O13 165.2(8) . . ? 
O57 W10 O13 88.6(7) . . ? 
O196 W10 O13 83.8(7) . . ? 
O14 W10 O13 71.8(7) . . ? 
O171 W10 O13 70.2(7) . . ? 
O94 W10 K8 37.1(7) . . ? 
O57 W10 K8 69.3(6) . . ? 
O196 W10 K8 92.8(6) . . ? 
O14 W10 K8 112.2(6) . . ? 
O171 W10 K8 131.2(6) . . ? 
O13 W10 K8 157.5(4) . . ? 
O51 W11 O199 104.3(10) . . ? 
O51 W11 O17 102.5(9) . . ? 
O199 W11 O17 92.5(9) . . ? 
O51 W11 O49 98.0(9) . . ? 
O199 W11 O49 92.7(8) . . ? 
O17 W11 O49 156.9(8) . . ? 
O51 W11 O161 95.0(9) . . ? 
O199 W11 O161 160.5(9) . . ? 
O17 W11 O161 85.7(8) . . ? 
O49 W11 O161 82.0(8) . . ? 
O51 W11 O137 164.1(8) . . ? 
O199 W11 O137 88.4(9) . . ? 
O17 W11 O137 86.2(7) . . ? 
O49 W11 O137 71.5(7) . . ? 
O161 W11 O137 72.1(7) . . ? 
O51 W11 K7 58.2(7) . . ? 
O199 W11 K7 130.4(7) . . ? 
O17 W11 K7 134.5(6) . . ? 
O49 W11 K7 51.5(6) . . ? 
O161 W11 K7 59.0(6) . . ? 
O137 W11 K7 106.3(5) . . ? 
O51 W11 K7 48.1(7) . 2_766 ? 
O199 W11 K7 57.1(7) . 2_766 ? 
O17 W11 K7 110.5(6) . 2_766 ? 
O49 W11 K7 91.2(6) . 2_766 ? 
O161 W11 K7 141.3(6) . 2_766 ? 
O137 W11 K7 141.1(5) . 2_766 ? 
K7 W11 K7 87.09(18) . 2_766 ? 
O187 W12 O171 101.1(10) . . ? 
O187 W12 O158 103.5(10) . . ? 
O171 W12 O158 92.1(10) . . ? 
O187 W12 O20 101.5(9) . . ? 
O171 W12 O20 156.9(8) . . ? 
O158 W12 O20 87.4(8) . . ? 
O187 W12 O48 100.9(8) . . ? 
O171 W12 O48 91.5(10) . . ? 
O158 W12 O48 154.2(9) . . ? 
O20 W12 O48 79.5(8) . . ? 
O187 W12 O13 169.9(8) . . ? 
O171 W12 O13 73.5(7) . . ? 
O158 W12 O13 85.5(8) . . ? 
O20 W12 O13 83.4(7) . . ? 
O48 W12 O13 71.1(6) . . ? 
O150 W13 O146 104.3(9) . . ? 
O150 W13 O105 103.1(10) . . ? 
O146 W13 O105 90.0(9) . . ? 
O150 W13 O56 100.6(9) . . ? 
O146 W13 O56 154.8(9) . . ? 
O105 W13 O56 87.6(10) . . ? 
O150 W13 O181 100.7(10) . . ? 
O146 W13 O181 87.4(9) . . ? 
O105 W13 O181 156.0(8) . . ? 
O56 W13 O181 84.8(10) . . ? 
O150 W13 O75 168.8(9) . . ? 
O146 W13 O75 82.3(7) . . ? 
O105 W13 O75 85.8(8) . . ? 
O56 W13 O75 72.6(8) . . ? 
O181 W13 O75 70.3(7) . . ? 
O150 W13 K5 85.6(8) . . ? 
O146 W13 K5 45.2(6) . . ? 
O105 W13 K5 134.6(6) . . ? 
O56 W13 K5 135.2(8) . . ? 
O181 W13 K5 50.6(6) . . ? 
O75 W13 K5 93.1(6) . . ? 
O150 W13 K10 51.7(8) . . ? 
O146 W13 K10 90.4(6) . . ? 
O105 W13 K10 53.1(6) . . ? 
O56 W13 K10 107.8(7) . . ? 
O181 W13 K10 150.7(6) . . ? 
O75 W13 K10 138.3(5) . . ? 
K5 W13 K10 110.5(2) . . ? 
O99 W14 O21 102.8(9) . . ? 
O99 W14 O11 101.2(8) . . ? 
O21 W14 O11 94.4(8) . . ? 
O99 W14 O40 103.5(8) . . ? 
O21 W14 O40 89.6(8) . . ? 
O11 W14 O40 153.5(7) . . ? 
O99 W14 O130 95.7(9) . . ? 
O21 W14 O130 161.4(8) . . ? 
O11 W14 O130 83.8(8) . . ? 
O40 W14 O130 84.1(8) . . ? 
O99 W14 O166 166.6(8) . . ? 
O21 W14 O166 88.8(8) . . ? 
O11 W14 O166 71.0(6) . . ? 
O40 W14 O166 82.9(7) . . ? 
O130 W14 O166 73.0(7) . . ? 
O99 W14 K2 91.6(7) . . ? 
O21 W14 K2 46.3(6) . . ? 
O11 W14 K2 52.3(6) . . ? 
O40 W14 K2 135.8(5) . . ? 
O130 W14 K2 136.1(6) . . ? 
O166 W14 K2 91.8(4) . . ? 
O132 W15 O8 102.2(11) . . ? 
O132 W15 O73 98.0(10) . . ? 
O8 W15 O73 94.6(9) . . ? 
O132 W15 O173 94.2(9) . . ? 
O8 W15 O173 91.3(9) . . ? 
O73 W15 O173 165.0(10) . . ? 
O132 W15 O191 99.3(10) . . ? 
O8 W15 O191 158.1(9) . . ? 
O73 W15 O191 86.2(10) . . ? 
O173 W15 O191 83.2(9) . . ? 
O132 W15 O165 169.2(10) . . ? 
O8 W15 O165 88.1(9) . . ? 
O73 W15 O165 83.7(9) . . ? 
O173 W15 O165 82.7(9) . . ? 
O191 W15 O165 70.2(8) . . ? 
O132 W15 K3 62.6(8) . . ? 
O8 W15 K3 59.4(6) . . ? 
O73 W15 K3 60.6(8) . . ? 
O173 W15 K3 133.7(7) . . ? 
O191 W15 K3 136.7(6) . . ? 
O165 W15 K3 126.5(6) . . ? 
O97 W16 O93 101.3(9) . . ? 
O97 W16 O88 103.8(10) . . ? 
O93 W16 O88 88.6(8) . . ? 
O97 W16 O33 100.9(10) . . ? 
O93 W16 O33 87.1(8) . . ? 
O88 W16 O33 155.3(9) . . ? 
O97 W16 O172 104.2(9) . . ? 
O93 W16 O172 154.5(8) . . ? 
O88 W16 O172 87.0(8) . . ? 
O33 W16 O172 86.5(8) . . ? 
O97 W16 O178 169.7(9) . . ? 
O93 W16 O178 71.6(7) . . ? 
O88 W16 O178 83.8(7) . . ? 
O33 W16 O178 71.7(8) . . ? 
O172 W16 O178 82.9(8) . . ? 
O97 W16 K27 84.9(7) . . ? 
O93 W16 K27 48.6(6) . . ? 
O88 W16 K27 48.8(7) . . ? 
O33 W16 K27 135.3(7) . . ? 
O172 W16 K27 135.4(6) . . ? 
O178 W16 K27 95.3(5) . . ? 
O97 W16 K17 43.9(8) . . ? 
O93 W16 K17 62.5(6) . . ? 
O88 W16 K17 119.8(6) . . ? 
O33 W16 K17 79.2(6) . . ? 
O172 W16 K17 139.7(6) . . ? 
O178 W16 K17 126.2(5) . . ? 
K27 W16 K17 75.0(3) . . ? 
O42 W17 O127 103.6(9) . . ? 
O42 W17 O37 103.3(9) . . ? 
O127 W17 O37 95.6(8) . . ? 
O42 W17 O71 100.6(9) . . ? 
O127 W17 O71 87.6(9) . . ? 
O37 W17 O71 154.4(8) . . ? 
O42 W17 O24 100.1(9) . . ? 
O127 W17 O24 155.5(8) . . ? 
O37 W17 O24 84.8(8) . . ? 
O71 W17 O24 82.0(8) . . ? 
O42 W17 O179 169.5(8) . . ? 
O127 W17 O179 85.6(8) . . ? 
O37 W17 O179 70.4(7) . . ? 
O71 W17 O179 84.7(8) . . ? 
O24 W17 O179 71.4(7) . . ? 
O42 W17 K19 48.1(7) . . ? 
O127 W17 K19 85.8(7) . . ? 
O37 W17 K19 150.3(6) . . ? 
O71 W17 K19 55.2(6) . . ? 
O24 W17 K19 105.9(6) . . ? 
O179 W17 K19 139.2(5) . . ? 
O113 W18 O167 102.5(9) . . ? 
O113 W18 O49 100.5(9) . . ? 
O167 W18 O49 156.0(8) . . ? 
O113 W18 O173 101.8(9) . . ? 
O167 W18 O173 89.2(10) . . ? 
O49 W18 O173 92.5(9) . . ? 
O113 W18 O107 100.8(9) . . ? 
O167 W18 O107 84.4(10) . . ? 
O49 W18 O107 84.9(9) . . ? 
O173 W18 O107 157.3(9) . . ? 
O113 W18 O137 169.9(8) . . ? 
O167 W18 O137 84.9(8) . . ? 
O49 W18 O137 71.5(8) . . ? 
O173 W18 O137 85.0(8) . . ? 
O107 W18 O137 72.8(7) . . ? 
O152 W19 O41 103.5(9) . . ? 
O152 W19 O118 104.0(9) . . ? 
O41 W19 O118 94.8(8) . . ? 
O152 W19 O105 100.0(10) . . ? 
O41 W19 O105 89.3(9) . . ? 
O118 W19 O105 153.9(8) . . ? 
O152 W19 O138 99.4(9) . . ? 
O41 W19 O138 156.4(8) . . ? 
O118 W19 O138 84.9(8) . . ? 
O105 W19 O138 81.3(9) . . ? 
O152 W19 O135 169.4(9) . . ? 
O41 W19 O135 86.4(7) . . ? 
O118 W19 O135 70.9(7) . . ? 
O105 W19 O135 83.7(8) . . ? 
O138 W19 O135 71.2(7) . . ? 
O152 W19 K10 47.5(8) . . ? 
O41 W19 K10 88.4(6) . . ? 
O118 W19 K10 150.9(6) . . ? 
O105 W19 K10 54.7(6) . . ? 
O138 W19 K10 103.3(6) . . ? 
O135 W19 K10 138.2(5) . . ? 
O126 W20 O98 104.2(9) . . ? 
O126 W20 O71 102.0(9) . . ? 
O98 W20 O71 89.2(9) . . ? 
O126 W20 O119 99.9(8) . . ? 
O98 W20 O119 88.5(8) . . ? 
O71 W20 O119 157.8(8) . . ? 
O126 W20 O33 99.7(9) . . ? 
O98 W20 O33 155.9(9) . . ? 
O71 W20 O33 88.9(9) . . ? 
O119 W20 O33 84.4(9) . . ? 
O126 W20 O178 169.4(8) . . ? 
O98 W20 O178 82.5(8) . . ? 
O71 W20 O178 86.1(8) . . ? 
O119 W20 O178 71.7(7) . . ? 
O33 W20 O178 73.4(8) . . ? 
O126 W20 K11 86.7(7) . . ? 
O98 W20 K11 45.4(6) . . ? 
O71 W20 K11 134.2(7) . . ? 
O119 W20 K11 50.2(7) . . ? 
O33 W20 K11 134.5(6) . . ? 
O178 W20 K11 92.5(4) . . ? 
O126 W20 K19 50.3(7) . . ? 
O98 W20 K19 87.8(6) . . ? 
O71 W20 K19 54.2(7) . . ? 
O119 W20 K19 147.6(6) . . ? 
O33 W20 K19 110.3(7) . . ? 
O178 W20 K19 139.4(5) . . ? 
K11 W20 K19 108.1(2) . . ? 
O29 W21 O3 102.6(9) . . ? 
O29 W21 O54 102.0(9) . . ? 
O3 W21 O54 91.4(8) . . ? 
O29 W21 O11 102.7(8) . . ? 
O3 W21 O11 93.2(8) . . ? 
O54 W21 O11 153.2(7) . . ? 
O29 W21 O65 94.6(9) . . ? 
O3 W21 O65 162.6(8) . . ? 
O54 W21 O65 82.8(8) . . ? 
O11 W21 O65 85.0(8) . . ? 
O29 W21 O166 166.4(8) . . ? 
O3 W21 O166 90.1(7) . . ? 
O54 W21 O166 82.3(6) . . ? 
O11 W21 O166 71.4(6) . . ? 
O65 W21 O166 72.9(7) . . ? 
O29 W21 K2 94.2(7) . . ? 
O3 W21 K2 45.2(6) . . ? 
O54 W21 K2 136.3(6) . . ? 
O11 W21 K2 51.3(5) . . ? 
O65 W21 K2 136.3(6) . . ? 
O166 W21 K2 91.4(4) . . ? 
O29 W21 K13 40.7(7) . . ? 
O3 W21 K13 143.0(6) . . ? 
O54 W21 K13 100.2(6) . . ? 
O11 W21 K13 91.8(5) . . ? 
O65 W21 K13 54.4(5) . . ? 
O166 W21 K13 126.0(4) . . ? 
K2 W21 K13 117.71(18) . . ? 
O29 W21 K27 79.3(8) . . ? 
O3 W21 K27 134.1(6) . . ? 
O54 W21 K27 44.8(6) . . ? 
O11 W21 K27 131.7(6) . . ? 
O65 W21 K27 47.1(6) . . ? 
O166 W21 K27 95.4(5) . . ? 
K2 W21 K27 173.3(3) . . ? 
K13 W21 K27 58.2(3) . . ? 
O29 W21 K18 27.3(7) . . ? 
O3 W21 K18 75.3(6) . . ? 
O54 W21 K18 104.0(5) . . ? 
O11 W21 K18 102.6(5) . . ? 
O65 W21 K18 122.0(6) . . ? 
O166 W21 K18 164.1(4) . . ? 
K2 W21 K18 73.94(16) . . ? 
K13 W21 K18 67.8(2) . . ? 
K27 W21 K18 99.3(3) . . ? 
O154 W22 O95 98.2(11) . . ? 
O154 W22 O159 105.8(10) . . ? 
O95 W22 O159 95.3(10) . . ? 
O154 W22 O25 99.8(10) . . ? 
O95 W22 O25 92.3(9) . . ? 
O159 W22 O25 151.8(9) . . ? 
O154 W22 O164 93.5(10) . . ? 
O95 W22 O164 167.6(9) . . ? 
O159 W22 O164 85.5(10) . . ? 
O25 W22 O164 81.5(9) . . ? 
O154 W22 O100 170.4(10) . . ? 
O95 W22 O100 85.7(9) . . ? 
O159 W22 O100 82.4(9) . . ? 
O25 W22 O100 71.2(9) . . ? 
O164 W22 O100 82.1(9) . . ? 
O154 W22 K16 33.8(9) . . ? 
O95 W22 K16 131.0(7) . . ? 
O159 W22 K16 92.2(6) . . ? 
O25 W22 K16 103.1(6) . . ? 
O164 W22 K16 61.3(6) . . ? 
O100 W22 K16 143.3(6) . . ? 
O124 W23 O123 103.3(12) . . ? 
O124 W23 O188 96.5(10) . . ? 
O123 W23 O188 92.3(10) . . ? 
O124 W23 O73 96.7(10) . . ? 
O123 W23 O73 94.3(10) . . ? 
O188 W23 O73 163.4(11) . . ? 
O124 W23 O206 100.4(11) . . ? 
O123 W23 O206 156.3(10) . . ? 
O188 W23 O206 83.4(10) . . ? 
O73 W23 O206 84.4(10) . . ? 
O124 W23 O201 169.2(10) . . ? 
O123 W23 O201 87.4(9) . . ? 
O188 W23 O201 81.0(9) . . ? 
O73 W23 O201 84.1(9) . . ? 
O206 W23 O201 69.0(8) . . ? 
O124 W23 K3 61.2(9) . . ? 
O123 W23 K3 62.3(7) . . ? 
O188 W23 K3 137.5(8) . . ? 
O73 W23 K3 58.5(8) . . ? 
O206 W23 K3 133.2(7) . . ? 
O201 W23 K3 127.0(5) . . ? 
O153 W24' O168 94.2(17) . . ? 
O153 W24' O9 90.1(16) . . ? 
O168 W24' O9 174.0(18) . . ? 
O153 W24' O196 174.3(18) . . ? 
O168 W24' O196 89.3(15) . . ? 
O9 W24' O196 86.1(14) . . ? 
O153 W24' O184 93.3(15) . . ? 
O168 W24' O184 90.2(15) . . ? 
O9 W24' O184 93.7(14) . . ? 
O196 W24' O184 91.2(14) . . ? 
O153 W24' O190 89.6(15) . . ? 
O168 W24' O190 90.7(14) . . ? 
O9 W24' O190 85.1(13) . . ? 
O196 W24' O190 85.8(13) . . ? 
O184 W24' O190 176.8(18) . . ? 
O153 W24' K1 58.8(11) . . ? 
O168 W24' K1 67.5(10) . . ? 
O9 W24' K1 118.4(11) . . ? 
O196 W24' K1 126.9(12) . . ? 
O184 W24' K1 44.8(8) . . ? 
O190 W24' K1 138.3(13) . . ? 
O190 W24 O168 104.3(11) . . ? 
O190 W24 O153 100.1(11) . . ? 
O168 W24 O153 89.3(10) . . ? 
O190 W24 O196 100.9(10) . . ? 
O168 W24 O196 89.9(9) . . ? 
O153 W24 O196 158.6(9) . . ? 
O190 W24 O9 97.0(10) . . ? 
O168 W24 O9 158.7(9) . . ? 
O153 W24 O9 86.1(9) . . ? 
O196 W24 O9 86.9(8) . . ? 
O190 W24 O184 177.5(11) . . ? 
O168 W24 O184 77.4(9) . . ? 
O153 W24 O184 78.2(9) . . ? 
O196 W24 O184 80.8(8) . . ? 
O9 W24 O184 81.2(8) . . ? 
O163 W25 O120 103.6(9) . . ? 
O163 W25 O79 103.7(10) . . ? 
O120 W25 O79 90.6(8) . . ? 
O163 W25 O156 100.0(10) . . ? 
O120 W25 O156 93.3(9) . . ? 
O79 W25 O156 154.4(9) . . ? 
O163 W25 O10 96.9(9) . . ? 
O120 W25 O10 159.4(9) . . ? 
O79 W25 O10 82.9(8) . . ? 
O156 W25 O10 84.7(9) . . ? 
O163 W25 O169 166.0(8) . . ? 
O120 W25 O169 87.3(8) . . ? 
O79 W25 O169 84.6(8) . . ? 
O156 W25 O169 70.3(8) . . ? 
O10 W25 O169 72.6(8) . . ? 
O163 W25 K25 48.7(8) . . ? 
O120 W25 K25 123.4(7) . . ? 
O79 W25 K25 137.9(5) . . ? 
O156 W25 K25 56.9(6) . . ? 
O10 W25 K25 72.2(6) . . ? 
O169 W25 K25 117.8(5) . . ? 
O163 W25 K3 91.0(8) . . ? 
O120 W25 K3 47.1(7) . . ? 
O79 W25 K3 137.6(5) . . ? 
O156 W25 K3 50.5(7) . . ? 
O10 W25 K3 135.2(6) . . ? 
O169 W25 K3 90.2(5) . . ? 
K25 W25 K3 80.82(11) . . ? 
O163 W25 K26 79.8(8) . . ? 
O120 W25 K26 134.4(7) . . ? 
O79 W25 K26 45.9(6) . . ? 
O156 W25 K26 131.5(7) . . ? 
O10 W25 K26 47.9(6) . . ? 
O169 W25 K26 98.9(6) . . ? 
K25 W25 K26 93.4(3) . . ? 
K3 W25 K26 170.7(3) . . ? 
O163 W25 K25' 21.7(8) . . ? 
O120 W25 K25' 121.6(7) . . ? 
O79 W25 K25' 112.9(7) . . ? 
O156 W25 K25' 86.4(7) . . ? 
O10 W25 K25' 78.8(7) . . ? 
O169 W25 K25' 144.3(6) . . ? 
K25 W25 K25' 30.2(4) . . ? 
K3 W25 K25' 95.4(4) . . ? 
K26 W25 K25' 76.2(5) . . ? 
O38 W26 O23 101.2(9) . . ? 
O38 W26 O143 103.4(9) . . ? 
O23 W26 O143 93.6(8) . . ? 
O38 W26 O47 101.0(9) . . ? 
O23 W26 O47 86.0(8) . . ? 
O143 W26 O47 155.2(8) . . ? 
O38 W26 O66 101.2(8) . . ? 
O23 W26 O66 156.8(8) . . ? 
O143 W26 O66 86.9(8) . . ? 
O47 W26 O66 84.0(8) . . ? 
O38 W26 O148 171.6(8) . . ? 
O23 W26 O148 72.4(7) . . ? 
O143 W26 O148 82.8(7) . . ? 
O47 W26 O148 73.4(7) . . ? 
O66 W26 O148 84.6(7) . . ? 
O197 W27 O103 104.3(11) . . ? 
O197 W27 O102 104.2(10) . . ? 
O103 W27 O102 90.8(9) . . ? 
O197 W27 O156 100.0(10) . . ? 
O103 W27 O156 92.3(9) . . ? 
O102 W27 O156 154.0(10) . . ? 
O197 W27 O61 95.2(10) . . ? 
O103 W27 O61 160.5(9) . . ? 
O102 W27 O61 83.6(9) . . ? 
O156 W27 O61 84.9(9) . . ? 
O197 W27 O169 165.0(9) . . ? 
O103 W27 O169 88.5(9) . . ? 
O102 W27 O169 83.1(8) . . ? 
O156 W27 O169 71.2(8) . . ? 
O61 W27 O169 72.4(7) . . ? 
O197 W27 K25' 50.9(9) . 2_866 ? 
O103 W27 K25' 120.6(8) . 2_866 ? 
O102 W27 K25' 142.1(7) . 2_866 ? 
O156 W27 K25' 53.5(8) . 2_866 ? 
O61 W27 K25' 72.7(7) . 2_866 ? 
O169 W27 K25' 115.8(6) . 2_866 ? 
O197 W27 K3 92.3(8) . . ? 
O103 W27 K3 45.2(6) . . ? 
O102 W27 K3 135.8(6) . . ? 
O156 W27 K3 51.1(7) . . ? 
O61 W27 K3 136.0(6) . . ? 
O169 W27 K3 91.2(5) . . ? 
K25' W27 K3 79.0(4) 2_866 . ? 
O197 W27 K15 80.6(8) . . ? 
O103 W27 K15 134.4(7) . . ? 
O102 W27 K15 45.4(6) . . ? 
O156 W27 K15 132.2(7) . . ? 
O61 W27 K15 47.8(6) . . ? 
O169 W27 K15 96.3(5) . . ? 
K25' W27 K15 97.9(4) 2_866 . ? 
K3 W27 K15 172.47(19) . . ? 
O77 W28 O157 99.8(10) . . ? 
O77 W28 O172 103.9(10) . . ? 
O157 W28 O172 156.2(8) . . ? 
O77 W28 O24 100.6(9) . . ? 
O157 W28 O24 89.4(8) . . ? 
O172 W28 O24 87.8(8) . . ? 
O77 W28 O12 103.8(10) . . ? 
O157 W28 O12 87.5(8) . . ? 
O172 W28 O12 85.4(8) . . ? 
O24 W28 O12 155.6(8) . . ? 
O77 W28 O179 167.1(9) . . ? 
O157 W28 O179 70.8(7) . . ? 
O172 W28 O179 86.0(8) . . ? 
O24 W28 O179 71.1(7) . . ? 
O12 W28 O179 85.0(8) . . ? 
O195 W29 O186 103.9(12) . . ? 
O195 W29 O110 102.5(10) . . ? 
O186 W29 O110 88.8(10) . . ? 
O195 W29 O56 101.2(11) . . ? 
O186 W29 O56 86.8(10) . . ? 
O110 W29 O56 156.2(8) . . ? 
O195 W29 O112 101.1(11) . . ? 
O186 W29 O112 155.0(9) . . ? 
O110 W29 O112 87.2(10) . . ? 
O56 W29 O112 87.0(11) . . ? 
O195 W29 O75 169.1(10) . . ? 
O186 W29 O75 84.0(8) . . ? 
O110 W29 O75 85.0(7) . . ? 
O56 W29 O75 71.3(8) . . ? 
O112 W29 O75 71.1(8) . . ? 
O195 W29 K15 86.3(9) . . ? 
O186 W29 K15 135.3(7) . . ? 
O110 W29 K15 46.7(7) . . ? 
O56 W29 K15 134.4(8) . . ? 
O112 W29 K15 47.6(7) . . ? 
O75 W29 K15 93.4(5) . . ? 
O81 W30 O58 102.0(9) . . ? 
O81 W30 O161 99.4(9) . . ? 
O58 W30 O161 90.5(8) . . ? 
O81 W30 O116 103.7(10) . . ? 
O58 W30 O116 84.9(9) . . ? 
O161 W30 O116 156.8(9) . . ? 
O81 W30 O107 101.6(9) . . ? 
O58 W30 O107 156.2(8) . . ? 
O161 W30 O107 88.8(9) . . ? 
O116 W30 O107 86.5(9) . . ? 
O81 W30 O137 169.7(8) . . ? 
O58 W30 O137 84.7(7) . . ? 
O161 W30 O137 72.5(7) . . ? 
O116 W30 O137 84.5(9) . . ? 
O107 W30 O137 72.4(7) . . ? 
O68 W31 O175 101.6(10) . . ? 
O68 W31 O44 101.9(9) . . ? 
O175 W31 O44 99.2(9) . . ? 
O68 W31 O98 94.6(9) . . ? 
O175 W31 O98 92.3(8) . . ? 
O44 W31 O98 157.4(7) . . ? 
O68 W31 O127 96.5(9) . . ? 
O175 W31 O127 160.0(8) . . ? 
O44 W31 O127 85.1(8) . . ? 
O98 W31 O127 77.7(7) . . ? 
O68 W31 O134 172.0(10) . . ? 
O175 W31 O134 84.6(8) . . ? 
O44 W31 O134 81.9(7) . . ? 
O98 W31 O134 80.0(7) . . ? 
O127 W31 O134 76.6(7) . . ? 
O68 W31 K9 56.2(8) . . ? 
O175 W31 K9 47.4(7) . . ? 
O44 W31 K9 94.8(6) . . ? 
O98 W31 K9 107.2(6) . . ? 
O127 W31 K9 152.2(5) . . ? 
O134 W31 K9 131.0(5) . . ? 
O68 W31 K11 103.1(7) . . ? 
O175 W31 K11 43.0(6) . . ? 
O44 W31 K11 138.3(6) . . ? 
O98 W31 K11 49.3(5) . . ? 
O127 W31 K11 124.2(5) . . ? 
O134 W31 K11 78.0(5) . . ? 
K9 W31 K11 72.69(17) . . ? 
O142 W32 O19 102.8(10) . . ? 
O142 W32 O59 101.8(11) . . ? 
O19 W32 O59 155.4(10) . . ? 
O142 W32 O74 98.0(11) . . ? 
O19 W32 O74 86.9(9) . . ? 
O59 W32 O74 89.8(10) . . ? 
O142 W32 O116 96.8(11) . . ? 
O19 W32 O116 88.5(10) . . ? 
O59 W32 O116 88.6(9) . . ? 
O74 W32 O116 165.1(9) . . ? 
O142 W32 O141 171.7(9) . . ? 
O19 W32 O141 85.2(8) . . ? 
O59 W32 O141 70.3(8) . . ? 
O74 W32 O141 84.5(8) . . ? 
O116 W32 O141 81.0(8) . . ? 
O142 W32 K12 41.4(9) . . ? 
O19 W32 K12 104.0(7) . . ? 
O59 W32 K12 94.4(6) . . ? 
O74 W32 K12 57.1(7) . . ? 
O116 W32 K12 137.8(7) . . ? 
O141 W32 K12 139.2(5) . . ? 
O162 W33 O115 99.8(12) . . ? 
O162 W33 O17 97.4(8) . . ? 
O115 W33 O17 100.0(9) . . ? 
O162 W33 O168 95.3(9) . . ? 
O115 W33 O168 95.6(10) . . ? 
O17 W33 O168 157.9(9) . . ? 
O162 W33 O144 169.9(10) . . ? 
O115 W33 O144 90.3(11) . . ? 
O17 W33 O144 80.7(8) . . ? 
O168 W33 O144 83.7(8) . . ? 
O162 W33 O189 89.3(10) . . ? 
O115 W33 O189 170.7(11) . . ? 
O17 W33 O189 80.5(8) . . ? 
O168 W33 O189 81.5(9) . . ? 
O144 W33 O189 80.6(8) . . ? 
O162 W33 K8 43.4(8) . . ? 
O115 W33 K8 142.1(9) . . ? 
O17 W33 K8 95.1(6) . . ? 
O168 W33 K8 81.7(6) . . ? 
O144 W33 K8 126.6(6) . . ? 
O189 W33 K8 46.6(6) . . ? 
O104 W34 O72 101.7(9) . . ? 
O104 W34 O30 98.8(8) . . ? 
O72 W34 O30 90.6(8) . . ? 
O104 W34 O2 100.2(8) . . ? 
O72 W34 O2 158.0(8) . . ? 
O30 W34 O2 85.1(8) . . ? 
O104 W34 O16 98.7(9) . . ? 
O72 W34 O16 89.2(8) . . ? 
O30 W34 O16 162.2(8) . . ? 
O2 W34 O16 88.5(8) . . ? 
O104 W34 O28 173.4(8) . . ? 
O72 W34 O28 72.1(7) . . ? 
O30 W34 O28 79.2(7) . . ? 
O2 W34 O28 85.9(7) . . ? 
O16 W34 O28 83.9(7) . . ? 
O104 W34 K13 46.9(7) . 2_657 ? 
O72 W34 K13 148.0(6) . 2_657 ? 
O30 W34 K13 89.3(5) . 2_657 ? 
O2 W34 K13 53.6(5) . 2_657 ? 
O16 W34 K13 100.2(6) . 2_657 ? 
O28 W34 K13 138.9(5) . 2_657 ? 
O170 W35 O45 102.5(10) . . ? 
O170 W35 O40 102.8(9) . . ? 
O45 W35 O40 90.2(8) . . ? 
O170 W35 O37 98.3(9) . . ? 
O45 W35 O37 93.0(8) . . ? 
O40 W35 O37 157.3(7) . . ? 
O170 W35 O157 98.8(9) . . ? 
O45 W35 O157 158.7(8) . . ? 
O40 W35 O157 84.6(7) . . ? 
O37 W35 O157 84.3(8) . . ? 
O170 W35 O179 167.3(9) . . ? 
O45 W35 O179 86.4(8) . . ? 
O40 W35 O179 86.0(7) . . ? 
O37 W35 O179 71.8(7) . . ? 
O157 W35 O179 72.7(7) . . ? 
O170 W35 K14 70.2(7) . . ? 
O45 W35 K14 52.6(6) . . ? 
O40 W35 K14 136.7(6) . . ? 
O37 W35 K14 59.0(6) . . ? 
O157 W35 K14 138.2(5) . . ? 
O179 W35 K14 109.5(5) . . ? 
O36 W36 O32 99.6(8) . . ? 
O36 W36 O16 98.8(9) . . ? 
O32 W36 O16 89.2(8) . . ? 
O36 W36 O46 100.7(8) . . ? 
O32 W36 O46 159.7(7) . . ? 
O16 W36 O46 86.8(8) . . ? 
O36 W36 O20 99.0(8) . . ? 
O32 W36 O20 89.2(8) . . ? 
O16 W36 O20 162.2(8) . . ? 
O46 W36 O20 88.6(8) . . ? 
O36 W36 O69 172.6(8) . . ? 
O32 W36 O69 87.8(7) . . ? 
O16 W36 O69 81.8(7) . . ? 
O46 W36 O69 72.0(7) . . ? 
O20 W36 O69 80.4(7) . . ? 
O36 W36 K17 29.7(6) . 1_545 ? 
O32 W36 K17 89.0(6) . 1_545 ? 
O16 W36 K17 70.9(6) . 1_545 ? 
O46 W36 K17 108.3(5) . 1_545 ? 
O20 W36 K17 126.8(6) . 1_545 ? 
O69 W36 K17 152.6(5) . 1_545 ? 
O131 W37 O144 103.9(9) . . ? 
O131 W37 O58 96.6(9) . . ? 
O144 W37 O58 93.0(9) . . ? 
O131 W37 O95 99.3(9) . . ? 
O144 W37 O95 94.7(9) . . ? 
O58 W37 O95 160.1(8) . . ? 
O131 W37 O59 98.5(9) . . ? 
O144 W37 O59 157.5(8) . . ? 
O58 W37 O59 81.9(9) . . ? 
O95 W37 O59 83.9(9) . . ? 
O131 W37 O141 167.5(9) . . ? 
O144 W37 O141 88.5(8) . . ? 
O58 W37 O141 81.6(7) . . ? 
O95 W37 O141 80.3(8) . . ? 
O59 W37 O141 69.0(7) . . ? 
O192 W38 O80 103.9(10) . . ? 
O192 W38 O79 101.8(10) . . ? 
O80 W38 O79 92.3(8) . . ? 
O192 W38 O118 100.5(9) . . ? 
O80 W38 O118 92.1(9) . . ? 
O79 W38 O118 155.5(9) . . ? 
O192 W38 O180 98.9(10) . . ? 
O80 W38 O180 157.2(9) . . ? 
O79 W38 O180 82.7(9) . . ? 
O118 W38 O180 84.0(9) . . ? 
O192 W38 O135 167.4(10) . . ? 
O80 W38 O135 85.9(7) . . ? 
O79 W38 O135 85.5(8) . . ? 
O118 W38 O135 70.8(7) . . ? 
O180 W38 O135 71.6(8) . . ? 
O192 W38 K9 70.9(7) . . ? 
O80 W38 K9 50.2(7) . . ? 
O79 W38 K9 135.0(6) . . ? 
O118 W38 K9 63.0(6) . . ? 
O180 W38 K9 141.8(7) . . ? 
O135 W38 K9 111.2(5) . . ? 
O192 W38 K26 81.8(7) . . ? 
O80 W38 K26 135.2(7) . . ? 
O79 W38 K26 43.9(6) . . ? 
O118 W38 K26 131.2(6) . . ? 
O180 W38 K26 48.0(7) . . ? 
O135 W38 K26 97.0(5) . . ? 
K9 W38 K26 151.8(3) . . ? 
O183 W39 O151 102.4(10) . . ? 
O183 W39 O48 103.9(10) . . ? 
O151 W39 O48 85.2(9) . . ? 
O183 W39 O14 99.8(10) . . ? 
O151 W39 O14 157.7(9) . . ? 
O48 W39 O14 90.9(9) . . ? 
O183 W39 O6 103.7(9) . . ? 
O151 W39 O6 86.3(8) . . ? 
O48 W39 O6 152.3(7) . . ? 
O14 W39 O6 87.0(9) . . ? 
O183 W39 O13 169.1(8) . . ? 
O151 W39 O13 86.8(7) . . ? 
O48 W39 O13 70.7(7) . . ? 
O14 W39 O13 71.2(7) . . ? 
O6 W39 O13 82.4(6) . . ? 
O78 W40 O176 98.5(11) . . ? 
O78 W40 O25 101.0(9) . . ? 
O176 W40 O25 88.1(9) . . ? 
O78 W40 O74 97.8(10) . . ? 
O176 W40 O74 163.6(9) . . ? 
O25 W40 O74 86.9(9) . . ? 
O78 W40 O96 101.3(10) . . ? 
O176 W40 O96 88.2(10) . . ? 
O25 W40 O96 157.7(8) . . ? 
O74 W40 O96 90.5(10) . . ? 
O78 W40 O100 172.9(9) . . ? 
O176 W40 O100 81.6(9) . . ? 
O25 W40 O100 71.9(8) . . ? 
O74 W40 O100 82.0(9) . . ? 
O96 W40 O100 85.8(9) . . ? 
O78 W40 K12 42.8(8) . . ? 
O176 W40 K12 140.3(7) . . ? 
O25 W40 K12 91.6(6) . . ? 
O74 W40 K12 55.5(7) . . ? 
O96 W40 K12 105.1(7) . . ? 
O100 W40 K12 135.5(6) . . ? 
O140 W41 O191 103.5(10) . . ? 
O140 W41 O182 98.8(10) . . ? 
O191 W41 O182 87.8(9) . . ? 
O140 W41 O19 101.3(10) . . ? 
O191 W41 O19 155.1(8) . . ? 
O182 W41 O19 87.6(9) . . ? 
O140 W41 O167 98.0(9) . . ? 
O191 W41 O167 89.2(9) . . ? 
O182 W41 O167 163.1(9) . . ? 
O19 W41 O167 88.1(9) . . ? 
O140 W41 O165 173.4(9) . . ? 
O191 W41 O165 69.8(8) . . ? 
O182 W41 O165 81.6(9) . . ? 
O19 W41 O165 85.3(8) . . ? 
O167 W41 O165 81.7(8) . . ? 
O121 W42 O84 104.9(10) . . ? 
O121 W42 O44 100.6(9) . . ? 
O84 W42 O44 99.3(8) . . ? 
O121 W42 O146 96.7(9) . . ? 
O84 W42 O146 91.2(9) . . ? 
O44 W42 O146 156.6(8) . . ? 
O121 W42 O41 93.7(9) . . ? 
O84 W42 O41 159.8(9) . . ? 
O44 W42 O41 84.7(7) . . ? 
O146 W42 O41 78.6(7) . . ? 
O121 W42 O101 169.5(9) . . ? 
O84 W42 O101 85.2(9) . . ? 
O44 W42 O101 79.9(8) . . ? 
O146 W42 O101 80.2(7) . . ? 
O41 W42 O101 75.9(7) . . ? 
O121 W42 K14 55.6(7) . . ? 
O84 W42 K14 51.5(7) . . ? 
O44 W42 K14 93.7(6) . . ? 
O146 W42 K14 109.1(6) . . ? 
O41 W42 K14 148.5(5) . . ? 
O101 W42 K14 134.9(5) . . ? 
O121 W42 K5 106.1(8) . . ? 
O84 W42 K5 42.3(6) . . ? 
O44 W42 K5 137.6(6) . . ? 
O146 W42 K5 48.9(6) . . ? 
O41 W42 K5 124.9(5) . . ? 
O101 W42 K5 79.5(5) . . ? 
K14 W42 K5 75.8(2) . . ? 
O133 W43 O90 101.8(9) . . ? 
O133 W43 O5 100.6(10) . . ? 
O90 W43 O5 89.0(8) . . ? 
O133 W43 O30 104.7(10) . . ? 
O90 W43 O30 85.9(8) . . ? 
O5 W43 O30 154.7(8) . . ? 
O133 W43 O47 101.7(9) . . ? 
O90 W43 O47 156.3(8) . . ? 
O5 W43 O47 89.9(8) . . ? 
O30 W43 O47 85.0(8) . . ? 
O133 W43 O148 170.4(9) . . ? 
O90 W43 O148 84.7(7) . . ? 
O5 W43 O148 72.3(7) . . ? 
O30 W43 O148 82.5(7) . . ? 
O47 W43 O148 72.4(7) . . ? 
O155 W44 O10 101.8(10) . . ? 
O155 W44 O61 101.8(10) . . ? 
O10 W44 O61 90.6(9) . . ? 
O155 W44 O67 103.3(10) . . ? 
O10 W44 O67 87.5(9) . . ? 
O61 W44 O67 154.7(8) . . ? 
O155 W44 O110 101.6(9) . . ? 
O10 W44 O110 156.6(7) . . ? 
O61 W44 O110 85.3(9) . . ? 
O67 W44 O110 86.5(9) . . ? 
O155 W44 K15 85.8(8) . . ? 
O10 W44 K15 136.8(7) . . ? 
O61 W44 K15 46.5(6) . . ? 
O67 W44 K15 132.5(7) . . ? 
O110 W44 K15 46.2(7) . . ? 
O155 W44 K26 85.7(8) . . ? 
O10 W44 K26 45.9(7) . . ? 
O61 W44 K26 136.3(7) . . ? 
O67 W44 K26 49.8(7) . . ? 
O110 W44 K26 135.9(7) . . ? 
K15 W44 K26 171.5(3) . . ? 
O203 W45 O202 104.1(12) . . ? 
O203 W45 O106 102.6(10) . . ? 
O202 W45 O106 90.9(11) . . ? 
O203 W45 O205 101.8(10) . . ? 
O202 W45 O205 94.8(11) . . ? 
O106 W45 O205 152.8(9) . . ? 
O203 W45 O160 99.5(12) . . ? 
O202 W45 O160 156.0(11) . . ? 
O106 W45 O160 88.5(11) . . ? 
O205 W45 O160 75.7(13) . . ? 
O203 W45 O193 167.2(10) . . ? 
O202 W45 O193 87.7(9) . . ? 
O106 W45 O193 71.6(8) . . ? 
O205 W45 O193 82.0(8) . . ? 
O160 W45 O193 69.4(8) . . ? 
O136 W46 O200 100.6(17) . . ? 
O136 W46 O122 96.9(14) . . ? 
O200 W46 O122 102.0(11) . . ? 
O136 W46 O108 99.7(14) . . ? 
O200 W46 O108 94.8(12) . . ? 
O122 W46 O108 153.7(9) . . ? 
O136 W46 O70 168.9(14) . . ? 
O200 W46 O70 90.3(12) . . ? 
O122 W46 O70 78.6(8) . . ? 
O108 W46 O70 81.2(8) . . ? 
O136 W46 O129 89.5(16) . . ? 
O200 W46 O129 169.3(15) . . ? 
O122 W46 O129 80.0(9) . . ? 
O108 W46 O129 80.0(9) . . ? 
O70 W46 O129 79.7(10) . . ? 
O136 W46 K1 72.6(13) . . ? 
O200 W46 K1 51.0(10) . . ? 
O122 W46 K1 146.0(7) . . ? 
O108 W46 K1 59.5(7) . . ? 
O70 W46 K1 116.7(5) . . ? 
O129 W46 K1 130.8(6) . . ? 
O145 W47 O180 102.4(10) . . ? 
O145 W47 O138 102.9(10) . . ? 
O180 W47 O138 89.9(9) . . ? 
O145 W47 O67 101.0(10) . . ? 
O180 W47 O67 86.9(10) . . ? 
O138 W47 O67 156.0(9) . . ? 
O145 W47 O186 103.2(11) . . ? 
O180 W47 O186 154.2(9) . . ? 
O138 W47 O186 87.6(9) . . ? 
O67 W47 O186 85.0(10) . . ? 
O145 W47 O135 170.3(9) . . ? 
O180 W47 O135 70.6(7) . . ? 
O138 W47 O135 71.0(8) . . ? 
O67 W47 O135 85.6(8) . . ? 
O186 W47 O135 84.4(8) . . ? 
O145 W47 K26 84.6(8) . . ? 
O180 W47 K26 47.0(7) . . ? 
O138 W47 K26 136.5(6) . . ? 
O67 W47 K26 48.2(7) . . ? 
O186 W47 K26 133.0(7) . . ? 
O135 W47 K26 94.8(5) . . ? 
O87 W48 O182 100.6(10) . . ? 
O87 W48 O206 102.6(10) . . ? 
O182 W48 O206 89.4(10) . . ? 
O87 W48 O96 99.9(10) . . ? 
O182 W48 O96 90.1(10) . . ? 
O206 W48 O96 157.2(9) . . ? 
O87 W48 O194 97.7(10) . . ? 
O182 W48 O194 161.7(10) . . ? 
O206 W48 O194 86.3(10) . . ? 
O96 W48 O194 87.1(10) . . ? 
O87 W48 O201 173.0(9) . . ? 
O182 W48 O201 82.3(9) . . ? 
O206 W48 O201 70.9(8) . . ? 
O96 W48 O201 86.4(8) . . ? 
O194 W48 O201 79.5(9) . . ? 
O174 W49 O114 103.8(12) . . ? 
O174 W49 O102 102.8(11) . . ? 
O114 W49 O102 91.2(11) . . ? 
O174 W49 O181 99.0(10) . . ? 
O114 W49 O181 91.7(11) . . ? 
O102 W49 O181 156.7(10) . . ? 
O174 W49 O112 95.9(10) . . ? 
O114 W49 O112 160.3(10) . . ? 
O102 W49 O112 85.5(10) . . ? 
O181 W49 O112 84.0(9) . . ? 
O174 W49 O75 166.4(10) . . ? 
O114 W49 O75 87.1(9) . . ? 
O102 W49 O75 84.8(9) . . ? 
O181 W49 O75 72.3(8) . . ? 
O112 W49 O75 73.2(7) . . ? 
O174 W49 K15 82.7(9) . . ? 
O114 W49 K15 136.0(9) . . ? 
O102 W49 K15 45.6(6) . . ? 
O181 W49 K15 130.9(6) . . ? 
O112 W49 K15 47.3(7) . . ? 
O75 W49 K15 95.1(5) . . ? 
O174 W49 K5 88.2(9) . . ? 
O114 W49 K5 47.8(9) . . ? 
O102 W49 K5 139.0(6) . . ? 
O181 W49 K5 49.4(6) . . ? 
O112 W49 K5 133.1(7) . . ? 
O75 W49 K5 93.5(5) . . ? 
K15 W49 K5 170.84(18) . . ? 
O204 W50 O194 102.4(12) . . ? 
O204 W50 O185 102.9(11) . . ? 
O194 W50 O185 86.8(11) . . ? 
O204 W50 O106 101.0(11) . . ? 
O194 W50 O106 156.5(9) . . ? 
O185 W50 O106 89.3(10) . . ? 
O204 W50 O188 103.6(12) . . ? 
O194 W50 O188 84.6(11) . . ? 
O185 W50 O188 153.3(9) . . ? 
O106 W50 O188 88.6(10) . . ? 
O204 W50 O193 170.6(10) . . ? 
O194 W50 O193 85.3(9) . . ? 
O185 W50 O193 72.0(7) . . ? 
O106 W50 O193 71.5(7) . . ? 
O188 W50 O193 82.1(8) . . ? 
W51' W51 O86 154.6(17) . . ? 
W51' W51 O108 61.8(16) . . ? 
O86 W51 O108 101.1(9) . . ? 
W51' W51 O205 62.9(17) . . ? 
O86 W51 O205 101.1(11) . . ? 
O108 W51 O205 90.2(10) . . ? 
W51' W51 O153 97.9(17) . . ? 
O86 W51 O153 100.9(10) . . ? 
O108 W51 O153 90.4(10) . . ? 
O205 W51 O153 157.4(10) . . ? 
W51' W51 O159 99.8(16) . . ? 
O86 W51 O159 98.1(9) . . ? 
O108 W51 O159 160.8(9) . . ? 
O205 W51 O159 85.1(10) . . ? 
O153 W51 O159 86.9(10) . . ? 
W51' W51 O147 26.4(16) . . ? 
O86 W51 O147 178.7(9) . . ? 
O108 W51 O147 80.2(8) . . ? 
O205 W51 O147 78.9(9) . . ? 
O153 W51 O147 78.9(9) . . ? 
O159 W51 O147 80.6(8) . . ? 
W51 W51' O108 102.8(17) . . ? 
W51 W51' O205 101.7(19) . . ? 
O108 W51' O205 102.9(12) . . ? 
W51 W51' O147 146.9(19) . . ? 
O108 W51' O147 99.3(11) . . ? 
O205 W51' O147 97.1(12) . . ? 
W51 W51' O153 67.6(16) . . ? 
O108 W51' O153 91.4(11) . . ? 
O205 W51' O153 164.0(13) . . ? 
O147 W51' O153 87.5(11) . . ? 
W51 W51' O159 66.3(15) . . ? 
O108 W51' O159 167.9(12) . . ? 
O205 W51' O159 85.1(11) . . ? 
O147 W51' O159 88.6(10) . . ? 
O153 W51' O159 79.7(10) . . ? 
W51 W51' O86 19.5(13) . . ? 
O108 W51' O86 90.3(10) . . ? 
O205 W51' O86 90.1(11) . . ? 
O147 W51' O86 166.4(11) . . ? 
O153 W51' O86 82.5(10) . . ? 
O159 W51' O86 80.5(9) . . ? 
W51 W51' K1 125.4(16) . . ? 
O108 W51' K1 64.5(8) . . ? 
O205 W51' K1 132.6(10) . . ? 
O147 W51' K1 46.5(7) . . ? 
O153 W51' K1 60.4(8) . . ? 
O159 W51' K1 116.5(8) . . ? 
O86 W51' K1 132.7(7) . . ? 
O198 W52 O160 102.0(10) . . ? 
O198 W52 O164 104.9(11) . . ? 
O160 W52 O164 88.3(14) . . ? 
O198 W52 O185 99.6(10) . . ? 
O160 W52 O185 94.1(14) . . ? 
O164 W52 O185 154.4(9) . . ? 
O198 W52 O176 102.4(10) . . ? 
O160 W52 O176 155.7(9) . . ? 
O164 W52 O176 86.0(10) . . ? 
O185 W52 O176 81.3(10) . . ? 
O198 W52 O193 167.9(10) . . ? 
O160 W52 O193 72.6(8) . . ? 
O164 W52 O193 86.0(9) . . ? 
O185 W52 O193 70.6(8) . . ? 
O176 W52 O193 83.4(8) . . ? 
O91 Pd1 O202 176.9(9) . . ? 
O91 Pd1 O50 94.3(9) . . ? 
O202 Pd1 O50 86.8(10) . . ? 
O91 Pd1 O123 89.9(9) . . ? 
O202 Pd1 O123 89.1(10) . . ? 
O50 Pd1 O123 175.1(9) . . ? 
O91 Pd1 Pd10 38.2(5) . . ? 
O202 Pd1 Pd10 139.0(8) . . ? 
O50 Pd1 Pd10 89.5(6) . . ? 
O123 Pd1 Pd10 95.3(7) . . ? 
O91 Pd1 K3 37.9(6) . . ? 
O202 Pd1 K3 142.0(7) . . ? 
O50 Pd1 K3 129.2(7) . . ? 
O123 Pd1 K3 54.2(7) . . ? 
Pd10 Pd1 K3 63.31(12) . . ? 
O125 Pd2 O26 94.2(8) . . ? 
O125 Pd2 O199 85.2(8) . . ? 
O26 Pd2 O199 176.5(9) . . ? 
O125 Pd2 O8 175.1(8) . . ? 
O26 Pd2 O8 90.6(8) . . ? 
O199 Pd2 O8 90.0(8) . . ? 
O125 Pd2 Pd4 71.0(6) . . ? 
O26 Pd2 Pd4 33.1(6) . . ? 
O199 Pd2 Pd4 143.9(6) . . ? 
O8 Pd2 Pd4 112.9(5) . . ? 
O125 Pd2 Pd10 87.1(6) . . ? 
O26 Pd2 Pd10 35.7(6) . . ? 
O199 Pd2 Pd10 147.6(6) . . ? 
O8 Pd2 Pd10 97.3(6) . . ? 
Pd4 Pd2 Pd10 59.91(7) . . ? 
O125 Pd2 K7 44.3(6) . 2_766 ? 
O26 Pd2 K7 120.1(6) . 2_766 ? 
O199 Pd2 K7 57.3(6) . 2_766 ? 
O8 Pd2 K7 131.8(6) . 2_766 ? 
Pd4 Pd2 K7 87.13(14) . 2_766 ? 
Pd10 Pd2 K7 129.66(15) . 2_766 ? 
O125 Pd2 K3 133.2(6) . . ? 
O26 Pd2 K3 40.8(6) . . ? 
O199 Pd2 K3 138.9(6) . . ? 
O8 Pd2 K3 51.3(6) . . ? 
Pd4 Pd2 K3 62.95(12) . . ? 
Pd10 Pd2 K3 63.23(12) . . ? 
K7 Pd2 K3 136.07(18) 2_766 . ? 
O91 Pd3 O103 90.2(8) . . ? 
O91 Pd3 O128 95.4(8) . . ? 
O103 Pd3 O128 172.7(9) . . ? 
O91 Pd3 O114 174.8(9) . . ? 
O103 Pd3 O114 88.4(9) . . ? 
O128 Pd3 O114 86.4(9) . . ? 
O91 Pd3 Pd10 36.6(5) . . ? 
O103 Pd3 Pd10 111.9(6) . . ? 
O128 Pd3 Pd10 70.7(6) . . ? 
O114 Pd3 Pd10 148.1(7) . . ? 
O91 Pd3 K3 45.3(5) . . ? 
O103 Pd3 K3 47.4(6) . . ? 
O128 Pd3 K3 136.3(6) . . ? 
O114 Pd3 K3 134.6(7) . . ? 
Pd10 Pd3 K3 65.74(12) . . ? 
O91 Pd3 K5 135.1(5) . . ? 
O103 Pd3 K5 134.6(6) . . ? 
O128 Pd3 K5 40.3(6) . . ? 
O114 Pd3 K5 46.2(7) . . ? 
Pd10 Pd3 K5 109.03(12) . . ? 
K3 Pd3 K5 170.11(17) . . ? 
O26 Pd4 O120 90.4(8) . . ? 
O26 Pd4 O80 175.6(8) . . ? 
O120 Pd4 O80 86.1(9) . . ? 
O26 Pd4 O177 96.4(8) . . ? 
O120 Pd4 O177 172.6(9) . . ? 
O80 Pd4 O177 87.3(8) . . ? 
O26 Pd4 Pd10 35.3(6) . . ? 
O120 Pd4 Pd10 111.8(6) . . ? 
O80 Pd4 Pd10 149.0(6) . . ? 
O177 Pd4 Pd10 72.8(6) . . ? 
O26 Pd4 Pd2 34.2(5) . . ? 
O120 Pd4 Pd2 100.2(6) . . ? 
O80 Pd4 Pd2 144.0(5) . . ? 
O177 Pd4 Pd2 87.1(6) . . ? 
Pd10 Pd4 Pd2 60.15(7) . . ? 
O26 Pd4 K3 43.7(6) . . ? 
O120 Pd4 K3 48.4(6) . . ? 
O80 Pd4 K3 133.5(6) . . ? 
O177 Pd4 K3 137.3(6) . . ? 
Pd10 Pd4 K3 64.90(12) . . ? 
Pd2 Pd4 K3 67.10(12) . . ? 
O26 Pd4 K9 135.0(6) . . ? 
O120 Pd4 K9 128.7(6) . . ? 
O80 Pd4 K9 47.1(6) . . ? 
O177 Pd4 K9 46.6(6) . . ? 
Pd10 Pd4 K9 119.39(13) . . ? 
Pd2 Pd4 K9 107.67(14) . . ? 
K3 Pd4 K9 171.25(17) . . ? 
O1 Pd5 O21 91.8(7) . . ? 
O1 Pd5 O45 174.6(7) . . ? 
O21 Pd5 O45 84.8(8) . . ? 
O1 Pd5 O64 96.1(7) . . ? 
O21 Pd5 O64 171.3(8) . . ? 
O45 Pd5 O64 87.5(8) . . ? 
O1 Pd5 Pd8 35.5(5) . . ? 
O21 Pd5 Pd8 101.3(6) . . ? 
O45 Pd5 Pd8 141.3(5) . . ? 
O64 Pd5 Pd8 87.2(6) . . ? 
O1 Pd5 Pd9 34.9(5) . . ? 
O21 Pd5 Pd9 112.5(6) . . ? 
O45 Pd5 Pd9 150.5(5) . . ? 
O64 Pd5 Pd9 72.9(6) . . ? 
Pd8 Pd5 Pd9 61.20(6) . . ? 
O1 Pd5 K2 45.4(5) . . ? 
O21 Pd5 K2 48.4(5) . . ? 
O45 Pd5 K2 132.2(5) . . ? 
O64 Pd5 K2 138.1(6) . . ? 
Pd8 Pd5 K2 69.58(11) . . ? 
Pd9 Pd5 K2 65.46(10) . . ? 
O1 Pd5 K14 136.0(5) . . ? 
O21 Pd5 K14 127.0(6) . . ? 
O45 Pd5 K14 45.5(5) . . ? 
O64 Pd5 K14 47.3(6) . . ? 
Pd8 Pd5 K14 107.96(18) . . ? 
Pd9 Pd5 K14 120.19(17) . . ? 
K2 Pd5 K14 172.38(19) . . ? 
O18 Pd6 O3 90.5(7) . . ? 
O18 Pd6 O55 177.6(7) . . ? 
O3 Pd6 O55 87.8(8) . . ? 
O18 Pd6 O83 94.4(7) . . ? 
O3 Pd6 O83 174.6(8) . . ? 
O55 Pd6 O83 87.4(8) . . ? 
O18 Pd6 Pd9 35.5(5) . . ? 
O3 Pd6 Pd9 112.3(5) . . ? 
O55 Pd6 Pd9 147.0(5) . . ? 
O83 Pd6 Pd9 71.0(5) . . ? 
O18 Pd6 K2 44.7(5) . . ? 
O3 Pd6 K2 48.1(6) . . ? 
O55 Pd6 K2 134.2(6) . . ? 
O83 Pd6 K2 135.9(5) . . ? 
Pd9 Pd6 K2 65.37(10) . . ? 
O18 Pd6 K11 135.5(5) . . ? 
O3 Pd6 K11 134.0(6) . . ? 
O55 Pd6 K11 46.2(6) . . ? 
O83 Pd6 K11 41.2(5) . . ? 
Pd9 Pd6 K11 109.05(12) . . ? 
K2 Pd6 K11 169.33(14) . . ? 
O18 Pd7 O57 176.4(7) . . ? 
O18 Pd7 O22 93.6(7) . . ? 
O57 Pd7 O22 88.5(8) . . ? 
O18 Pd7 O4 89.7(7) . . ? 
O57 Pd7 O4 88.3(7) . . ? 
O22 Pd7 O4 176.8(8) . . ? 
O18 Pd7 Pd9 37.8(5) . . ? 
O57 Pd7 Pd9 139.5(5) . . ? 
O22 Pd7 Pd9 88.5(5) . . ? 
O4 Pd7 Pd9 94.0(5) . . ? 
O18 Pd7 K2 38.5(5) . . ? 
O57 Pd7 K2 140.4(5) . . ? 
O22 Pd7 K2 129.4(6) . . ? 
O4 Pd7 K2 53.7(5) . . ? 
Pd9 Pd7 K2 63.33(9) . . ? 
O1 Pd8 O53 89.7(7) . . ? 
O1 Pd8 O52 95.1(8) . . ? 
O53 Pd8 O52 175.1(9) . . ? 
O1 Pd8 O117 177.0(8) . . ? 
O53 Pd8 O117 90.8(8) . . ? 
O52 Pd8 O117 84.5(8) . . ? 
O1 Pd8 Pd5 34.5(4) . . ? 
O53 Pd8 Pd5 112.6(6) . . ? 
O52 Pd8 Pd5 72.2(6) . . ? 
O117 Pd8 Pd5 142.9(6) . . ? 
O1 Pd8 K6 123.8(5) . . ? 
O53 Pd8 K6 137.1(6) . . ? 
O52 Pd8 K6 39.8(6) . . ? 
O117 Pd8 K6 54.4(6) . . ? 
Pd5 Pd8 K6 90.61(14) . . ? 
O1 Pd8 K2 39.0(5) . . ? 
O53 Pd8 K2 52.6(6) . . ? 
O52 Pd8 K2 132.3(6) . . ? 
O117 Pd8 K2 140.5(6) . . ? 
Pd5 Pd8 K2 61.34(10) . . ? 
K6 Pd8 K2 143.25(17) . . ? 
O1 Pd9 O18 86.7(7) . . ? 
O1 Pd9 O82 94.4(7) . . ? 
O18 Pd9 O82 178.7(8) . . ? 
O1 Pd9 O76 178.0(7) . . ? 
O18 Pd9 O76 95.3(7) . . ? 
O82 Pd9 O76 83.6(7) . . ? 
O1 Pd9 Pd7 110.9(4) . . ? 
O18 Pd9 Pd7 37.1(5) . . ? 
O82 Pd9 Pd7 141.6(5) . . ? 
O76 Pd9 Pd7 70.7(5) . . ? 
O1 Pd9 Pd5 34.0(5) . . ? 
O18 Pd9 Pd5 94.3(5) . . ? 
O82 Pd9 Pd5 87.0(5) . . ? 
O76 Pd9 Pd5 145.9(6) . . ? 
Pd7 Pd9 Pd5 129.89(8) . . ? 
O1 Pd9 Pd6 94.3(5) . . ? 
O18 Pd9 Pd6 35.1(5) . . ? 
O82 Pd9 Pd6 145.4(5) . . ? 
O76 Pd9 Pd6 87.6(5) . . ? 
Pd7 Pd9 Pd6 63.32(6) . . ? 
Pd5 Pd9 Pd6 81.75(7) . . ? 
O1 Pd9 K1 132.4(5) . . ? 
O18 Pd9 K1 132.5(5) . . ? 
O82 Pd9 K1 46.1(5) . . ? 
O76 Pd9 K1 45.7(5) . . ? 
Pd7 Pd9 K1 96.66(13) . . ? 
Pd5 Pd9 K1 133.07(13) . . ? 
Pd6 Pd9 K1 133.15(14) . . ? 
O1 Pd9 K2 44.2(5) . . ? 
O18 Pd9 K2 43.3(5) . . ? 
O82 Pd9 K2 137.6(5) . . ? 
O76 Pd9 K2 137.7(5) . . ? 
Pd7 Pd9 K2 68.85(10) . . ? 
Pd5 Pd9 K2 63.60(10) . . ? 
Pd6 Pd9 K2 63.57(10) . . ? 
K1 Pd9 K2 151.37(16) . . ? 
O26 Pd10 O91 86.9(7) . . ? 
O26 Pd10 O149 178.5(9) . . ? 
O91 Pd10 O149 94.4(8) . . ? 
O26 Pd10 O111 95.5(8) . . ? 
O91 Pd10 O111 177.4(8) . . ? 
O149 Pd10 O111 83.2(8) . . ? 
O26 Pd10 Pd1 111.6(6) . . ? 
O91 Pd10 Pd1 36.0(5) . . ? 
O149 Pd10 Pd1 70.0(6) . . ? 
O111 Pd10 Pd1 141.5(6) . . ? 
O26 Pd10 Pd3 93.0(5) . . ? 
O91 Pd10 Pd3 36.1(6) . . ? 
O149 Pd10 Pd3 87.5(6) . . ? 
O111 Pd10 Pd3 144.6(6) . . ? 
Pd1 Pd10 Pd3 63.23(7) . . ? 
O26 Pd10 Pd4 33.5(6) . . ? 
O91 Pd10 Pd4 95.8(5) . . ? 
O149 Pd10 Pd4 145.3(7) . . ? 
O111 Pd10 Pd4 86.8(6) . . ? 
Pd1 Pd10 Pd4 130.62(9) . . ? 
Pd3 Pd10 Pd4 81.59(8) . . ? 
O26 Pd10 Pd2 35.0(5) . . ? 
O91 Pd10 Pd2 108.7(6) . . ? 
O149 Pd10 Pd2 144.7(6) . . ? 
O111 Pd10 Pd2 72.9(6) . . ? 
Pd1 Pd10 Pd2 114.83(9) . . ? 
Pd3 Pd10 Pd2 126.70(9) . . ? 
Pd4 Pd10 Pd2 59.94(7) . . ? 
O26 Pd10 K1 135.7(5) . . ? 
O91 Pd10 K1 131.1(5) . . ? 
O149 Pd10 K1 43.6(6) . . ? 
O111 Pd10 K1 46.2(6) . . ? 
Pd1 Pd10 K1 96.65(14) . . ? 
Pd3 Pd10 K1 130.78(14) . . ? 
Pd4 Pd10 K1 132.69(14) . . ? 
Pd2 Pd10 K1 102.47(13) . . ? 
O26 Pd10 K3 44.0(5) . . ? 
O91 Pd10 K3 43.8(5) . . ? 
O149 Pd10 K3 137.4(6) . . ? 
O111 Pd10 K3 138.3(6) . . ? 
Pd1 Pd10 K3 69.17(12) . . ? 
Pd3 Pd10 K3 63.59(11) . . ? 
Pd4 Pd10 K3 64.34(12) . . ? 
Pd2 Pd10 K3 66.82(11) . . ? 
K1 Pd10 K3 153.83(17) . . ? 
O31 Se1 O28 101.6(9) . . ? 
O31 Se1 O148 99.1(8) . . ? 
O28 Se1 O148 99.6(10) . . ? 
O31 Se1 W2' 139.2(12) . . ? 
O28 Se1 W2' 37.8(12) . . ? 
O148 Se1 W2' 87.8(12) . . ? 
O141 Se2 O165 102.6(10) . . ? 
O141 Se2 O137 99.9(9) . . ? 
O165 Se2 O137 100.9(10) . . ? 
O69 Se3 O43 100.8(9) . . ? 
O69 Se3 O13 99.2(9) . . ? 
O43 Se3 O13 100.7(8) . . ? 
O178 Se4 O166 97.3(9) . . ? 
O178 Se4 O179 98.8(10) . . ? 
O166 Se4 O179 99.0(9) . . ? 
O100 Se5 O193 100.6(11) . . ? 
O100 Se5 O201 100.2(10) . . ? 
O193 Se5 O201 100.4(9) . . ? 
O75 Se6 O169 97.3(9) . . ? 
O75 Se6 O135 99.7(11) . . ? 
O169 Se6 O135 100.8(10) . . ? 
O52 Se7 O82 103.4(9) . . ? 
O52 Se7 O64 102.0(10) . . ? 
O82 Se7 O64 104.2(10) . . ? 
O52 Se7 K6 33.7(7) . . ? 
O82 Se7 K6 133.4(6) . . ? 
O64 Se7 K6 103.2(7) . . ? 
O111 Se8 O177 104.3(10) . . ? 
O111 Se8 O125 104.9(10) . . ? 
O177 Se8 O125 101.1(10) . . ? 
O111 Se8 K9 148.9(7) . . ? 
O177 Se8 K9 46.5(7) . . ? 
O125 Se8 K9 93.3(8) . . ? 
O50 Se9 O149 103.0(11) . . ? 
O50 Se9 O128 102.1(10) . . ? 
O149 Se9 O128 101.1(11) . . ? 
O50 Se9 K5 111.0(7) . . ? 
O149 Se9 K5 133.4(8) . . ? 
O128 Se9 K5 42.1(7) . . ? 
O22 Se10 O83 101.6(9) . . ? 
O22 Se10 O76 102.4(9) . . ? 
O83 Se10 O76 102.7(9) . . ? 
O22 Se10 K8 49.6(6) . . ? 
O83 Se10 K8 128.1(7) . . ? 
O76 Se10 K8 123.3(7) . . ? 
O22 Se10 K11 112.6(7) . . ? 
O83 Se10 K11 40.2(6) . . ? 
O76 Se10 K11 132.1(7) . . ? 
K8 Se10 K11 104.44(19) . . ? 
O149 K1 O76 124.3(7) . . ? 
O149 K1 O82 82.7(7) . . ? 
O76 K1 O82 60.8(6) . . ? 
O149 K1 O111 60.5(6) . . ? 
O76 K1 O111 79.4(7) . . ? 
O82 K1 O111 92.6(6) . . ? 
O149 K1 O184 162.3(8) . . ? 
O76 K1 O184 69.6(7) . . ? 
O82 K1 O184 97.4(6) . . ? 
O111 K1 O184 137.0(8) . . ? 
O149 K1 O147 68.9(7) . . ? 
O76 K1 O147 156.3(7) . . ? 
O82 K1 O147 142.7(7) . . ? 
O111 K1 O147 93.9(7) . . ? 
O184 K1 O147 102.6(7) . . ? 
O149 K1 O200 102.9(8) . . ? 
O76 K1 O200 98.1(6) . . ? 
O82 K1 O200 65.0(7) . . ? 
O111 K1 O200 154.7(8) . . ? 
O184 K1 O200 61.9(8) . . ? 
O147 K1 O200 97.4(7) . . ? 
O149 K1 O153 118.1(7) . . ? 
O76 K1 O153 117.3(6) . . ? 
O82 K1 O153 136.5(6) . . ? 
O111 K1 O153 130.8(7) . . ? 
O184 K1 O153 51.1(6) . . ? 
O147 K1 O153 51.5(6) . . ? 
O200 K1 O153 72.9(7) . . ? 
O149 K1 O115 94.1(6) . . ? 
O76 K1 O115 100.6(6) . . ? 
O82 K1 O115 152.8(7) . . ? 
O111 K1 O115 63.0(7) . . ? 
O184 K1 O115 93.6(7) . . ? 
O147 K1 O115 56.7(7) . . ? 
O200 K1 O115 141.2(8) . . ? 
O153 K1 O115 68.3(6) . . ? 
O149 K1 Pd9 114.0(6) . . ? 
O76 K1 Pd9 33.1(4) . . ? 
O82 K1 Pd9 33.0(4) . . ? 
O111 K1 Pd9 98.7(5) . . ? 
O184 K1 Pd9 70.8(5) . . ? 
O147 K1 Pd9 166.8(5) . . ? 
O200 K1 Pd9 69.5(5) . . ? 
O153 K1 Pd9 120.6(4) . . ? 
O115 K1 Pd9 133.6(5) . . ? 
O149 K1 Pd10 31.9(4) . . ? 
O76 K1 Pd10 110.8(5) . . ? 
O82 K1 Pd10 99.2(4) . . ? 
O111 K1 Pd10 32.9(4) . . ? 
O184 K1 Pd10 160.9(6) . . ? 
O147 K1 Pd10 69.1(4) . . ? 
O200 K1 Pd10 134.7(6) . . ? 
O153 K1 Pd10 118.6(4) . . ? 
O115 K1 Pd10 67.4(4) . . ? 
Pd9 K1 Pd10 120.7(2) . . ? 
O149 K1 W51' 87.2(6) . . ? 
O76 K1 W51' 148.5(5) . . ? 
O82 K1 W51' 131.1(5) . . ? 
O111 K1 W51' 123.0(5) . . ? 
O184 K1 W51' 79.4(6) . . ? 
O147 K1 W51' 29.1(5) . . ? 
O200 K1 W51' 71.0(5) . . ? 
O153 K1 W51' 31.7(5) . . ? 
O115 K1 W51' 75.3(5) . . ? 
Pd9 K1 W51' 138.3(3) . . ? 
Pd10 K1 W51' 96.6(2) . . ? 
O18 K2 O1 60.1(5) . . ? 
O18 K2 O212 146.4(6) . . ? 
O1 K2 O212 151.8(6) . . ? 
O18 K2 O3 61.4(5) . . ? 
O1 K2 O3 98.5(5) . . ? 
O212 K2 O3 105.0(6) . . ? 
O18 K2 O21 99.1(6) . . ? 
O1 K2 O21 61.4(5) . . ? 
O212 K2 O21 108.2(6) . . ? 
O3 K2 O21 78.3(6) . . ? 
O18 K2 O11 115.7(5) . . ? 
O1 K2 O11 115.2(5) . . ? 
O212 K2 O11 67.9(5) . . ? 
O3 K2 O11 56.2(5) . . ? 
O21 K2 O11 55.7(5) . . ? 
O18 K2 O7 107.0(5) . . ? 
O1 K2 O7 105.5(5) . . ? 
O212 K2 O7 63.6(5) . . ? 
O3 K2 O7 142.5(5) . . ? 
O21 K2 O7 138.8(6) . . ? 
O11 K2 O7 131.4(5) . . ? 
O18 K2 O92 145.1(6) . . ? 
O1 K2 O92 94.8(5) . . ? 
O212 K2 O92 57.4(6) . . ? 
O3 K2 O92 152.4(6) . . ? 
O21 K2 O92 87.2(6) . . ? 
O11 K2 O92 96.3(5) . . ? 
O7 K2 O92 53.5(5) . . ? 
O18 K2 O39 92.0(6) . . ? 
O1 K2 O39 140.8(5) . . ? 
O212 K2 O39 55.8(6) . . ? 
O3 K2 O39 89.6(5) . . ? 
O21 K2 O39 156.9(6) . . ? 
O11 K2 O39 101.2(5) . . ? 
O7 K2 O39 53.8(5) . . ? 
O92 K2 O39 95.3(6) . . ? 
O18 K2 O53 93.6(5) . . ? 
O1 K2 O53 55.8(5) . . ? 
O212 K2 O53 102.7(6) . . ? 
O3 K2 O53 152.2(5) . . ? 
O21 K2 O53 95.3(6) . . ? 
O11 K2 O53 140.1(6) . . ? 
O7 K2 O53 52.5(4) . . ? 
O92 K2 O53 51.5(5) . . ? 
O39 K2 O53 104.2(5) . . ? 
O18 K2 O4 56.1(5) . . ? 
O1 K2 O4 87.8(5) . . ? 
O212 K2 O4 102.3(5) . . ? 
O3 K2 O4 101.6(5) . . ? 
O21 K2 O4 148.4(5) . . ? 
O11 K2 O4 148.8(5) . . ? 
O7 K2 O4 52.0(4) . . ? 
O92 K2 O4 103.0(5) . . ? 
O39 K2 O4 53.1(5) . . ? 
O53 K2 O4 69.9(5) . . ? 
O18 K2 W4' 123.9(9) . . ? 
O1 K2 W4' 86.3(10) . . ? 
O212 K2 W4' 69.6(10) . . ? 
O3 K2 W4' 174.4(9) . . ? 
O21 K2 W4' 101.6(9) . . ? 
O11 K2 W4' 119.1(8) . . ? 
O7 K2 W4' 37.1(9) . . ? 
O92 K2 W4' 22.9(8) . . ? 
O39 K2 W4' 88.6(9) . . ? 
O53 K2 W4' 33.3(9) . . ? 
O4 K2 W4' 81.4(8) . . ? 
O91 K3 O26 60.9(6) . . ? 
O91 K3 O103 61.5(6) . . ? 
O26 K3 O103 97.2(6) . . ? 
O91 K3 O120 98.2(6) . . ? 
O26 K3 O120 59.1(6) . . ? 
O103 K3 O120 76.7(7) . . ? 
O91 K3 O156 115.9(6) . . ? 
O26 K3 O156 113.6(7) . . ? 
O103 K3 O156 55.9(6) . . ? 
O120 K3 O156 56.1(6) . . ? 
O91 K3 O8 94.2(6) . . ? 
O26 K3 O8 58.4(6) . . ? 
O103 K3 O8 153.0(6) . . ? 
O120 K3 O8 97.0(6) . . ? 
O156 K3 O8 140.7(6) . . ? 
O91 K3 O73 104.9(6) . . ? 
O26 K3 O73 107.3(6) . . ? 
O103 K3 O73 141.1(6) . . ? 
O120 K3 O73 142.0(6) . . ? 
O156 K3 O73 132.3(6) . . ? 
O8 K3 O73 52.0(5) . . ? 
O91 K3 O132 146.1(6) . . ? 
O26 K3 O132 99.1(6) . . ? 
O103 K3 O132 152.3(6) . . ? 
O120 K3 O132 92.6(6) . . ? 
O156 K3 O132 96.8(5) . . ? 
O8 K3 O132 52.5(5) . . ? 
O73 K3 O132 52.2(5) . . ? 
O91 K3 O124 89.8(6) . . ? 
O26 K3 O124 140.2(7) . . ? 
O103 K3 O124 90.3(7) . . ? 
O120 K3 O124 159.0(6) . . ? 
O156 K3 O124 103.0(6) . . ? 
O8 K3 O124 101.8(6) . . ? 
O73 K3 O124 51.7(6) . . ? 
O132 K3 O124 91.4(6) . . ? 
O91 K3 O123 55.1(6) . . ? 
O26 K3 O123 89.4(6) . . ? 
O103 K3 O123 101.2(6) . . ? 
O120 K3 O123 147.4(6) . . ? 
O156 K3 O123 148.0(6) . . ? 
O8 K3 O123 69.9(6) . . ? 
O73 K3 O123 50.7(5) . . ? 
O132 K3 O123 101.3(6) . . ? 
O124 K3 O123 50.8(6) . . ? 
O91 K3 W15 117.5(5) . . ? 
O26 K3 W15 87.6(4) . . ? 
O103 K3 W15 173.2(6) . . ? 
O120 K3 W15 110.0(4) . . ? 
O156 K3 W15 126.3(5) . . ? 
O8 K3 W15 30.1(4) . . ? 
O73 K3 W15 32.1(3) . . ? 
O132 K3 W15 29.6(3) . . ? 
O124 K3 W15 82.9(5) . . ? 
O123 K3 W15 73.9(4) . . ? 
O91 K3 W23 81.9(5) . . ? 
O26 K3 W23 114.6(5) . . ? 
O103 K3 W23 110.0(5) . . ? 
O120 K3 W23 172.0(5) . . ? 
O156 K3 W23 131.1(5) . . ? 
O8 K3 W23 75.0(4) . . ? 
O73 K3 W23 32.0(3) . . ? 
O132 K3 W23 83.2(4) . . ? 
O124 K3 W23 28.7(4) . . ? 
O123 K3 W23 29.0(4) . . ? 
W15 K3 W23 63.41(12) . . ? 
O63 K4 O63 179.998(2) . 2_657 ? 
O63 K4 O27 86.2(5) . . ? 
O63 K4 O27 93.8(5) 2_657 . ? 
O63 K4 O27 93.8(5) . 2_657 ? 
O63 K4 O27 86.2(5) 2_657 2_657 ? 
O27 K4 O27 180.0(7) . 2_657 ? 
O63 K4 O212 95.9(5) . . ? 
O63 K4 O212 84.1(5) 2_657 . ? 
O27 K4 O212 97.8(5) . . ? 
O27 K4 O212 82.2(5) 2_657 . ? 
O63 K4 O212 84.1(5) . 2_657 ? 
O63 K4 O212 95.9(5) 2_657 2_657 ? 
O27 K4 O212 82.2(5) . 2_657 ? 
O27 K4 O212 97.8(5) 2_657 2_657 ? 
O212 K4 O212 179.998(2) . 2_657 ? 
O63 K4 O7 54.3(5) . . ? 
O63 K4 O7 125.7(5) 2_657 . ? 
O27 K4 O7 55.1(5) . . ? 
O27 K4 O7 124.9(5) 2_657 . ? 
O212 K4 O7 61.7(5) . . ? 
O212 K4 O7 118.3(5) 2_657 . ? 
O63 K4 O7 125.7(5) . 2_657 ? 
O63 K4 O7 54.3(5) 2_657 2_657 ? 
O27 K4 O7 124.9(5) . 2_657 ? 
O27 K4 O7 55.1(5) 2_657 2_657 ? 
O212 K4 O7 118.3(5) . 2_657 ? 
O212 K4 O7 61.7(5) 2_657 2_657 ? 
O7 K4 O7 179.999(2) . 2_657 ? 
O63 K4 W4' 85.7(8) . . ? 
O63 K4 W4' 94.3(8) 2_657 . ? 
O27 K4 W4' 33.4(9) . . ? 
O27 K4 W4' 146.6(9) 2_657 . ? 
O212 K4 W4' 64.8(9) . . ? 
O212 K4 W4' 115.2(9) 2_657 . ? 
O7 K4 W4' 34.4(8) . . ? 
O7 K4 W4' 145.6(8) 2_657 . ? 
O63 K4 W4' 94.3(8) . 2_657 ? 
O63 K4 W4' 85.7(8) 2_657 2_657 ? 
O27 K4 W4' 146.6(9) . 2_657 ? 
O27 K4 W4' 33.4(9) 2_657 2_657 ? 
O212 K4 W4' 115.2(9) . 2_657 ? 
O212 K4 W4' 64.8(9) 2_657 2_657 ? 
O7 K4 W4' 145.6(8) . 2_657 ? 
O7 K4 W4' 34.4(8) 2_657 2_657 ? 
W4' K4 W4' 179.998(3) . 2_657 ? 
O63 K4 W4 79.8(4) . . ? 
O63 K4 W4 100.2(4) 2_657 . ? 
O27 K4 W4 31.9(4) . . ? 
O27 K4 W4 148.1(4) 2_657 . ? 
O212 K4 W4 67.7(4) . . ? 
O212 K4 W4 112.3(4) 2_657 . ? 
O7 K4 W4 30.0(3) . . ? 
O7 K4 W4 150.0(3) 2_657 . ? 
W4' K4 W4 6.2(7) . . ? 
W4' K4 W4 173.8(7) 2_657 . ? 
O63 K4 W4 100.2(4) . 2_657 ? 
O63 K4 W4 79.8(4) 2_657 2_657 ? 
O27 K4 W4 148.1(4) . 2_657 ? 
O27 K4 W4 31.9(4) 2_657 2_657 ? 
O212 K4 W4 112.3(4) . 2_657 ? 
O212 K4 W4 67.7(4) 2_657 2_657 ? 
O7 K4 W4 150.0(3) . 2_657 ? 
O7 K4 W4 30.0(3) 2_657 2_657 ? 
W4' K4 W4 173.8(7) . 2_657 ? 
W4' K4 W4 6.2(7) 2_657 2_657 ? 
W4 K4 W4 180.0 . 2_657 ? 
O84 K5 O211 80.3(8) . . ? 
O84 K5 O214 71.8(7) . . ? 
O211 K5 O214 84.2(8) . . ? 
O84 K5 O128 73.3(6) . . ? 
O211 K5 O128 84.7(8) . . ? 
O214 K5 O128 144.6(7) . . ? 
O84 K5 O146 56.8(6) . . ? 
O211 K5 O146 137.1(8) . . ? 
O214 K5 O146 82.4(6) . . ? 
O128 K5 O146 83.2(6) . . ? 
O84 K5 O114 106.8(6) . . ? 
O211 K5 O114 134.2(9) . . ? 
O214 K5 O114 141.5(8) . . ? 
O128 K5 O114 56.5(6) . . ? 
O146 K5 O114 67.0(7) . . ? 
O84 K5 O181 109.0(7) . . ? 
O211 K5 O181 167.1(8) . . ? 
O214 K5 O181 90.3(6) . . ? 
O128 K5 O181 106.3(6) . . ? 
O146 K5 O181 53.0(5) . . ? 
O114 K5 O181 52.8(6) . . ? 
O84 K5 W42 24.9(4) . . ? 
O211 K5 W42 105.2(7) . . ? 
O214 K5 W42 74.8(5) . . ? 
O128 K5 W42 75.9(5) . . ? 
O146 K5 W42 31.9(3) . . ? 
O114 K5 W42 89.1(5) . . ? 
O181 K5 W42 84.5(4) . . ? 
O84 K5 W13 80.1(5) . . ? 
O211 K5 W13 154.8(7) . . ? 
O214 K5 W13 74.6(5) . . ? 
O128 K5 W13 104.7(5) . . ? 
O146 K5 W13 27.6(3) . . ? 
O114 K5 W13 67.4(5) . . ? 
O181 K5 W13 29.7(4) . . ? 
W42 K5 W13 56.41(13) . . ? 
O84 K5 Se9 76.1(5) . . ? 
O211 K5 Se9 60.9(7) . . ? 
O214 K5 Se9 135.8(5) . . ? 
O128 K5 Se9 24.3(4) . . ? 
O146 K5 Se9 104.4(4) . . ? 
O114 K5 Se9 76.7(5) . . ? 
O181 K5 Se9 129.0(4) . . ? 
W42 K5 Se9 88.36(16) . . ? 
W13 K5 Se9 128.4(2) . . ? 
O84 K5 W49 118.7(5) . . ? 
O211 K5 W49 152.4(7) . . ? 
O214 K5 W49 119.6(5) . . ? 
O128 K5 W49 82.5(4) . . ? 
O146 K5 W49 65.2(4) . . ? 
O114 K5 W49 26.0(4) . . ? 
O181 K5 W49 29.4(4) . . ? 
W42 K5 W49 95.23(19) . . ? 
W13 K5 W49 52.79(11) . . ? 
Se9 K5 W49 102.14(19) . . ? 
O84 K5 Pd3 90.5(5) . . ? 
O211 K5 Pd3 108.6(7) . . ? 
O214 K5 Pd3 156.5(5) . . ? 
O128 K5 Pd3 27.4(4) . . ? 
O146 K5 Pd3 74.8(4) . . ? 
O114 K5 Pd3 29.2(4) . . ? 
O181 K5 Pd3 80.7(4) . . ? 
W42 K5 Pd3 82.63(16) . . ? 
W13 K5 Pd3 87.37(17) . . ? 
Se9 K5 Pd3 48.31(11) . . ? 
W49 K5 Pd3 55.23(11) . . ? 
O52 K6 O230 86.6(9) . . ? 
O52 K6 O211 77.1(8) . . ? 
O230 K6 O211 99.5(11) . . ? 
O52 K6 O109 99.8(7) . . ? 
O230 K6 O109 156.5(9) . . ? 
O211 K6 O109 103.9(9) . . ? 
O52 K6 O23 159.0(6) . 2_757 ? 
O230 K6 O23 85.5(9) . 2_757 ? 
O211 K6 O23 85.1(8) . 2_757 ? 
O109 K6 O23 95.2(6) . 2_757 ? 
O52 K6 O109 140.2(7) . 2_757 ? 
O230 K6 O109 79.8(9) . 2_757 ? 
O211 K6 O109 141.9(8) . 2_757 ? 
O109 K6 O109 81.0(7) . 2_757 ? 
O23 K6 O109 56.8(5) 2_757 2_757 ? 
O52 K6 O117 53.5(6) . . ? 
O230 K6 O117 117.1(9) . . ? 
O211 K6 O117 112.9(8) . . ? 
O109 K6 O117 54.0(5) . . ? 
O23 K6 O117 146.4(6) 2_757 . ? 
O109 K6 O117 100.6(6) 2_757 . ? 
O52 K6 W6 77.6(5) . . ? 
O230 K6 W6 140.7(8) . . ? 
O211 K6 W6 111.3(7) . . ? 
O109 K6 W6 25.9(4) . . ? 
O23 K6 W6 119.9(4) 2_757 . ? 
O109 K6 W6 89.7(4) 2_757 . ? 
O117 K6 W6 28.1(3) . . ? 
O52 K6 W6 160.4(6) . 2_757 ? 
O230 K6 W6 77.1(8) . 2_757 ? 
O211 K6 W6 115.9(7) . 2_757 ? 
O109 K6 W6 91.3(5) . 2_757 ? 
O23 K6 W6 31.1(3) 2_757 2_757 ? 
O109 K6 W6 26.3(4) 2_757 2_757 ? 
O117 K6 W6 125.4(4) . 2_757 ? 
W6 K6 W6 108.4(2) . 2_757 ? 
O52 K6 Pd8 28.1(5) . . ? 
O230 K6 Pd8 91.5(8) . . ? 
O211 K6 Pd8 103.5(7) . . ? 
O109 K6 Pd8 84.3(4) . . ? 
O23 K6 Pd8 171.3(4) 2_757 . ? 
O109 K6 Pd8 114.6(4) 2_757 . ? 
O117 K6 Pd8 30.8(3) . . ? 
W6 K6 Pd8 58.72(11) . . ? 
W6 K6 Pd8 140.1(2) 2_757 . ? 
O52 K6 Se7 20.1(5) . . ? 
O230 K6 Se7 81.4(8) . . ? 
O211 K6 Se7 59.4(7) . . ? 
O109 K6 Se7 111.8(5) . . ? 
O23 K6 Se7 139.0(4) 2_757 . ? 
O109 K6 Se7 154.0(5) 2_757 . ? 
O117 K6 Se7 72.5(4) . . ? 
W6 K6 Se7 93.62(16) . . ? 
W6 K6 Se7 156.9(3) 2_757 . ? 
Pd8 K6 Se7 48.10(10) . . ? 
O52 K6 K6 128.8(5) . 2_757 ? 
O230 K6 K6 117.9(8) . 2_757 ? 
O211 K6 K6 133.2(8) . 2_757 ? 
O109 K6 K6 41.8(5) . 2_757 ? 
O23 K6 K6 71.8(4) 2_757 2_757 ? 
O109 K6 K6 39.2(4) 2_757 2_757 ? 
O117 K6 K6 75.4(4) . 2_757 ? 
W6 K6 K6 54.61(17) . 2_757 ? 
W6 K6 K6 53.82(15) 2_757 2_757 ? 
Pd8 K6 K6 102.6(2) . 2_757 ? 
Se7 K6 K6 147.6(3) . 2_757 ? 
O125 K7 O220 85.2(7) 2_766 . ? 
O125 K7 O49 148.2(7) 2_766 . ? 
O220 K7 O49 112.6(7) . . ? 
O125 K7 O51 95.6(7) 2_766 2_766 ? 
O220 K7 O51 174.8(7) . 2_766 ? 
O49 K7 O51 69.1(6) . 2_766 ? 
O125 K7 O231 70.4(8) 2_766 2_766 ? 
O220 K7 O231 122.5(8) . 2_766 ? 
O49 K7 O231 77.8(7) . 2_766 ? 
O51 K7 O231 62.5(7) 2_766 2_766 ? 
O125 K7 O221 93.4(7) 2_766 . ? 
O220 K7 O221 88.7(8) . . ? 
O49 K7 O221 112.3(7) . . ? 
O51 K7 O221 86.0(7) 2_766 . ? 
O231 K7 O221 141.8(9) 2_766 . ? 
O125 K7 O51 142.9(7) 2_766 . ? 
O220 K7 O51 112.7(7) . . ? 
O49 K7 O51 55.8(5) . . ? 
O51 K7 O51 63.8(7) 2_766 . ? 
O231 K7 O51 118.1(7) 2_766 . ? 
O221 K7 O51 56.7(7) . . ? 
O125 K7 O161 154.2(7) 2_766 . ? 
O220 K7 O161 69.1(6) . . ? 
O49 K7 O161 52.2(5) . . ? 
O51 K7 O161 109.8(6) 2_766 . ? 
O231 K7 O161 125.2(7) 2_766 . ? 
O221 K7 O161 84.1(7) . . ? 
O51 K7 O161 53.3(5) . . ? 
O125 K7 O199 54.5(6) 2_766 2_766 ? 
O220 K7 O199 122.6(7) . 2_766 ? 
O49 K7 O199 123.1(6) . 2_766 ? 
O51 K7 O199 54.7(6) 2_766 2_766 ? 
O231 K7 O199 83.9(7) 2_766 2_766 ? 
O221 K7 O199 59.3(7) . 2_766 ? 
O51 K7 O199 89.3(6) . 2_766 ? 
O161 K7 O199 139.2(6) . 2_766 ? 
O125 K7 O216 76.8(7) 2_766 2_766 ? 
O220 K7 O216 70.8(7) . 2_766 ? 
O49 K7 O216 84.4(7) . 2_766 ? 
O51 K7 O216 114.5(7) 2_766 2_766 ? 
O231 K7 O216 53.6(8) 2_766 2_766 ? 
O221 K7 O216 157.8(8) . 2_766 ? 
O51 K7 O216 138.9(7) . 2_766 ? 
O161 K7 O216 96.0(7) . 2_766 ? 
O199 K7 O216 124.7(7) 2_766 2_766 ? 
O125 K7 W11 169.8(6) 2_766 . ? 
O220 K7 W11 103.1(5) . . ? 
O49 K7 W11 32.8(4) . . ? 
O51 K7 W11 75.6(4) 2_766 . ? 
O231 K7 W11 108.8(6) 2_766 . ? 
O221 K7 W11 81.2(6) . . ? 
O51 K7 W11 28.1(4) . . ? 
O161 K7 W11 34.3(3) . . ? 
O199 K7 W11 115.5(4) 2_766 . ? 
O216 K7 W11 111.1(6) 2_766 . ? 
O125 K7 W11 77.1(5) 2_766 2_766 ? 
O220 K7 W11 150.2(6) . 2_766 ? 
O49 K7 W11 94.5(5) . 2_766 ? 
O51 K7 W11 26.4(4) 2_766 2_766 ? 
O231 K7 W11 73.8(6) 2_766 2_766 ? 
O221 K7 W11 68.8(6) . 2_766 ? 
O51 K7 W11 71.9(4) . 2_766 ? 
O161 K7 W11 124.9(4) . 2_766 ? 
O199 K7 W11 28.6(4) 2_766 2_766 ? 
O216 K7 W11 126.4(6) 2_766 2_766 ? 
W11 K7 W11 92.91(18) . 2_766 ? 
O94 K8 O22 95.9(6) . . ? 
O94 K8 O189 69.7(7) . . ? 
O22 K8 O189 116.3(7) . . ? 
O94 K8 O162 109.2(7) . . ? 
O22 K8 O162 74.4(5) . . ? 
O189 K8 O162 55.9(6) . . ? 
O94 K8 O215 151.0(9) . . ? 
O22 K8 O215 63.8(8) . . ? 
O189 K8 O215 136.8(8) . . ? 
O162 K8 O215 86.2(8) . . ? 
O94 K8 Se10 116.1(5) . . ? 
O22 K8 Se10 26.5(3) . . ? 
O189 K8 Se10 105.6(5) . . ? 
O162 K8 Se10 53.2(4) . . ? 
O215 K8 Se10 53.6(7) . . ? 
O94 K8 W10 22.1(4) . . ? 
O22 K8 W10 74.3(4) . . ? 
O189 K8 W10 76.4(5) . . ? 
O162 K8 W10 98.5(4) . . ? 
O215 K8 W10 134.9(7) . . ? 
Se10 K8 W10 94.13(19) . . ? 
O94 K8 W33 90.3(5) . . ? 
O22 K8 W33 90.1(4) . . ? 
O189 K8 W33 32.5(5) . . ? 
O162 K8 W33 23.7(4) . . ? 
O215 K8 W33 109.3(7) . . ? 
Se10 K8 W33 73.92(16) . . ? 
W10 K8 W33 85.93(18) . . ? 
O94 K8 K15 105.4(6) . 1_455 ? 
O22 K8 K15 89.1(4) . 1_455 ? 
O189 K8 K15 154.3(6) . 1_455 ? 
O162 K8 K15 142.8(5) . 1_455 ? 
O215 K8 K15 56.7(7) . 1_455 ? 
Se10 K8 K15 99.1(3) . 1_455 ? 
W10 K8 K15 108.8(2) . 1_455 ? 
W33 K8 K15 164.3(3) . 1_455 ? 
O175 K9 O220 129.6(7) . 2_766 ? 
O175 K9 O177 66.0(6) . . ? 
O220 K9 O177 84.1(7) 2_766 . ? 
O175 K9 O68 57.1(6) . . ? 
O220 K9 O68 173.0(7) 2_766 . ? 
O177 K9 O68 98.6(7) . . ? 
O175 K9 O80 117.0(6) . . ? 
O220 K9 O80 68.9(6) 2_766 . ? 
O177 K9 O80 56.6(6) . . ? 
O68 K9 O80 107.1(6) . . ? 
O175 K9 O216 66.8(7) . . ? 
O220 K9 O216 71.8(7) 2_766 . ? 
O177 K9 O216 86.0(7) . . ? 
O68 K9 O216 114.8(7) . . ? 
O80 K9 O216 127.2(7) . . ? 
O175 K9 O118 120.2(5) . . ? 
O220 K9 O118 101.4(6) 2_766 . ? 
O177 K9 O118 95.6(5) . . ? 
O68 K9 O118 72.0(5) . . ? 
O80 K9 O118 49.6(5) . . ? 
O216 K9 O118 172.8(6) . . ? 
O175 K9 W31 28.9(4) . . ? 
O220 K9 W31 157.0(6) 2_766 . ? 
O177 K9 W31 77.2(4) . . ? 
O68 K9 W31 29.1(4) . . ? 
O80 K9 W31 110.0(5) . . ? 
O216 K9 W31 93.6(5) . . ? 
O118 K9 W31 93.7(3) . . ? 
O175 K9 W38 137.5(5) . . ? 
O220 K9 W38 71.7(5) 2_766 . ? 
O177 K9 W38 83.7(4) . . ? 
O68 K9 W38 102.1(4) . . ? 
O80 K9 W38 27.4(4) . . ? 
O216 K9 W38 142.8(6) . . ? 
O118 K9 W38 31.0(3) . . ? 
W31 K9 W38 118.6(2) . . ? 
O175 K9 Se8 55.2(5) . . ? 
O220 K9 Se8 80.5(6) 2_766 . ? 
O177 K9 Se8 24.7(4) . . ? 
O68 K9 Se8 104.6(5) . . ? 
O80 K9 Se8 78.3(4) . . ? 
O216 K9 Se8 61.6(6) . . ? 
O118 K9 Se8 120.3(4) . . ? 
W31 K9 Se8 76.92(16) . . ? 
W38 K9 Se8 105.5(2) . . ? 
O175 K9 Pd4 96.1(5) . . ? 
O220 K9 Pd4 64.5(5) 2_766 . ? 
O177 K9 Pd4 30.3(4) . . ? 
O68 K9 Pd4 115.1(5) . . ? 
O80 K9 Pd4 29.8(4) . . ? 
O216 K9 Pd4 100.7(6) . . ? 
O118 K9 Pd4 77.7(4) . . ? 
W31 K9 Pd4 102.6(2) . . ? 
W38 K9 Pd4 56.72(13) . . ? 
Se8 K9 Pd4 48.92(13) . . ? 
O175 K9 K11 37.6(4) . . ? 
O220 K9 K11 113.3(5) 2_766 . ? 
O177 K9 K11 94.3(4) . . ? 
O68 K9 K11 73.1(4) . . ? 
O80 K9 K11 150.8(5) . . ? 
O216 K9 K11 41.7(5) . . ? 
O118 K9 K11 144.8(4) . . ? 
W31 K9 K11 55.96(14) . . ? 
W38 K9 K11 174.5(2) . . ? 
Se8 K9 K11 73.62(17) . . ? 
Pd4 K9 K11 122.5(2) . . ? 
O121 K10 O234 148.3(9) . . ? 
O121 K10 O42 71.4(7) . . ? 
O234 K10 O42 99.0(9) . . ? 
O121 K10 O152 77.8(7) . . ? 
O234 K10 O152 70.5(9) . . ? 
O42 K10 O152 73.0(6) . . ? 
O121 K10 O77 126.7(7) . 2_767 ? 
O234 K10 O77 78.9(8) . 2_767 ? 
O42 K10 O77 144.5(6) . 2_767 ? 
O152 K10 O77 135.9(7) . 2_767 ? 
O121 K10 O150 70.7(7) . . ? 
O234 K10 O150 118.8(9) . . ? 
O42 K10 O150 140.7(7) . . ? 
O152 K10 O150 108.2(7) . . ? 
O77 K10 O150 60.5(6) 2_767 . ? 
O121 K10 O105 71.3(6) . . ? 
O234 K10 O105 89.7(9) . . ? 
O42 K10 O105 120.4(6) . . ? 
O152 K10 O105 54.9(6) . . ? 
O77 K10 O105 95.1(6) 2_767 . ? 
O150 K10 O105 54.3(6) . . ? 
O121 K10 W19 67.8(5) . . ? 
O234 K10 W19 82.8(7) . . ? 
O42 K10 W19 91.8(4) . . ? 
O152 K10 W19 25.0(5) . . ? 
O77 K10 W19 122.6(5) 2_767 . ? 
O150 K10 W19 83.2(5) . . ? 
O105 K10 W19 30.8(4) . . ? 
O121 K10 W13 64.0(5) . . ? 
O234 K10 W13 110.2(8) . . ? 
O42 K10 W13 132.5(5) . . ? 
O152 K10 W13 82.4(5) . . ? 
O77 K10 W13 79.2(4) 2_767 . ? 
O150 K10 W13 25.8(4) . . ? 
O105 K10 W13 29.2(4) . . ? 
W19 K10 W13 57.36(13) . . ? 
O121 K10 K19 82.2(5) . . ? 
O234 K10 K19 72.1(7) . . ? 
O42 K10 K19 41.0(5) . . ? 
O152 K10 K19 34.9(5) . . ? 
O77 K10 K19 150.6(5) 2_767 . ? 
O150 K10 K19 139.7(5) . . ? 
O105 K10 K19 89.3(5) . . ? 
W19 K10 K19 58.6(2) . . ? 
W13 K10 K19 114.8(3) . . ? 
O121 K10 K14 32.5(5) . . ? 
O234 K10 K14 169.8(8) . . ? 
O42 K10 K14 71.3(5) . . ? 
O152 K10 K14 108.4(5) . . ? 
O77 K10 K14 107.0(5) 2_767 . ? 
O150 K10 K14 71.3(5) . . ? 
O105 K10 K14 97.9(5) . . ? 
W19 K10 K14 100.2(2) . . ? 
W13 K10 K14 79.3(2) . . ? 
K19 K10 K14 101.1(3) . . ? 
O175 K11 O83 73.1(6) . . ? 
O175 K11 O98 57.8(5) . . ? 
O83 K11 O98 86.2(5) . . ? 
O175 K11 O216 68.3(7) . . ? 
O83 K11 O216 103.1(7) . . ? 
O98 K11 O216 119.6(7) . . ? 
O175 K11 O55 106.4(6) . . ? 
O83 K11 O55 56.9(5) . . ? 
O98 K11 O55 67.9(5) . . ? 
O216 K11 O55 159.4(7) . . ? 
O175 K11 O119 110.1(6) . . ? 
O83 K11 O119 109.1(6) . . ? 
O98 K11 O119 52.9(5) . . ? 
O216 K11 O119 145.7(7) . . ? 
O55 K11 O119 54.7(5) . . ? 
O175 K11 O215 116.4(8) . . ? 
O83 K11 O215 66.9(8) . . ? 
O98 K11 O215 152.3(8) . . ? 
O216 K11 O215 75.1(8) . . ? 
O55 K11 O215 90.8(7) . . ? 
O119 K11 O215 128.5(8) . . ? 
O175 K11 W31 26.0(4) . . ? 
O83 K11 W31 77.0(4) . . ? 
O98 K11 W31 31.9(4) . . ? 
O216 K11 W31 91.7(6) . . ? 
O55 K11 W31 88.5(4) . . ? 
O119 K11 W31 84.5(4) . . ? 
O215 K11 W31 136.9(7) . . ? 
O175 K11 W7 119.8(4) . . ? 
O83 K11 W7 84.3(4) . . ? 
O98 K11 W7 65.8(4) . . ? 
O216 K11 W7 170.8(6) . . ? 
O55 K11 W7 27.3(3) . . ? 
O119 K11 W7 30.2(3) . . ? 
O215 K11 W7 103.3(7) . . ? 
W31 K11 W7 95.42(16) . . ? 
O175 K11 W20 81.4(4) . . ? 
O83 K11 W20 107.0(4) . . ? 
O98 K11 W20 27.1(4) . . ? 
O216 K11 W20 128.1(6) . . ? 
O55 K11 W20 68.0(4) . . ? 
O119 K11 W20 29.4(3) . . ? 
O215 K11 W20 156.2(7) . . ? 
W31 K11 W20 56.57(10) . . ? 
W7 K11 W20 52.93(10) . . ? 
O175 K11 Se10 74.2(5) . . ? 
O83 K11 Se10 22.9(4) . . ? 
O98 K11 Se10 105.3(4) . . ? 
O216 K11 Se10 82.7(6) . . ? 
O55 K11 Se10 76.8(3) . . ? 
O119 K11 Se10 131.0(4) . . ? 
O215 K11 Se10 50.6(7) . . ? 
W31 K11 Se10 87.55(15) . . ? 
W7 K11 Se10 103.50(17) . . ? 
W20 K11 Se10 128.85(19) . . ? 
O175 K11 Pd6 90.2(4) . . ? 
O83 K11 Pd6 28.2(4) . . ? 
O98 K11 Pd6 76.2(4) . . ? 
O216 K11 Pd6 131.0(6) . . ? 
O55 K11 Pd6 28.8(3) . . ? 
O119 K11 Pd6 82.3(4) . . ? 
O215 K11 Pd6 76.8(7) . . ? 
W31 K11 Pd6 82.46(14) . . ? 
W7 K11 Pd6 56.10(10) . . ? 
W20 K11 Pd6 88.09(15) . . ? 
Se10 K11 Pd6 48.68(10) . . ? 
O142 K12 O35 74.2(7) . 2_756 ? 
O142 K12 O190 138.5(8) . 2_756 ? 
O35 K12 O190 72.2(7) 2_756 2_756 ? 
O142 K12 O154 73.1(7) . 2_756 ? 
O35 K12 O154 71.6(6) 2_756 2_756 ? 
O190 K12 O154 73.7(7) 2_756 2_756 ? 
O142 K12 O78 107.4(7) . . ? 
O35 K12 O78 156.3(7) 2_756 . ? 
O190 K12 O78 113.2(8) 2_756 . ? 
O154 K12 O78 132.0(8) 2_756 . ? 
O142 K12 O228 68.3(8) . . ? 
O35 K12 O228 89.8(7) 2_756 . ? 
O190 K12 O228 134.3(9) 2_756 . ? 
O154 K12 O228 140.4(8) 2_756 . ? 
O78 K12 O228 69.9(8) . . ? 
O142 K12 O74 54.7(6) . . ? 
O35 K12 O74 127.6(6) 2_756 . ? 
O190 K12 O74 157.6(7) 2_756 . ? 
O154 K12 O74 100.9(7) 2_756 . ? 
O78 K12 O74 54.0(6) . . ? 
O228 K12 O74 62.9(7) . . ? 
O142 K12 W32 24.5(5) . . ? 
O35 K12 W32 98.6(5) 2_756 . ? 
O190 K12 W32 156.7(6) 2_756 . ? 
O154 K12 W32 83.1(5) 2_756 . ? 
O78 K12 W32 84.1(5) . . ? 
O228 K12 W32 65.1(6) . . ? 
O74 K12 W32 30.4(3) . . ? 
O142 K12 W3' 86.7(9) . 2_756 ? 
O35 K12 W3' 15.3(8) 2_756 2_756 ? 
O190 K12 W3' 65.3(9) 2_756 2_756 ? 
O154 K12 W3' 83.4(9) 2_756 2_756 ? 
O78 K12 W3' 144.1(9) . 2_756 ? 
O228 K12 W3' 86.2(10) . 2_756 ? 
O74 K12 W3' 136.5(8) . 2_756 ? 
W32 K12 W3' 110.3(7) . 2_756 ? 
O142 K12 W40 84.1(5) . . ? 
O35 K12 W40 152.4(5) 2_756 . ? 
O190 K12 W40 134.3(6) 2_756 . ? 
O154 K12 W40 118.3(6) 2_756 . ? 
O78 K12 W40 24.5(5) . . ? 
O228 K12 W40 66.1(6) . . ? 
O74 K12 W40 29.6(3) . . ? 
W32 K12 W40 60.00(13) . . ? 
W3' K12 W40 152.3(8) 2_756 . ? 
O142 K12 W3 91.6(5) . 2_756 ? 
O35 K12 W3 20.1(4) 2_756 2_756 ? 
O190 K12 W3 61.8(5) 2_756 2_756 ? 
O154 K12 W3 85.9(6) 2_756 2_756 ? 
O78 K12 W3 140.8(6) . 2_756 ? 
O228 K12 W3 87.0(6) . 2_756 ? 
O74 K12 W3 140.4(5) . 2_756 ? 
W32 K12 W3 115.1(2) . 2_756 ? 
W3' K12 W3 5.1(7) 2_756 2_756 ? 
W40 K12 W3 152.5(3) . 2_756 ? 
O142 K12 K16 49.8(5) . 2_756 ? 
O35 K12 K16 41.8(4) 2_756 2_756 ? 
O190 K12 K16 88.8(6) 2_756 2_756 ? 
O154 K12 K16 38.9(5) 2_756 2_756 ? 
O78 K12 K16 154.0(6) . 2_756 ? 
O228 K12 K16 105.3(7) . 2_756 ? 
O74 K12 K16 100.6(4) . 2_756 ? 
W32 K12 K16 71.3(2) . 2_756 ? 
W3' K12 K16 56.9(7) 2_756 2_756 ? 
W40 K12 K16 129.6(3) . 2_756 ? 
W3 K12 K16 61.3(2) 2_756 2_756 ? 
O223 K13 O222 134.8(10) . . ? 
O223 K13 O97 117.2(8) . 2_667 ? 
O222 K13 O97 86.5(8) . 2_667 ? 
O223 K13 O29 100.9(8) . . ? 
O222 K13 O29 89.5(8) . . ? 
O97 K13 O29 129.1(7) 2_667 . ? 
O223 K13 O104 77.7(7) . 2_657 ? 
O222 K13 O104 80.9(8) . 2_657 ? 
O97 K13 O104 63.1(6) 2_667 2_657 ? 
O29 K13 O104 164.3(7) . 2_657 ? 
O223 K13 O65 150.9(8) . . ? 
O222 K13 O65 65.6(7) . . ? 
O97 K13 O65 79.3(6) 2_667 . ? 
O29 K13 O65 53.4(5) . . ? 
O104 K13 O65 130.9(6) 2_657 . ? 
O223 K13 O15 71.8(7) . 2_657 ? 
O222 K13 O15 75.9(8) . 2_657 ? 
O97 K13 O15 160.3(7) 2_667 2_657 ? 
O29 K13 O15 60.5(6) . 2_657 ? 
O104 K13 O15 104.8(6) 2_657 2_657 ? 
O65 K13 O15 100.8(5) . 2_657 ? 
O223 K13 O2 67.5(7) . 2_657 ? 
O222 K13 O2 67.8(7) . 2_657 ? 
O97 K13 O2 112.9(6) 2_667 2_657 ? 
O29 K13 O2 112.1(6) . 2_657 ? 
O104 K13 O2 52.6(5) 2_657 2_657 ? 
O65 K13 O2 130.8(6) . 2_657 ? 
O15 K13 O2 52.3(5) 2_657 2_657 ? 
O223 K13 K27 114.8(7) . . ? 
O222 K13 K27 110.3(7) . . ? 
O97 K13 K27 62.1(6) 2_667 . ? 
O29 K13 K27 72.2(5) . . ? 
O104 K13 K27 122.9(5) 2_657 . ? 
O65 K13 K27 49.2(5) . . ? 
O15 K13 K27 132.3(5) 2_657 . ? 
O2 K13 K27 175.0(5) 2_657 . ? 
O223 K13 W21 123.8(6) . . ? 
O222 K13 W21 75.9(6) . . ? 
O97 K13 W21 108.7(5) 2_667 . ? 
O29 K13 W21 23.2(4) . . ? 
O104 K13 W21 156.0(5) 2_657 . ? 
O65 K13 W21 30.5(3) . . ? 
O15 K13 W21 75.8(4) 2_657 . ? 
O2 K13 W21 121.5(4) 2_657 . ? 
K27 K13 W21 61.4(3) . . ? 
O223 K13 W34 69.4(6) . 2_657 ? 
O222 K13 W34 74.9(6) . 2_657 ? 
O97 K13 W34 86.3(5) 2_667 2_657 ? 
O29 K13 W34 140.8(5) . 2_657 ? 
O104 K13 W34 24.1(4) 2_657 2_657 ? 
O65 K13 W34 138.6(5) . 2_657 ? 
O15 K13 W34 80.7(4) 2_657 2_657 ? 
O2 K13 W34 28.7(3) 2_657 2_657 ? 
K27 K13 W34 146.9(3) . 2_657 ? 
W21 K13 W34 146.1(3) . 2_657 ? 
O223 K13 W1 65.1(6) . 2_657 ? 
O222 K13 W1 72.4(7) . 2_657 ? 
O97 K13 W1 140.3(6) 2_667 2_657 ? 
O29 K13 W1 84.9(5) . 2_657 ? 
O104 K13 W1 80.3(4) 2_657 2_657 ? 
O65 K13 W1 118.8(4) . 2_657 ? 
O15 K13 W1 24.5(4) 2_657 2_657 ? 
O2 K13 W1 28.0(3) 2_657 2_657 ? 
K27 K13 W1 156.8(3) . 2_657 ? 
W21 K13 W1 98.42(19) . 2_657 ? 
W34 K13 W1 56.25(14) 2_657 2_657 ? 
O213 K14 O84 135.6(8) . . ? 
O213 K14 O214 78.8(7) . . ? 
O84 K14 O214 71.4(6) . . ? 
O213 K14 O230 92.7(10) . . ? 
O84 K14 O230 118.0(10) . . ? 
O214 K14 O230 88.4(9) . . ? 
O213 K14 O121 87.1(8) . . ? 
O84 K14 O121 56.5(7) . . ? 
O214 K14 O121 80.6(7) . . ? 
O230 K14 O121 168.8(9) . . ? 
O213 K14 O45 99.3(7) . . ? 
O84 K14 O45 117.0(6) . . ? 
O214 K14 O45 166.6(7) . . ? 
O230 K14 O45 78.4(9) . . ? 
O121 K14 O45 112.7(7) . . ? 
O213 K14 O64 155.0(7) . . ? 
O84 K14 O64 63.3(6) . . ? 
O214 K14 O64 126.2(7) . . ? 
O230 K14 O64 88.4(9) . . ? 
O121 K14 O64 96.5(7) . . ? 
O45 K14 O64 56.5(6) . . ? 
O213 K14 O37 59.6(6) . . ? 
O84 K14 O37 125.2(7) . . ? 
O214 K14 O37 133.7(7) . . ? 
O230 K14 O37 111.3(9) . . ? 
O121 K14 O37 78.2(6) . . ? 
O45 K14 O37 51.7(5) . . ? 
O64 K14 O37 96.9(6) . . ? 
O213 K14 W42 114.6(6) . . ? 
O84 K14 W42 28.8(5) . . ? 
O214 K14 W42 79.3(5) . . ? 
O230 K14 W42 146.7(9) . . ? 
O121 K14 W42 28.6(5) . . ? 
O45 K14 W42 113.2(5) . . ? 
O64 K14 W42 74.8(4) . . ? 
O37 K14 W42 99.2(4) . . ? 
O213 K14 W35 71.5(5) . . ? 
O84 K14 W35 139.4(5) . . ? 
O214 K14 W35 148.2(6) . . ? 
O230 K14 W35 82.0(8) . . ? 
O121 K14 W35 108.5(6) . . ? 
O45 K14 W35 27.8(4) . . ? 
O64 K14 W35 83.9(5) . . ? 
O37 K14 W35 31.9(3) . . ? 
W42 K14 W35 123.3(3) . . ? 
O213 K14 Pd5 127.6(6) . . ? 
O84 K14 Pd5 93.4(5) . . ? 
O214 K14 Pd5 147.2(6) . . ? 
O230 K14 Pd5 73.0(8) . . ? 
O121 K14 Pd5 115.7(5) . . ? 
O45 K14 Pd5 29.3(4) . . ? 
O64 K14 Pd5 30.2(4) . . ? 
O37 K14 Pd5 78.9(4) . . ? 
W42 K14 Pd5 101.5(3) . . ? 
W35 K14 Pd5 56.89(14) . . ? 
O213 K14 K5 114.6(6) . . ? 
O84 K14 K5 35.8(4) . . ? 
O214 K14 K5 37.7(5) . . ? 
O230 K14 K5 97.8(8) . . ? 
O121 K14 K5 72.2(5) . . ? 
O45 K14 K5 146.2(5) . . ? 
O64 K14 K5 90.0(5) . . ? 
O37 K14 K5 150.2(5) . . ? 
W42 K14 K5 54.61(18) . . ? 
W35 K14 K5 173.9(3) . . ? 
Pd5 K14 K5 117.2(3) . . ? 
O102 K15 O110 66.8(6) . . ? 
O102 K15 O112 55.2(6) . . ? 
O110 K15 O112 53.5(5) . . ? 
O102 K15 O61 53.5(6) . . ? 
O110 K15 O61 53.1(6) . . ? 
O112 K15 O61 89.9(6) . . ? 
O102 K15 W29 67.6(5) . . ? 
O110 K15 W29 28.2(4) . . ? 
O112 K15 W29 29.0(4) . . ? 
O61 K15 W29 77.6(4) . . ? 
O102 K15 W27 28.1(4) . . ? 
O110 K15 W27 68.7(4) . . ? 
O112 K15 W27 79.9(4) . . ? 
O61 K15 W27 30.7(4) . . ? 
W29 K15 W27 82.60(18) . . ? 
O102 K15 W49 28.7(4) . . ? 
O110 K15 W49 67.2(4) . . ? 
O112 K15 W49 30.5(4) . . ? 
O61 K15 W49 78.1(4) . . ? 
W29 K15 W49 53.45(13) . . ? 
W27 K15 W49 56.63(13) . . ? 
O102 K15 W44 66.6(5) . . ? 
O110 K15 W44 29.5(4) . . ? 
O112 K15 W44 79.0(4) . . ? 
O61 K15 W44 27.5(4) . . ? 
W29 K15 W44 57.33(13) . . ? 
W27 K15 W44 53.61(13) . . ? 
W49 K15 W44 81.37(18) . . ? 
O102 K15 K8 117.8(6) . 1_655 ? 
O110 K15 K8 166.9(5) . 1_655 ? 
O112 K15 K8 139.6(5) . 1_655 ? 
O61 K15 K8 118.3(5) . 1_655 ? 
W29 K15 K8 163.7(3) . 1_655 ? 
W27 K15 K8 109.2(3) . 1_655 ? 
W49 K15 K8 123.2(3) . 1_655 ? 
W44 K15 K8 138.7(3) . 1_655 ? 
O154 K16 O35 71.8(6) . . ? 
O154 K16 O86 72.0(7) . . ? 
O35 K16 O86 70.4(6) . . ? 
O154 K16 O233 65.7(8) . 1_545 ? 
O35 K16 O233 127.5(8) . 1_545 ? 
O86 K16 O233 120.4(8) . 1_545 ? 
O154 K16 O142 67.0(8) . 2_756 ? 
O35 K16 O142 65.7(6) . 2_756 ? 
O86 K16 O142 126.8(7) . 2_756 ? 
O233 K16 O142 70.2(7) 1_545 2_756 ? 
O154 K16 W3' 83.9(9) . . ? 
O35 K16 W3' 15.9(8) . . ? 
O86 K16 W3' 63.6(8) . . ? 
O233 K16 W3' 143.3(10) 1_545 . ? 
O142 K16 W3' 79.5(9) 2_756 . ? 
O154 K16 W22 20.8(5) . . ? 
O35 K16 W22 86.5(4) . . ? 
O86 K16 W22 62.2(4) . . ? 
O233 K16 W22 63.4(6) 1_545 . ? 
O142 K16 W22 86.2(5) 2_756 . ? 
W3' K16 W22 95.2(8) . . ? 
O154 K16 K21 108.1(7) . 1_545 ? 
O35 K16 K21 162.0(7) . 1_545 ? 
O86 K16 K21 127.2(7) . 1_545 ? 
O233 K16 K21 44.1(7) 1_545 1_545 ? 
O142 K16 K21 97.3(7) 2_756 1_545 ? 
W3' K16 K21 165.4(9) . 1_545 ? 
W22 K16 K21 98.8(4) . 1_545 ? 
O154 K16 K12 40.8(5) . 2_756 ? 
O35 K16 K12 40.1(4) . 2_756 ? 
O86 K16 K12 86.6(5) . 2_756 ? 
O233 K16 K12 87.6(6) 1_545 2_756 ? 
O142 K16 K12 40.3(5) 2_756 2_756 ? 
W3' K16 K12 55.8(8) . 2_756 ? 
W22 K16 K12 61.1(2) . 2_756 ? 
K21 K16 K12 129.0(6) 1_545 2_756 ? 
O154 K16 K21' 101.4(7) . 1_545 ? 
O35 K16 K21' 161.0(8) . 1_545 ? 
O86 K16 K21' 125.3(7) . 1_545 ? 
O233 K16 K21' 37.9(7) 1_545 1_545 ? 
O142 K16 K21' 95.3(7) 2_756 1_545 ? 
W3' K16 K21' 170.6(9) . 1_545 ? 
W22 K16 K21' 92.3(5) . 1_545 ? 
K21 K16 K21' 6.7(6) 1_545 1_545 ? 
K12 K16 K21' 124.1(6) 2_756 1_545 ? 
O236 K17 O36 74.8(9) 1_565 1_565 ? 
O236 K17 O34 137.4(10) 1_565 2_667 ? 
O36 K17 O34 137.0(8) 1_565 2_667 ? 
O236 K17 O97 98.1(9) 1_565 . ? 
O36 K17 O97 140.1(8) 1_565 . ? 
O34 K17 O97 73.6(7) 2_667 . ? 
O236 K17 O222 139.7(10) 1_565 2_667 ? 
O36 K17 O222 79.2(7) 1_565 2_667 ? 
O34 K17 O222 81.8(8) 2_667 2_667 ? 
O97 K17 O222 82.6(8) . 2_667 ? 
O236 K17 O93 67.4(8) 1_565 . ? 
O36 K17 O93 142.1(6) 1_565 . ? 
O34 K17 O93 75.7(6) 2_667 . ? 
O97 K17 O93 51.7(6) . . ? 
O222 K17 O93 133.0(7) 2_667 . ? 
O236 K17 W16 77.7(8) 1_565 . ? 
O36 K17 W16 142.1(6) 1_565 . ? 
O34 K17 W16 80.4(5) 2_667 . ? 
O97 K17 W16 24.6(5) . . ? 
O222 K17 W16 107.1(6) 2_667 . ? 
O93 K17 W16 29.1(3) . . ? 
O236 K17 W36 78.7(8) 1_565 1_565 ? 
O36 K17 W36 17.8(4) 1_565 1_565 ? 
O34 K17 W36 141.3(6) 2_667 1_565 ? 
O97 K17 W36 122.9(6) . 1_565 ? 
O222 K17 W36 67.8(6) 2_667 1_565 ? 
O93 K17 W36 142.9(5) . 1_565 ? 
W16 K17 W36 130.2(4) . 1_565 ? 
O236 K17 K13 122.4(8) 1_565 2_667 ? 
O36 K17 K13 108.1(5) 1_565 2_667 ? 
O34 K17 K13 79.8(5) 2_667 2_667 ? 
O97 K17 K13 42.6(5) . 2_667 ? 
O222 K17 K13 40.8(6) 2_667 2_667 ? 
O93 K17 K13 94.3(4) . 2_667 ? 
W16 K17 K13 66.6(2) . 2_667 ? 
W36 K17 K13 91.2(3) 1_565 2_667 ? 
O236 K17 K27 102.2(8) 1_565 . ? 
O36 K17 K27 160.1(6) 1_565 . ? 
O34 K17 K27 37.2(5) 2_667 . ? 
O97 K17 K27 59.4(5) . . ? 
O222 K17 K27 112.3(7) 2_667 . ? 
O93 K17 K27 38.9(4) . . ? 
W16 K17 K27 52.3(3) . . ? 
W36 K17 K27 177.5(4) 1_565 . ? 
K13 K17 K27 90.2(3) 2_667 . ? 
O39 K18 O29 97.4(7) . . ? 
O39 K18 O237 74.6(8) . 1_455 ? 
O29 K18 O237 128.7(9) . 1_455 ? 
O39 K18 O15 76.6(6) . 2_657 ? 
O29 K18 O15 64.5(6) . 2_657 ? 
O237 K18 O15 149.7(8) 1_455 2_657 ? 
O39 K18 W21 87.0(5) . . ? 
O29 K18 W21 16.6(4) . . ? 
O237 K18 W21 113.3(7) 1_455 . ? 
O15 K18 W21 74.1(4) 2_657 . ? 
O39 K18 K13 113.4(5) . . ? 
O29 K18 K13 37.0(4) . . ? 
O237 K18 K13 162.0(8) 1_455 . ? 
O15 K18 K13 45.2(4) 2_657 . ? 
W21 K18 K13 53.43(15) . . ? 
O39 K18 K2 38.0(5) . . ? 
O29 K18 K2 62.3(5) . . ? 
O237 K18 K2 87.4(7) 1_455 . ? 
O15 K18 K2 75.6(4) 2_657 . ? 
W21 K18 K2 49.56(13) . . ? 
K13 K18 K2 90.3(2) . . ? 
O68 K19 O152 73.7(7) . . ? 
O68 K19 O42 79.0(7) . . ? 
O152 K19 O42 71.7(6) . . ? 
O68 K19 O126 70.1(6) . . ? 
O152 K19 O126 143.6(7) . . ? 
O42 K19 O126 104.5(6) . . ? 
O68 K19 O71 70.1(6) . . ? 
O152 K19 O71 117.6(7) . . ? 
O42 K19 O71 52.8(5) . . ? 
O126 K19 O71 52.2(5) . . ? 
O68 K19 W17 67.7(5) . . ? 
O152 K19 W17 89.9(5) . . ? 
O42 K19 W17 24.5(3) . . ? 
O126 K19 W17 80.1(4) . . ? 
O71 K19 W17 29.3(4) . . ? 
O68 K19 W20 62.5(5) . . ? 
O152 K19 W20 131.2(6) . . ? 
O42 K19 W20 79.5(4) . . ? 
O126 K19 W20 25.1(4) . . ? 
O71 K19 W20 28.0(4) . . ? 
W17 K19 W20 54.99(16) . . ? 
O68 K19 K10 84.2(5) . . ? 
O152 K19 K10 37.4(5) . . ? 
O42 K19 K10 37.3(4) . . ? 
O126 K19 K10 138.8(5) . . ? 
O71 K19 K10 89.5(5) . . ? 
W17 K19 K10 60.2(2) . . ? 
W20 K19 K10 114.1(3) . . ? 
O68 K19 K9 31.6(5) . . ? 
O152 K19 K9 75.5(6) . . ? 
O42 K19 K9 109.2(5) . . ? 
O126 K19 K9 71.8(5) . . ? 
O71 K19 K9 96.0(5) . . ? 
W17 K19 K9 99.2(2) . . ? 
W20 K19 K9 78.0(2) . . ? 
K10 K19 K9 102.4(3) . . ? 
O92 K20 O99 85.0(7) 2_657 2_657 ? 
O92 K20 O60 78.0(6) 2_657 . ? 
O99 K20 O60 64.9(6) 2_657 . ? 
O92 K20 O224 67.1(9) 2_657 . ? 
O99 K20 O224 140.5(9) 2_657 . ? 
O60 K20 O224 81.8(9) . . ? 
O92 K20 W4' 13.9(9) 2_657 2_657 ? 
O99 K20 W4' 97.1(10) 2_657 2_657 ? 
O60 K20 W4' 89.4(10) . 2_657 ? 
O224 K20 W4' 60.3(11) . 2_657 ? 
O92 K20 W8 83.7(5) 2_657 . ? 
O99 K20 W8 83.5(5) 2_657 . ? 
O60 K20 W8 19.2(4) . . ? 
O224 K20 W8 66.8(7) . . ? 
W4' K20 W8 91.8(9) 2_657 . ? 
K21' K21 O81 91(6) . 2_766 ? 
K21' K21 O192 76(5) . . ? 
O81 K21 O192 81.9(11) 2_766 . ? 
K21' K21 O233 85(5) . . ? 
O81 K21 O233 82.5(12) 2_766 . ? 
O192 K21 O233 155.1(15) . . ? 
K21' K21 O198 69(5) . 1_565 ? 
O81 K21 O198 146.9(13) 2_766 1_565 ? 
O192 K21 O198 116.9(12) . 1_565 ? 
O233 K21 O198 69.6(10) . 1_565 ? 
K21' K21 K16 132(5) . 1_565 ? 
O81 K21 K16 95.6(10) 2_766 1_565 ? 
O192 K21 K16 151.8(9) . 1_565 ? 
O233 K21 K16 49.4(8) . 1_565 ? 
O198 K21 K16 79.9(9) 1_565 1_565 ? 
K21' K21 K9 118(5) . . ? 
O81 K21 K9 58.0(6) 2_766 . ? 
O192 K21 K9 49.2(6) . . ? 
O233 K21 K9 132.9(11) . . ? 
O198 K21 K9 154.8(11) 1_565 . ? 
K16 K21 K9 106.0(6) 1_565 . ? 
K21 K21' O192 89(5) . . ? 
K21 K21' O198 97(6) . 1_565 ? 
O192 K21' O198 125.9(15) . 1_565 ? 
K21 K21' O233 81(5) . . ? 
O192 K21' O233 160.8(16) . . ? 
O198 K21' O233 71.7(12) 1_565 . ? 
K21 K21' O81 74(5) . 2_766 ? 
O192 K21' O81 81.4(12) . 2_766 ? 
O198 K21' O81 151.7(16) 1_565 2_766 ? 
O233 K21' O81 80.2(12) . 2_766 ? 
K21 K21' K16 41(5) . 1_565 ? 
O192 K21' K16 130.3(11) . 1_565 ? 
O198 K21' K16 72.7(10) 1_565 1_565 ? 
O233 K21' K16 41.7(8) . 1_565 ? 
O81 K21' K16 83.9(9) 2_766 1_565 ? 
O124 K22 O197 93.8(8) . . ? 
O124 K22 K25' 76.7(7) . 2_866 ? 
O197 K22 K25' 35.5(6) . 2_866 ? 
O124 K22 K3 38.7(6) . . ? 
O197 K22 K3 58.9(5) . . ? 
K25' K22 K3 58.7(4) 2_866 . ? 
K25' K25 K25' 180.0(13) . 2_866 ? 
K25' K25 O163 118.8(8) . 2_866 ? 
K25' K25 O163 61.2(8) 2_866 2_866 ? 
K25' K25 O163 61.2(8) . . ? 
K25' K25 O163 118.8(8) 2_866 . ? 
O163 K25 O163 179.999(3) 2_866 . ? 
K25' K25 O156 118.2(8) . . ? 
K25' K25 O156 61.8(8) 2_866 . ? 
O163 K25 O156 123.0(6) 2_866 . ? 
O163 K25 O156 57.0(6) . . ? 
K25' K25 O156 61.8(8) . 2_866 ? 
K25' K25 O156 118.2(8) 2_866 2_866 ? 
O163 K25 O156 57.0(6) 2_866 2_866 ? 
O163 K25 O156 123.0(6) . 2_866 ? 
O156 K25 O156 180.0(6) . 2_866 ? 
K25' K25 W25 93.1(7) . 2_866 ? 
K25' K25 W25 86.9(7) 2_866 2_866 ? 
O163 K25 W25 27.3(4) 2_866 2_866 ? 
O163 K25 W25 152.7(4) . 2_866 ? 
O156 K25 W25 147.7(4) . 2_866 ? 
O156 K25 W25 32.3(4) 2_866 2_866 ? 
K25' K25 W25 86.9(7) . . ? 
K25' K25 W25 93.1(7) 2_866 . ? 
O163 K25 W25 152.7(4) 2_866 . ? 
O163 K25 W25 27.3(4) . . ? 
O156 K25 W25 32.3(4) . . ? 
O156 K25 W25 147.7(4) 2_866 . ? 
W25 K25 W25 179.999(1) 2_866 . ? 
K25' K25 K3 71.0(7) . 2_866 ? 
K25' K25 K3 109.0(7) 2_866 2_866 ? 
O163 K25 K3 59.6(5) 2_866 2_866 ? 
O163 K25 K3 120.4(5) . 2_866 ? 
O156 K25 K3 144.1(4) . 2_866 ? 
O156 K25 K3 35.9(4) 2_866 2_866 ? 
W25 K25 K3 50.62(9) 2_866 2_866 ? 
W25 K25 K3 129.38(9) . 2_866 ? 
K25' K25 K3 109.0(7) . . ? 
K25' K25 K3 71.0(7) 2_866 . ? 
O163 K25 K3 120.4(5) 2_866 . ? 
O163 K25 K3 59.6(5) . . ? 
O156 K25 K3 35.9(4) . . ? 
O156 K25 K3 144.1(4) 2_866 . ? 
W25 K25 K3 129.38(9) 2_866 . ? 
W25 K25 K3 50.62(9) . . ? 
K3 K25 K3 180.000(1) 2_866 . ? 
K25 K25' O163 74.2(9) . . ? 
K25 K25' O197 137.8(13) . 2_866 ? 
O163 K25' O197 147.9(13) . 2_866 ? 
K25 K25' O156 77.1(9) . 2_866 ? 
O163 K25' O156 151.3(13) . 2_866 ? 
O197 K25' O156 60.7(8) 2_866 2_866 ? 
K25 K25' W27 109.9(9) . 2_866 ? 
O163 K25' W27 169.1(11) . 2_866 ? 
O197 K25' W27 28.8(6) 2_866 2_866 ? 
O156 K25' W27 34.0(5) 2_866 2_866 ? 
K25 K25' W25 62.9(6) . . ? 
O163 K25' W25 14.4(5) . . ? 
O197 K25' W25 158.5(10) 2_866 . ? 
O156 K25' W25 139.2(9) 2_866 . ? 
W27 K25' W25 172.7(8) 2_866 . ? 
K25 K25' K25' 0.0(7) . 2_866 ? 
O163 K25' K25' 74.2(9) . 2_866 ? 
O197 K25' K25' 137.8(13) 2_866 2_866 ? 
O156 K25' K25' 77.1(9) 2_866 2_866 ? 
W27 K25' K25' 109.9(9) 2_866 2_866 ? 
W25 K25' K25' 62.9(6) . 2_866 ? 
K25 K25' K22 145.6(10) . 2_866 ? 
O163 K25' K22 119.8(10) . 2_866 ? 
O197 K25' K22 37.7(7) 2_866 2_866 ? 
O156 K25' K22 85.3(8) 2_866 2_866 ? 
W27 K25' K22 62.7(5) 2_866 2_866 ? 
W25 K25' K22 123.6(7) . 2_866 ? 
K25' K25' K22 145.6(10) 2_866 2_866 ? 
K25 K25' K3 83.8(7) . 2_866 ? 
O163 K25' K3 137.4(9) . 2_866 ? 
O197 K25' K3 63.8(7) 2_866 2_866 ? 
O156 K25' K3 38.1(6) 2_866 2_866 ? 
W27 K25' K3 53.4(3) 2_866 2_866 ? 
W25 K25' K3 124.2(6) . 2_866 ? 
K25' K25' K3 83.8(7) 2_866 2_866 ? 
K22 K25' K3 64.7(4) 2_866 2_866 ? 
K25 K25' K26 94.7(8) . . ? 
O163 K25' K26 53.6(7) . . ? 
O197 K25' K26 112.7(9) 2_866 . ? 
O156 K25' K26 131.2(9) 2_866 . ? 
W27 K25' K26 134.1(7) 2_866 . ? 
W25 K25' K26 50.5(4) . . ? 
K25' K25' K26 94.7(8) 2_866 . ? 
K22 K25' K26 75.0(5) 2_866 . ? 
K3 K25' K26 93.6(5) 2_866 . ? 
O227 K26 O79 130.9(10) . . ? 
O227 K26 O10 79.6(9) . . ? 
O79 K26 O10 53.3(6) . . ? 
O227 K26 O180 120.0(10) . . ? 
O79 K26 O180 51.1(6) . . ? 
O10 K26 O180 85.4(7) . . ? 
O227 K26 O67 76.8(9) . . ? 
O79 K26 O67 63.4(7) . . ? 
O10 K26 O67 50.5(6) . . ? 
O180 K26 O67 50.4(6) . . ? 
O227 K26 W44 66.5(8) . . ? 
O79 K26 W44 64.7(5) . . ? 
O10 K26 W44 25.9(4) . . ? 
O180 K26 W44 75.1(6) . . ? 
O67 K26 W44 28.5(4) . . ? 
O227 K26 W25 109.9(9) . . ? 
O79 K26 W25 28.3(4) . . ? 
O10 K26 W25 30.9(4) . . ? 
O180 K26 W25 76.0(5) . . ? 
O67 K26 W25 66.0(5) . . ? 
W44 K26 W25 52.3(2) . . ? 
O227 K26 W47 93.7(8) . . ? 
O79 K26 W47 63.6(5) . . ? 
O10 K26 W47 74.6(6) . . ? 
O180 K26 W47 26.7(4) . . ? 
O67 K26 W47 27.7(4) . . ? 
W44 K26 W47 55.9(2) . . ? 
W25 K26 W47 79.5(3) . . ? 
O227 K26 W38 141.6(9) . . ? 
O79 K26 W38 26.6(4) . . ? 
O10 K26 W38 76.2(5) . . ? 
O180 K26 W38 29.3(4) . . ? 
O67 K26 W38 64.8(5) . . ? 
W44 K26 W38 79.0(3) . . ? 
W25 K26 W38 54.9(2) . . ? 
W47 K26 W38 51.3(2) . . ? 
O227 K26 K25' 90.3(9) . . ? 
O79 K26 K25' 77.1(6) . . ? 
O10 K26 K25' 57.8(6) . . ? 
O180 K26 K25' 128.1(7) . . ? 
O67 K26 K25' 108.3(6) . . ? 
W44 K26 K25' 81.5(4) . . ? 
W25 K26 K25' 53.3(4) . . ? 
W47 K26 K25' 130.7(5) . . ? 
W38 K26 K25' 101.3(5) . . ? 
O226 K27 O54 65.8(7) . . ? 
O226 K27 O93 90.3(7) . . ? 
O54 K27 O93 54.0(6) . . ? 
O226 K27 O88 130.0(8) . . ? 
O54 K27 O88 65.0(6) . . ? 
O93 K27 O88 53.1(6) . . ? 
O226 K27 O34 109.3(8) . 2_667 ? 
O54 K27 O34 133.9(8) . 2_667 ? 
O93 K27 O34 81.2(7) . 2_667 ? 
O88 K27 O34 98.4(8) . 2_667 ? 
O226 K27 O65 101.2(7) . . ? 
O54 K27 O65 52.1(6) . . ? 
O93 K27 O65 88.7(7) . . ? 
O88 K27 O65 52.5(6) . . ? 
O34 K27 O65 147.9(9) 2_667 . ? 
O226 K27 O88 134.7(8) . 2_667 ? 
O54 K27 O88 158.8(8) . 2_667 ? 
O93 K27 O88 121.2(7) . 2_667 ? 
O88 K27 O88 95.3(7) . 2_667 ? 
O34 K27 O88 52.9(6) 2_667 2_667 ? 
O65 K27 O88 110.4(7) . 2_667 ? 
O226 K27 K13 81.1(6) . . ? 
O54 K27 K13 86.2(5) . . ? 
O93 K27 K13 138.7(7) . . ? 
O88 K27 K13 103.8(6) . . ? 
O34 K27 K13 139.7(7) 2_667 . ? 
O65 K27 K13 54.3(5) . . ? 
O88 K27 K13 91.5(5) 2_667 . ? 
O226 K27 W16 118.2(7) . . ? 
O54 K27 W16 66.7(5) . . ? 
O93 K27 W16 28.6(4) . . ? 
O88 K27 W16 28.9(4) . . ? 
O34 K27 W16 78.9(6) 2_667 . ? 
O65 K27 W16 77.8(5) . . ? 
O88 K27 W16 100.1(6) 2_667 . ? 
K13 K27 W16 131.6(5) . . ? 
O226 K27 W9 126.5(7) . . ? 
O54 K27 W9 65.4(5) . . ? 
O93 K27 W9 78.2(5) . . ? 
O88 K27 W9 28.8(4) . . ? 
O34 K27 W9 119.9(7) 2_667 . ? 
O65 K27 W9 28.0(4) . . ? 
O88 K27 W9 93.6(5) 2_667 . ? 
K13 K27 W9 75.1(3) . . ? 
W16 K27 W9 57.5(3) . . ? 
O226 K27 W9 120.1(7) . 2_667 ? 
O54 K27 W9 156.0(6) . 2_667 ? 
O93 K27 W9 102.0(6) . 2_667 ? 
O88 K27 W9 101.9(6) . 2_667 ? 
O34 K27 W9 23.7(5) 2_667 2_667 ? 
O65 K27 W9 136.9(6) . 2_667 ? 
O88 K27 W9 29.8(3) 2_667 2_667 ? 
K13 K27 W9 117.3(4) . 2_667 ? 
W16 K27 W9 92.0(4) . 2_667 ? 
W9 K27 W9 113.4(4) . 2_667 ? 
O226 K27 W7 66.2(5) . . ? 
O54 K27 W7 28.3(4) . . ? 
O93 K27 W7 30.1(4) . . ? 
O88 K27 W7 66.5(5) . . ? 
O34 K27 W7 105.9(6) 2_667 . ? 
O65 K27 W7 77.0(5) . . ? 
O88 K27 W7 151.3(6) 2_667 . ? 
K13 K27 W7 113.7(4) . . ? 
W16 K27 W7 53.2(2) . . ? 
W9 K27 W7 80.7(3) . . ? 
W9 K27 W7 129.0(4) 2_667 . ? 
Pd5 O1 Pd9 111.2(8) . . ? 
Pd5 O1 Pd8 110.0(7) . . ? 
Pd9 O1 Pd8 111.6(8) . . ? 
Pd5 O1 K2 104.4(7) . . ? 
Pd9 O1 K2 105.5(6) . . ? 
Pd8 O1 K2 113.9(7) . . ? 
W34 O2 W1 157.5(10) . . ? 
W34 O2 K13 97.7(7) . 2_657 ? 
W1 O2 K13 100.5(6) . 2_657 ? 
W21 O3 Pd6 149.4(11) . . ? 
W21 O3 K2 107.5(7) . . ? 
Pd6 O3 K2 100.1(7) . . ? 
W5 O4 Pd7 141.1(10) . . ? 
W5 O4 K2 85.6(7) . . ? 
Pd7 O4 K2 95.7(7) . . ? 
W43 O5 W6 123.8(9) . . ? 
W39 O6 W5 147.9(9) . . ? 
W4 O7 W5 163.8(9) . . ? 
W4 O7 W4' 10.0(14) . . ? 
W5 O7 W4' 170.3(18) . . ? 
W4 O7 K2 89.9(6) . . ? 
W5 O7 K2 89.7(7) . . ? 
W4' O7 K2 84.5(15) . . ? 
W4 O7 K4 97.1(6) . . ? 
W5 O7 K4 98.1(6) . . ? 
W4' O7 K4 91.2(15) . . ? 
K2 O7 K4 111.4(5) . . ? 
W15 O8 Pd2 154.1(12) . . ? 
W15 O8 K3 90.5(7) . . ? 
Pd2 O8 K3 97.8(7) . . ? 
W3 O9 W24' 153.9(12) . . ? 
W3 O9 W24 141.3(9) . . ? 
W24' O9 W24 12.6(7) . . ? 
W3 O9 W3' 9.5(12) . . ? 
W24' O9 W3' 146.8(17) . . ? 
W24 O9 W3' 134.5(15) . . ? 
W44 O10 W25 127.0(11) . . ? 
W44 O10 K26 108.1(9) . . ? 
W25 O10 K26 101.2(8) . . ? 
W14 O11 W21 127.1(8) . . ? 
W14 O11 K2 97.1(7) . . ? 
W21 O11 K2 98.0(6) . . ? 
W9 O12 W28 153.0(11) . . ? 
Se3 O13 W12 127.1(10) . . ? 
Se3 O13 W10 120.1(8) . . ? 
W12 O13 W10 93.0(6) . . ? 
Se3 O13 W39 124.9(8) . . ? 
W12 O13 W39 91.1(5) . . ? 
W10 O13 W39 90.7(6) . . ? 
W39 O14 W10 126.2(10) . . ? 
W1 O15 K18 139.9(10) . 2_657 ? 
W1 O15 K13 105.6(8) . 2_657 ? 
K18 O15 K13 93.7(6) 2_657 2_657 ? 
W36 O16 W34 174.1(12) . . ? 
W11 O17 W33 154.8(12) . . ? 
Pd7 O18 Pd6 116.5(9) . . ? 
Pd7 O18 Pd9 105.1(8) . . ? 
Pd6 O18 Pd9 109.4(8) . . ? 
Pd7 O18 K2 114.7(7) . . ? 
Pd6 O18 K2 104.4(7) . . ? 
Pd9 O18 K2 106.3(7) . . ? 
W32 O19 W41 158.0(13) . . ? 
W36 O20 W12 146.1(11) . . ? 
W14 O21 Pd5 152.0(11) . . ? 
W14 O21 K2 106.5(8) . . ? 
Pd5 O21 K2 99.3(7) . . ? 
Se10 O22 Pd7 119.3(9) . . ? 
Se10 O22 K8 104.0(8) . . ? 
Pd7 O22 K8 127.6(8) . . ? 
W26 O23 W6 124.4(11) . . ? 
W26 O23 K6 133.0(9) . 2_757 ? 
W6 O23 K6 98.8(7) . 2_757 ? 
W28 O24 W17 127.2(10) . . ? 
W40 O25 W22 122.7(10) . . ? 
Pd4 O26 Pd2 112.6(9) . . ? 
Pd4 O26 Pd10 111.2(10) . . ? 
Pd2 O26 Pd10 109.3(9) . . ? 
Pd4 O26 K3 107.2(8) . . ? 
Pd2 O26 K3 111.0(9) . . ? 
Pd10 O26 K3 105.3(7) . . ? 
W1 O27 W4 120.2(9) . . ? 
W1 O27 W4' 129.8(16) . . ? 
W4 O27 W4' 11.4(12) . . ? 
W1 O27 K4 119.6(8) . . ? 
W4 O27 K4 99.8(7) . . ? 
W4' O27 K4 97.2(17) . . ? 
Se1 O28 W2' 110.4(17) . . ? 
Se1 O28 W2 118.2(9) . . ? 
W2' O28 W2 8.3(15) . . ? 
Se1 O28 W34 135.7(9) . . ? 
W2' O28 W34 99.9(17) . . ? 
W2 O28 W34 94.7(7) . . ? 
W21 O29 K18 136.1(10) . . ? 
W21 O29 K13 116.1(9) . . ? 
K18 O29 K13 107.3(7) . . ? 
W34 O30 W43 146.7(10) . . ? 
Se1 O31 W4 119.0(9) . . ? 
Se1 O31 W1 135.0(11) . . ? 
W4 O31 W1 95.4(7) . . ? 
W36 O32 W8 155.1(10) . . ? 
W16 O33 W20 127.1(12) . . ? 
W9 O34 K17 135.2(10) . 2_667 ? 
W9 O34 K27 111.8(10) . 2_667 ? 
K17 O34 K27 108.0(8) 2_667 2_667 ? 
W3' O35 W3 7(2) . . ? 
W3' O35 K12 132(2) . 2_756 ? 
W3 O35 K12 126.7(9) . 2_756 ? 
W3' O35 K16 129(2) . . ? 
W3 O35 K16 132.8(9) . . ? 
K12 O35 K16 98.1(6) 2_756 . ? 
W36 O36 K17 132.5(10) . 1_545 ? 
W17 O37 W35 125.6(9) . . ? 
W17 O37 K14 117.6(8) . . ? 
W35 O37 K14 89.1(7) . . ? 
W5 O39 K18 147.8(11) . . ? 
W5 O39 K2 88.9(8) . . ? 
K18 O39 K2 109.2(7) . . ? 
W35 O40 W14 145.9(10) . . ? 
W19 O41 W42 140.0(10) . . ? 
W17 O42 K10 141.5(12) . . ? 
W17 O42 K19 107.4(9) . . ? 
K10 O42 K19 101.7(6) . . ? 
Se3 O43 W5 117.3(11) . . ? 
Se3 O43 W8 135.1(10) . . ? 
W5 O43 W8 96.3(7) . . ? 
W31 O44 W42 146.5(11) . . ? 
W35 O45 Pd5 153.5(11) . . ? 
W35 O45 K14 99.6(8) . . ? 
Pd5 O45 K14 105.2(7) . . ? 
W36 O46 W3' 133.9(15) . . ? 
W36 O46 W3 121.7(9) . . ? 
W3' O46 W3 12.1(12) . . ? 
W26 O47 W43 123.9(9) . . ? 
W39 O48 W12 126.3(8) . . ? 
W18 O49 W11 124.3(11) . . ? 
W18 O49 K7 122.6(9) . . ? 
W11 O49 K7 95.8(7) . . ? 
Se9 O50 Pd1 117.5(11) . . ? 
W11 O51 K7 105.5(9) . 2_766 ? 
W11 O51 K7 93.7(9) . . ? 
K7 O51 K7 116.2(7) 2_766 . ? 
Se7 O52 Pd8 121.3(11) . . ? 
Se7 O52 K6 126.2(10) . . ? 
Pd8 O52 K6 112.2(9) . . ? 
W4 O53 W4' 11.7(14) . . ? 
W4 O53 Pd8 152.7(13) . . ? 
W4' O53 Pd8 142.1(19) . . ? 
W4 O53 K2 85.8(7) . . ? 
W4' O53 K2 81.9(18) . . ? 
Pd8 O53 K2 97.7(7) . . ? 
W21 O54 W7 145.4(11) . . ? 
W21 O54 K27 107.6(8) . . ? 
W7 O54 K27 106.5(8) . . ? 
W7 O55 Pd6 151.5(12) . . ? 
W7 O55 K11 103.5(7) . . ? 
Pd6 O55 K11 105.0(7) . . ? 
W29 O56 W13 127.9(11) . . ? 
W10 O57 Pd7 178.1(11) . . ? 
W30 O58 W37 149.9(11) . . ? 
W32 O59 W37 124.6(11) . . ? 
W8 O60 K20 128.1(10) . . ? 
W44 O61 W27 128.4(10) . . ? 
W44 O61 K15 106.0(8) . . ? 
W27 O61 K15 101.5(8) . . ? 
W3 O62 W3' 13.0(13) . . ? 
W3 O62 W2 169.9(12) . . ? 
W3' O62 W2 173.3(17) . . ? 
W3 O62 W2' 159.0(18) . . ? 
W3' O62 W2' 171(2) . . ? 
W2 O62 W2' 11.8(13) . . ? 
W8 O63 W5 119.6(9) . . ? 
W8 O63 K4 118.3(8) . . ? 
W5 O63 K4 102.9(7) . . ? 
Se7 O64 Pd5 118.2(11) . . ? 
Se7 O64 K14 109.9(9) . . ? 
Pd5 O64 K14 102.5(8) . . ? 
W9 O65 W21 127.2(10) . . ? 
W9 O65 K27 104.8(7) . . ? 
W21 O65 K27 103.6(8) . . ? 
W9 O65 K13 134.3(8) . . ? 
W21 O65 K13 95.2(6) . . ? 
K27 O65 K13 76.5(6) . . ? 
W1 O66 W26 144.9(11) . . ? 
W47 O67 W44 151.9(11) . . ? 
W47 O67 K26 104.1(9) . . ? 
W44 O67 K26 101.7(8) . . ? 
W31 O68 K19 142.7(13) . . ? 
W31 O68 K9 94.6(10) . . ? 
K19 O68 K9 120.0(8) . . ? 
Se3 O69 W3 118.9(8) . . ? 
Se3 O69 W36 135.1(10) . . ? 
W3 O69 W36 94.4(6) . . ? 
W2' O70 W2 14.6(17) . . ? 
W2' O70 W46 157(2) . . ? 
W2 O70 W46 163.3(11) . . ? 
W20 O71 W17 145.6(12) . . ? 
W20 O71 K19 97.7(8) . . ? 
W17 O71 K19 95.5(7) . . ? 
W34 O72 W2 122.3(10) . . ? 
W34 O72 W2' 110.2(16) . . ? 
W2 O72 W2' 12.4(13) . . ? 
W15 O73 W23 163.5(12) . . ? 
W15 O73 K3 87.3(8) . . ? 
W23 O73 K3 89.5(9) . . ? 
W40 O74 W32 171.2(13) . . ? 
W40 O74 K12 94.9(8) . . ? 
W32 O74 K12 92.5(7) . . ? 
Se6 O75 W49 120.3(11) . . ? 
Se6 O75 W13 118.3(9) . . ? 
W49 O75 W13 92.6(7) . . ? 
Se6 O75 W29 134.9(11) . . ? 
W49 O75 W29 91.6(6) . . ? 
W13 O75 W29 88.2(6) . . ? 
Se10 O76 Pd9 119.2(10) . . ? 
Se10 O76 K1 139.4(10) . . ? 
Pd9 O76 K1 101.2(7) . . ? 
W28 O77 K10 122.1(11) . 2_767 ? 
W40 O78 K12 112.7(11) . . ? 
W38 O79 W25 144.4(10) . . ? 
W38 O79 K26 109.5(7) . . ? 
W25 O79 K26 105.8(8) . . ? 
W38 O80 Pd4 151.0(12) . . ? 
W38 O80 K9 102.4(8) . . ? 
Pd4 O80 K9 103.1(8) . . ? 
W30 O81 K21 145.9(12) . 2_766 ? 
W30 O81 K21' 140.3(12) . 2_766 ? 
K21 O81 K21' 14.4(8) 2_766 2_766 ? 
Se7 O82 Pd9 120.5(10) . . ? 
Se7 O82 K1 138.5(9) . . ? 
Pd9 O82 K1 100.9(7) . . ? 
Se10 O83 Pd6 122.1(9) . . ? 
Se10 O83 K11 116.9(9) . . ? 
Pd6 O83 K11 110.6(8) . . ? 
W42 O84 K5 112.8(9) . . ? 
W42 O84 K14 99.7(10) . . ? 
K5 O84 K14 107.8(7) . . ? 
W2 O85 W2' 6.6(15) . . ? 
W51 O86 W51' 5.8(4) . . ? 
W51 O86 K16 146.6(10) . . ? 
W51' O86 K16 149.4(9) . . ? 
W16 O88 W9 151.5(12) . . ? 
W16 O88 K27 102.3(8) . . ? 
W9 O88 K27 104.7(9) . . ? 
W16 O88 K27 102.2(8) . 2_667 ? 
W9 O88 K27 89.2(7) . 2_667 ? 
K27 O88 K27 84.7(7) . 2_667 ? 
W8 O89 W1 174.1(12) . . ? 
W2' O90 W43 137.8(19) . . ? 
W2' O90 W2 13.4(16) . . ? 
W43 O90 W2 147.7(10) . . ? 
Pd1 O91 Pd3 117.3(10) . . ? 
Pd1 O91 Pd10 105.8(8) . . ? 
Pd3 O91 Pd10 107.3(9) . . ? 
Pd1 O91 K3 116.6(9) . . ? 
Pd3 O91 K3 103.5(7) . . ? 
Pd10 O91 K3 105.5(8) . . ? 
W4' O92 W4 6(2) . . ? 
W4' O92 K20 137(3) . 2_657 ? 
W4 O92 K20 143.1(10) . 2_657 ? 
W4' O92 K2 95(2) . . ? 
W4 O92 K2 89.7(8) . . ? 
K20 O92 K2 121.7(8) 2_657 . ? 
W16 O93 W7 125.7(9) . . ? 
W16 O93 K27 102.8(8) . . ? 
W7 O93 K27 103.4(8) . . ? 
W16 O93 K17 88.4(7) . . ? 
W7 O93 K17 135.4(7) . . ? 
K27 O93 K17 94.2(6) . . ? 
W10 O94 K8 120.8(10) . . ? 
W22 O95 W37 171.1(13) . . ? 
W48 O96 W40 157.8(12) . . ? 
W16 O97 K13 150.3(11) . 2_667 ? 
W16 O97 K17 111.4(11) . . ? 
K13 O97 K17 94.0(7) 2_667 . ? 
W20 O98 W31 139.1(9) . . ? 
W20 O98 K11 107.4(8) . . ? 
W31 O98 K11 98.8(7) . . ? 
W14 O99 K20 152.7(11) . 2_657 ? 
Se5 O100 W22 118.8(12) . . ? 
Se5 O100 W40 134.9(12) . . ? 
W22 O100 W40 93.7(10) . . ? 
W27 O102 W49 146.9(11) . . ? 
W27 O102 K15 106.5(8) . . ? 
W49 O102 K15 105.8(9) . . ? 
W27 O103 Pd3 149.6(12) . . ? 
W27 O103 K3 107.5(9) . . ? 
Pd3 O103 K3 100.8(7) . . ? 
W34 O104 K13 109.1(9) . 2_657 ? 
W13 O105 W19 145.4(13) . . ? 
W13 O105 K10 97.7(8) . . ? 
W19 O105 K10 94.5(7) . . ? 
W45 O106 W50 127.0(10) . . ? 
W30 O107 W18 124.1(10) . . ? 
W51' O108 W51 15.5(4) . . ? 
W51' O108 W46 178.0(15) . . ? 
W51 O108 W46 164.6(12) . . ? 
W6 O109 K6 108.7(9) . . ? 
W6 O109 K6 104.2(8) . 2_757 ? 
K6 O109 K6 99.0(7) . 2_757 ? 
W29 O110 W44 148.4(12) . . ? 
W29 O110 K15 105.2(8) . . ? 
W44 O110 K15 104.3(8) . . ? 
Se8 O111 Pd10 119.3(10) . . ? 
Se8 O111 K1 139.7(10) . . ? 
Pd10 O111 K1 100.8(8) . . ? 
W29 O112 W49 124.2(10) . . ? 
W29 O112 K15 103.4(9) . . ? 
W49 O112 K15 102.1(9) . . ? 
W49 O114 Pd3 149.2(15) . . ? 
W49 O114 K5 106.2(11) . . ? 
Pd3 O114 K5 104.6(8) . . ? 
W33 O115 K1 106.0(9) . . ? 
W32 O116 W30 146.6(12) . . ? 
W6 O117 Pd8 167.8(13) . . ? 
W6 O117 K6 92.5(7) . . ? 
Pd8 O117 K6 94.8(7) . . ? 
W19 O118 W38 126.0(10) . . ? 
W19 O118 K9 118.9(7) . . ? 
W38 O118 K9 85.9(6) . . ? 
W20 O119 W7 124.4(10) . . ? 
W20 O119 K11 100.4(8) . . ? 
W7 O119 K11 98.7(8) . . ? 
W25 O120 Pd4 152.6(12) . . ? 
W25 O120 K3 105.5(8) . . ? 
Pd4 O120 K3 100.6(8) . . ? 
W42 O121 K10 142.5(10) . . ? 
W42 O121 K14 95.8(10) . . ? 
K10 O121 K14 117.5(8) . . ? 
W46 O122 W6 150.0(12) . . ? 
W23 O123 Pd1 142.6(13) . . ? 
W23 O123 K3 88.7(8) . . ? 
Pd1 O123 K3 95.0(8) . . ? 
W23 O124 K22 146.1(12) . . ? 
W23 O124 K3 90.1(10) . . ? 
K22 O124 K3 108.2(9) . . ? 
Se8 O125 Pd2 121.3(10) . . ? 
Se8 O125 K7 132.4(10) . 2_766 ? 
Pd2 O125 K7 104.7(9) . 2_766 ? 
W20 O126 K19 104.6(9) . . ? 
W17 O127 W31 142.0(11) . . ? 
Se9 O128 Pd3 119.6(11) . . ? 
Se9 O128 K5 113.6(10) . . ? 
Pd3 O128 K5 112.3(8) . . ? 
W9 O130 W14 127.0(10) . . ? 
W15 O132 K3 87.8(8) . . ? 
Se6 O135 W38 119.3(10) . . ? 
Se6 O135 W19 119.6(9) . . ? 
W38 O135 W19 92.1(7) . . ? 
Se6 O135 W47 133.3(10) . . ? 
W38 O135 W47 91.5(6) . . ? 
W19 O135 W47 90.7(7) . . ? 
Se2 O137 W11 118.8(9) . . ? 
Se2 O137 W18 125.9(11) . . ? 
W11 O137 W18 92.4(7) . . ? 
Se2 O137 W30 126.5(10) . . ? 
W11 O137 W30 93.3(7) . . ? 
W18 O137 W30 90.6(6) . . ? 
W47 O138 W19 127.0(11) . . ? 
Se2 O141 W37 118.3(10) . . ? 
Se2 O141 W32 134.3(10) . . ? 
W37 O141 W32 94.6(8) . . ? 
W32 O142 K12 114.1(12) . . ? 
W32 O142 K16 140.3(12) . 2_756 ? 
K12 O142 K16 90.0(7) . 2_756 ? 
W26 O143 W4' 156.0(18) . . ? 
W26 O143 W4 147.3(11) . . ? 
W4' O143 W4 11.8(13) . . ? 
W37 O144 W33 162.4(13) . . ? 
W13 O146 W42 136.1(12) . . ? 
W13 O146 K5 107.2(8) . . ? 
W42 O146 K5 99.2(7) . . ? 
W51' O147 W51 6.7(4) . . ? 
W51' O147 K1 104.4(9) . . ? 
W51 O147 K1 104.3(7) . . ? 
Se1 O148 W6 119.9(10) . . ? 
Se1 O148 W26 127.2(10) . . ? 
W6 O148 W26 90.8(7) . . ? 
Se1 O148 W43 126.6(11) . . ? 
W6 O148 W43 91.9(7) . . ? 
W26 O148 W43 90.1(6) . . ? 
Se9 O149 Pd10 119.5(11) . . ? 
Se9 O149 K1 135.4(11) . . ? 
Pd10 O149 K1 104.6(8) . . ? 
W13 O150 K10 102.4(10) . . ? 
W39 O151 W8 146.7(12) . . ? 
W19 O152 K19 138.2(11) . . ? 
W19 O152 K10 107.5(11) . . ? 
K19 O152 K10 107.7(8) . . ? 
W24' O153 W24 12.9(7) . . ? 
W24' O153 W51 161.2(18) . . ? 
W24 O153 W51 152.6(15) . . ? 
W24' O153 W51' 174.4(18) . . ? 
W24 O153 W51' 166.4(15) . . ? 
W51 O153 W51' 14.5(4) . . ? 
W24' O153 K1 94.5(13) . . ? 
W24 O153 K1 105.6(10) . . ? 
W51 O153 K1 101.7(9) . . ? 
W51' O153 K1 87.9(8) . . ? 
W22 O154 K16 125.4(13) . . ? 
W22 O154 K12 132.0(12) . 2_756 ? 
K16 O154 K12 100.3(7) . 2_756 ? 
W27 O156 W25 126.1(12) . . ? 
W27 O156 K25' 92.4(9) . 2_866 ? 
W25 O156 K25' 130.1(11) . 2_866 ? 
W27 O156 K3 98.3(8) . . ? 
W25 O156 K3 98.7(8) . . ? 
K25' O156 K3 106.4(9) 2_866 . ? 
W27 O156 K25 131.6(9) . . ? 
W25 O156 K25 90.8(7) . . ? 
K25' O156 K25 41.1(6) 2_866 . ? 
K3 O156 K25 106.5(7) . . ? 
W28 O157 W35 125.3(9) . . ? 
W12 O158 W3 145.0(12) . . ? 
W12 O158 W3' 151.6(17) . . ? 
W3 O158 W3' 11.0(11) . . ? 
W22 O159 W51 140.1(11) . . ? 
W22 O159 W51' 152.1(12) . . ? 
W51 O159 W51' 13.9(3) . . ? 
W52 O160 W45 125.4(10) . . ? 
W30 O161 W11 122.2(9) . . ? 
W30 O161 K7 118.2(8) . . ? 
W11 O161 K7 86.8(6) . . ? 
W33 O162 K8 112.8(10) . . ? 
W25 O163 K25' 143.9(12) . . ? 
W25 O163 K25 104.0(9) . . ? 
K25' O163 K25 44.6(7) . . ? 
W52 O164 W22 146.1(12) . . ? 
Se2 O165 W15 119.6(11) . . ? 
Se2 O165 W41 131.7(12) . . ? 
W15 O165 W41 95.0(8) . . ? 
Se4 O166 W21 122.2(9) . . ? 
Se4 O166 W14 121.3(8) . . ? 
W21 O166 W14 90.5(6) . . ? 
W18 O167 W41 144.4(13) . . ? 
W24' O168 W24 13.2(7) . . ? 
W24' O168 W33 167.3(15) . . ? 
W24 O168 W33 158.8(13) . . ? 
Se6 O169 W27 124.3(11) . . ? 
Se6 O169 W25 121.4(9) . . ? 
W27 O169 W25 92.5(7) . . ? 
W12 O171 W10 123.2(11) . . ? 
W28 O172 W16 150.6(11) . . ? 
W18 O173 W15 145.6(13) . . ? 
W31 O175 K9 103.7(9) . . ? 
W31 O175 K11 111.0(9) . . ? 
K9 O175 K11 105.7(7) . . ? 
W40 O176 W52 145.8(12) . . ? 
Se8 O177 Pd4 119.0(12) . . ? 
Se8 O177 K9 108.8(9) . . ? 
Pd4 O177 K9 103.1(8) . . ? 
Se4 O178 W7 119.7(10) . . ? 
Se4 O178 W20 120.3(11) . . ? 
W7 O178 W20 91.0(7) . . ? 
Se4 O178 W16 136.2(9) . . ? 
W7 O178 W16 89.9(8) . . ? 
W20 O178 W16 87.8(7) . . ? 
Se4 O179 W35 120.3(11) . . ? 
Se4 O179 W17 119.9(9) . . ? 
W35 O179 W17 92.1(6) . . ? 
Se4 O179 W28 132.9(10) . . ? 
W35 O179 W28 91.1(6) . . ? 
W17 O179 W28 90.1(7) . . ? 
W47 O180 W38 126.2(10) . . ? 
W47 O180 K26 106.3(9) . . ? 
W38 O180 K26 102.7(9) . . ? 
W13 O181 W49 124.9(10) . . ? 
W13 O181 K5 99.7(8) . . ? 
W49 O181 K5 101.2(8) . . ? 
W48 O182 W41 173.1(13) . . ? 
W24' O184 W24 2.2(9) . . ? 
W24' O184 K1 106.2(12) . . ? 
W24 O184 K1 107.9(8) . . ? 
W50 O185 W52 126.0(9) . . ? 
W29 O186 W47 151.7(14) . . ? 
W23 O188 W50 147.9(14) . . ? 
W33 O189 K8 100.9(8) . . ? 
W24 O190 W24' 2.6(9) . . ? 
W24 O190 K12 150.8(13) . 2_756 ? 
W24' O190 K12 151.0(14) . 2_756 ? 
W41 O191 W15 123.9(9) . . ? 
W38 O192 K21' 151.6(15) . . ? 
W38 O192 K21 144.5(14) . . ? 
K21' O192 K21 14.7(8) . . ? 
Se5 O193 W50 126.8(10) . . ? 
Se5 O193 W45 120.7(10) . . ? 
W50 O193 W45 89.9(8) . . ? 
Se5 O193 W52 126.4(12) . . ? 
W50 O193 W52 90.8(7) . . ? 
W45 O193 W52 91.8(7) . . ? 
W50 O194 W48 150.1(15) . . ? 
W24 O196 W10 170.1(12) . . ? 
W24 O196 W24' 12.6(7) . . ? 
W10 O196 W24' 157.9(13) . . ? 
W27 O197 K25' 100.3(11) . 2_866 ? 
W27 O197 K22 134.4(12) . . ? 
K25' O197 K22 106.8(11) 2_866 . ? 
W52 O198 K21' 151.6(15) . 1_545 ? 
W52 O198 K21 145.6(14) . 1_545 ? 
K21' O198 K21 13.7(9) 1_545 1_545 ? 
W11 O199 Pd2 169.1(12) . . ? 
W11 O199 K7 94.3(8) . 2_766 ? 
Pd2 O199 K7 90.3(7) . 2_766 ? 
W46 O200 K1 104.5(12) . . ? 
Se5 O201 W23 116.8(9) . . ? 
Se5 O201 W48 134.9(11) . . ? 
W23 O201 W48 96.0(6) . . ? 
W45 O202 Pd1 174.6(16) . . ? 
W51' O205 W51 15.5(4) . . ? 
W51' O205 W45 156.5(17) . . ? 
W51 O205 W45 171.6(16) . . ? 
W48 O206 W23 123.1(11) . . ? 
K6 O211 K5 144.7(13) . . ? 
K2 O212 K4 123.2(7) . . ? 
K14 O214 K5 104.9(8) . . ? 
K8 O215 K11 151.1(13) . . ? 
K11 O216 K9 93.9(8) . . ? 
K11 O216 K7 164.2(11) . 2_766 ? 
K9 O216 K7 95.9(8) . 2_766 ? 
K7 O220 K9 114.1(8) . 2_766 ? 
K13 O222 K17 95.4(9) . 2_667 ? 
K6 O230 K14 113.4(13) . . ? 
K21 O233 K21' 14.5(7) . . ? 
K21 O233 K16 86.4(10) . 1_565 ? 
K21' O233 K16 100.4(12) . 1_565 ? 
 
_diffrn_measured_fraction_theta_max    0.998 
_diffrn_reflns_theta_full              26.00 
_diffrn_measured_fraction_theta_full   0.998 
_refine_diff_density_max    4.57  
_refine_diff_density_min   -1.96  
_refine_diff_density_rms    0.65 
3
